advertisement

1. Visualization of the Silicon Crystal 2. Conductivity 3. Temperature Dependence of Semiconductor Conductivity 4. Electron and Hole Concentrations 5. The Concept of Mobility , FIELD DEPENDENCE 6. complete ionization 7. Effective masses and Fermi distribution Function 8. Energy: Density of States 9. Compounds 10. Transparent Semiconductors 11. THE DRIFT CURRENT , THE DIFFUSION CURRENT 12. continuity equation 13. p-n junction theory 14. ideal and Nonideal p-n Junction 15. The transition capacitance , The diffusion capacitance 16. photoelectric effect 17. Schottky Diode 18. solar cell Part (1) Solved PROBLEMS Visualization of the Silicon Crystal Example (1): Write the electronic configuration of silicon has 14 electrons in its atom, determine in which sub shell and in which orbit and how many electrons in the highest sub shell energy. Solution: The electronic configuration of silicon as follows, 1S2 2S2 2p6 3S2 3p2 The highest sub shell energy lies in (M) orbit, in the sub shell (p) which is not fully occupied , it has only 2 electrons Example (2): Write the electronic configuration of iodine (I) has 53 electrons in its atom, determine in which sub shell and in which orbit and how many electrons in the highest sub shell energy. Solution: The electronic configuration of iodine (I) as follows, 1S2 2S2 2p6 3S2 3p6 3D10 4S2 4p6 4D10 4F7 The highest sub shell energy lies in (N) orbit, in the sub shell (F) is not fully occupied, it has only seven electrons Example (3): Write the electronic configuration of Tantalum 73 has 73 electrons in its atom, determine in which sub shell and in which orbit and how many electrons in the highest sub shell energy. Solution: The electronic configuration of iodine (I) as follows, 1S2 2S2 2p6 3S2 3p6 3D10 4S2 4p6 4D10 4F14 5S2 5p6 5D5 The highest sub shell energy lies in (O) orbit, in the sub shell (D) which is not fully occupied, it has only 5 electrons Example (4) : Write the electron configuration of silicon in its following energy states + +2 +3 14Si . 14Si , 14Si . Solution: From tables, the atomic number for silicon is 14, which means, it has 14 electrons in its steady state distributed among orbits and sub shells. Therefore, the electron configuration in the following energy states + +2 +3 14Si . 14Si , 14Si can be represented as, ๏ท + 14Si has ๏ท +2 14Si has 14-2=12 electrons 1s22s22p63s2 ๏ท +3 14Si has 14-3=11 electrons 1s22s22p63s1 14-1=13 electrons 1s22s22p63s23p1 Problem 1 The expression for the Bohr radius can also be applied to the hydrogen-like atom consisting of an ionized donor and the electron provided by the donor. Modify the expression for the Bohr radius so that it applies to this hydrogen-like atom. Calculate the resulting radius of an electron orbiting around the ionized donor in silicon. (๐๐ = 11.9 and µe* = 0.26 µ0) Solution The Bohr radius is obtained from: ๐๐ ๐๐ ๐๐ ๐๐ = ๐ ๐๐ ๐๐ However, since the electron travel through silicon one has to replace the permittivity of vacuum with the dielectric constant of silicon and the free electron mass with the effective mass for conductivity calculations so that: ๐๐ ๐๐. ๐ ๐๐ , ๐ ๐๐๐๐ ๐๐ ๐๐๐๐๐๐๐ = ๐๐ ∗ = ๐๐๐ ๐ ๐๐ = ๐. ๐๐ ๐๐ ๐๐ ๐๐ ๐. ๐๐ Problem 2 Electron mobility in Si is 1400 cm2 V−1s−1. Calculate the mean free time in scattering, (Relaxationszeit) of electrons. Effective mass is m*e/m0 = 0.33. Solution: (1.3) From μ = eτ/m* we get that τ = 2.6 × 10−13 s. Problem 3 Calculate thermal velocity of electrons and holes in GaAs at room temperature. Effective masses are m*e/m0 = 0.063 and m*h/m0 = 0.53. Solution: ๐ ∞ ∫๐ ๐ ๐๐๐ (– ๐∗ ๐ ⁄๐ ๐ฒ๐ป) ๐ ๐ ๐ ๐ ๐ฒ๐ป √ ๐๐ = ∞ = ๐ ๐ ๐∗ ∫๐ ๐๐๐ (– ๐∗ ๐ ⁄๐ ๐ฒ๐ป) ๐ ๐ ๐ Thermal velocities of electrons and holes are 4.3 × 107 and 1.5 × 107 cm/s, respectively. Problem 4 Calculate dielectric relaxation time in p-type Ge at room temperature. Assume that all acceptors are ionized. Na = 1015 cm−3, ε = 16, μp = 1900 cm2 V−1s−1. Solution: (1.6) τr = ε/4 πe Na μp = 4.7 × 10−12 s. Problem 5 Calculate dielectric relaxation time in intrinsic Si at 300 K. ε = 12, μn = 1400 cm2 V−1s−1, μn = 3.1 μp. Solution: In this case, ๐๐ = ๐ ๐ ๐ ๐ ๐๐ (๐๐ + ๐๐ ) = ๐. ๐ ๐ ๐๐−๐ ๐ Problem 6 Calculate the ambipolar diffusion coefficient of intrinsic (undoped) Ge at 300 K. μn/μp = 2.1, μn = 3900 cm2 V−1s−1. Solution: D = 65 cm2/s. Problem 7 Holes are injected into n-type Ge so that at the sample surface Δp0 = 1014 cm−3. Calculate Δp at the distance of 4 mm from the surface if τp = 10−3 s and Dp = 49 cm2/s. Solution: โ ๐ = โ๐๐ ๐ ๐๐๐ (− ๐ณ √๐ซ ๐ ๐๐ ) = ๐. ๐ ๐ ๐๐๐๐ ๐๐−๐ Problem 8 What is the width of an infinite quantum well if the second lowest energy of a free electron confined to the well equals 100 meV? Solution The second lowest energy is calculated from ๐๐ ๐ ๐ ๐ฌ๐ = ( ) = ๐. ๐ ๐๐๐−๐๐ ๐ฑ ∗ ๐ ๐ ๐ ๐ฐ๐ One can therefore solve for the width, Lx, of the well, yielding: ๐ ๐. ๐๐๐ ๐ ๐๐−๐๐ ๐ฐ๐ = = = ๐. ๐๐ ๐๐ ∗ −๐๐ −๐๐ √๐ ๐๐. ๐๐ ๐ ๐๐ ๐๐. ๐ ๐๐๐ √๐ ๐ ๐ฌ๐ Problem 9 Calculate the lowest three possible energies of an electron in a hydrogen atom in units of electron volt. Identify all possible electron energies between the lowest energy and -2 eV. Solution The three lowest electron energies in a hydrogen atom can be calculated from ๐๐. ๐ ๐๐ฝ ๐ฌ๐ = − ๐๐๐๐ ๐ = ๐ . ๐ , ๐๐๐ ๐ ๐๐ resulting in: E1 = –13.6 eV, E2 = -3.4 eV and E3 = -1.51 eV The second lowest energy, E2, is the only one between the lowest energy, E1, and –2 eV. Problem 9 Calculate the maximum fraction of the volume in a simple cubic crystal occupied by the atoms. Assume that the atoms are closely packed and that they can be treated as hard spheres. This fraction is also called the packing density. Solution: The atoms in a simple cubic crystal are located at the corners of the units cell, a cube with side a. Adjacent atoms touch each other so that the radius of each atom equals a/2. There are eight atoms occupying the corners of the cube, but only one eighth of each is within the unit cell so that the number of atoms equals one per unit cell. The packing density is then obtained from: ๐ ๐ ๐ ๐ ๐ ๐ฉ( ) ๐ฉ๐ซ ๐ฏ๐จ๐ฅ๐ฎ๐ฆ๐ ๐จ๐ ๐๐ญ๐จ๐ฆ๐ฌ ๐ ๐ ๐ ๐ = = = = ๐๐% ๐ฏ๐จ๐ฅ๐ฎ๐ฆ๐ ๐จ๐ ๐ฎ๐ง๐ข๐ญ ๐๐๐ฅ๐ฅ ๐๐ ๐๐ ๐ or about half the volume of the unit cell is occupied by the atoms. The packing density of four cubic crystals is listed in the table below. Radius Simple cubic Body centered cubic Face centered cubic Diamond ๐⁄ ๐ √๐ ๐⁄ ๐ √๐ ๐⁄ ๐ √๐ ๐⁄ ๐ Atoms/ unit cell 1 2 4 8 Packing density ๐ ⁄๐ = ๐๐% ๐√๐⁄ ๐ = ๐๐% ๐√๐⁄ ๐ = ๐๐% ๐√๐⁄ ๐๐ = ๐๐% Problem 10 Calculate the packing density of the body centered cubic, the face centered cubic and the diamond lattice, listed in example 2.1 p 28. Solution The packing density is calculated as obtained from: ๐ ๐ฉ ๐ซ๐ ๐ฏ๐จ๐ฅ๐ฎ๐ฆ๐ ๐จ๐ ๐๐ญ๐จ๐ฆ๐ฌ = ๐ ๐ ๐ฏ๐จ๐ฅ๐ฎ๐ฆ๐ ๐จ๐ ๐ฎ๐ง๐ข๐ญ ๐๐๐ฅ๐ฅ ๐ The correct radius and number of atoms per unit cell should be used. A body centered cubic lattice contains an additional atom in the middle and therefore contains two atoms per unit cell. The atoms touch along the body diagonal, which equals √๐ a. The radius is one quarter of the body diagonal. A face centered cubic lattice contains six additional atoms in the center of all six faces of the cube. Since only half of the atoms is within the cube the total number of atoms per unit cell equals four. The atoms touch along the diagonal of the faces of the cube, which equals √๐a . The radius is one quarter of the diagonal. The diamond lattice contains two face centered cubic lattice so that the total number of atoms per unit cell equals twice that of the face centered lattice, namely eight. The atoms touch along the body diagonal, where two atoms are one quarter of the body diagonal apart or √๐ a/4 . The radius equals half the distance between the two atoms. The radius, number of atoms per unit cell and the packing density are summarized in the table below. Radius Simple cubic Body centered cubic Face centered cubic Diamond ๐⁄ ๐ √๐ ๐⁄ ๐ √๐ ๐⁄ ๐ √๐ ๐⁄ ๐ Atoms/ unit cell 1 2 4 8 Packing density ๐ ⁄๐ = ๐๐% ๐√๐⁄ ๐ = ๐๐% ๐√๐⁄ ๐ = ๐๐% ๐√๐⁄ ๐๐ = ๐๐% Problem 11 Electrons in undoped gallium arsenide have a mobility of 8,800 cm2/V-s. Calculate the average time between collisions. Calculate the distance traveled between two collisions (also called the mean free path). Use an average velocity of 10 7 cm/s. Solution The collision time, tc, is obtained from: ๐๐ ๐๐∗ ๐. ๐๐ ๐ ๐. ๐๐๐ ๐ ๐. ๐ ๐ ๐๐−๐๐ ๐๐ = = = ๐. ๐๐ ๐๐ ๐ ๐. ๐ ๐ ๐๐−๐๐ ๐ = ๐๐๐๐๐๐๐๐ ๐๐ = ๐๐๐ ๐ ๐. ๐๐ ๐ ๐๐−๐๐ = ๐๐ ๐๐ Problem 12 Calculate dielectric relaxation time in p-type Ge at room temperature. Assume that all acceptors are ionized. Na = 1015 cm−3, ฯต = 16, µp = 1900 cm2 V−1s−1. Solution: ๐๐ = ๐ = ๐. ๐ ๐ ๐๐−๐๐ ๐ ๐ ๐ ๐ ๐ต๐ ๐๐ Problem 13 Calculate dielectric relaxation time in intrinsic Si at 300 K. ฯต = 12, µn = 1400 cm2 V−1s−1, µn = 3.1µp. Solution: In this case ๐๐ = ๐ ๐ ๐ ๐ ๐๐ (๐๐ + ๐๐ ) = ๐. ๐ ๐ ๐๐−๐ ๐ Part (2) Solved PROBLEMS conductivity Example (1) Calculate the conductivity and the resistivity of n-type silicon wafer which contains 1016 electrons per cubic centimeter with an electron mobility of 1400 cm2/Vs. Solution: The conductivity is obtained by adding the product of the electronic charge, q, the carrier mobility, and the density of carriers of each carrier type, or: ๐ = ๐ (๐ ๐๐ + ๐ ๐๐ ) As n-type material contains almost no holes, the conductivity equals: ๐ = ๐ ๐ ๐๐ = ๐. ๐ ๐ ๐๐−๐๐ ๐ ๐๐๐๐ ๐ ๐๐๐ = ๐. ๐๐ ๐๐๐๐ The resistivity equals the inverse of the conductivity or: ๐ ๐ ๐= = ๐ ๐ (๐ ๐๐ + ๐ ๐๐ ) and equals ρ = 1/ σ = 1/2.24 = 0.446 Ω cm. Example (2) An n-type piece of silicon of length L = 10 micron has a cross sectional area A= 0.001 cm2. A voltage V = 10 Volts applied across the sample yielding a current I = 100 mA. What is the resistance, R of the silicon sample, its conductivity, σ , and electron density, n? μn= 1400 cm2/Vs Solution The resistance of the sample equals R = V/I = 10/0.1 = 100 Ω. Since R = L /(σA)the conductivity is obtained from: σ = L/(R A) = 0.001/(100 x 0.001) = 0.01 1/ Ω cm. The required electron density is related to the conductivity by: σ = q n μn so that the density equals: n = σ/(qμn) = 0.01/(1.6 x 10-19x 1400) = 4.46 x 1013cm-3. Example (3) A silicon wafer contains 1018cm-3phosphor atoms. Using the data in the table; Arsenic Phosphorus Boron ๐ −๐ −๐ 52.2 68.5 44.9 μmin(๐ ๐ฝ ๐ ) ๐ −๐ −๐ 1417 1414 470.5 μmax(๐ ๐ฝ ๐ ) -3 16 16 Ni (cm ) 9.68 x 10 9.20 x 10 2.23 x 1017 α 0.68 0.711 0.719 Calculate the resistivity and conductivity of the material. Repeat for arsenic and boron atoms. Solution Plugging the values from table into the following equation, ๐๐๐๐ − ๐๐๐๐ ๐ = ๐๐๐๐ + ๐ต ๐ + (๐ต ) ๐ถ ๐ one obtains a mobility of 277 cm2/V-sec for phosphorus-doped material, 284 cm2/V-sec for arsenic-doped material and 153 cm2/V-sec for boron-doped material, corresponding to a resistivity of 22.6, 22.0 and 40.9 mΩ .cm and a conductivity of 44.3, 45.4 and 24.5 1/Ω cm. Example 4 Estimate the electrical conductivity of intrinsic silicon at 300 K, given that the electron and hole motilities are0.15 m2 /V-s and 0.05 m2 /V-s. Solution The conductivity arises due to both electrons and holes ๐ = ๐ ๐๐ (๐๐ + ๐๐ ) The intrinsic carrier concentration was calculated to be at 300 K. Thus ๐ = ๐. ๐ ๐ ๐๐−๐๐ ๐ ๐. ๐ ๐ ๐๐๐๐ ๐ ๐. ๐ = ๐. ๐๐ ๐ ๐๐−๐ ๐/๐ Exercise 5 A sample of an intrinsic semiconductor has a band gap of 0.7 eV, assumed independent of temperature. Taking µh = 0.5 µe and µh = 2 µe, find the relationship between the conductivity at 200 K and300 K. (Ans. ratio of conductivity = 2014.6 eV) EF (300 K) - EF (200 K) = 4.33 x 10-3 eV Example 2.9 A piece of silicon doped with arsenic (Nd = 1017 cm-3) is 100 µm long, 10 µm wide and 1 µm thick. Calculate the resistance of this sample when contacted one each end. Solution The resistivity of the silicon equals: ๐ ๐ ๐= = = ๐. ๐๐๐ ๐ ๐๐ ๐ ๐ ๐๐ ๐. ๐ ๐ ๐๐−๐๐ ๐ ๐๐๐๐ ๐ ๐๐๐ where the mobility was obtained from Table . The resistance then equals ๐ณ ๐๐๐ ๐ ๐๐−๐ ๐น= ๐ = ๐. ๐๐๐ ๐ = ๐. ๐ ๐ฒ๐ ๐๐ ๐๐๐ ๐ ๐๐−๐ ๐๐๐−๐ ๐ ๐. ๐๐๐ ๐น๐ = = = ๐๐๐ ๐/๐๐ ๐ ๐๐−๐ From which one then obtains the resistance: ๐ณ ๐๐๐ ๐ ๐๐−๐ ๐น = ๐น๐ = ๐๐๐ ๐ = ๐. ๐ ๐ฒ๐ ๐ ๐๐ ๐ ๐๐−๐ Problem 2.13 The resistivity of a silicon wafer at room temperature is 5 โฆcm. What is the doping density? Find all possible solutions. Solution Starting with a initial guess that the conductivity is due to electrons with a mobility of 1400 cm2/V-s, the corresponding doping density equals: ๐ ๐ ๐ต๐ซ = ๐ = = = ๐. ๐ ๐ ๐๐๐๐ ๐๐−๐ −๐๐ ๐ ๐๐ ๐ ๐. ๐ ๐ ๐๐ ๐ ๐๐๐๐ ๐ ๐ The mobility corresponding to this doping density equals ๐๐๐๐ − ๐๐๐๐ ๐ ๐๐ = ๐๐๐๐ + ๐ = ๐๐๐๐ ๐๐ /๐๐ ๐ต ๐ + ( ๐ซ) ๐ต๐ Since the calculated mobility is not the same as the initial guess, this process must be repeated until the assumed mobility is the same as the mobility corresponding to the calculated doping density, yielding: Nd = 9.12 x 1014 cm-3 and µn = 1365 cm2/V-s For p-type material one finds: Na = 2.56 x 1015 cm-3 and µp = 453 cm2/V-s Example 2.11 Calculate the electron and hole densities in an n-type silicon wafer (Nd = 1017 cm-3) illuminated uniformly with 10 mW/cm2 of red light (Eph = 1.8 eV). The absorption coefficient of red light in silicon is 10 3 cm-1. The minority carrier lifetime is 10 ms. Solution The generation rate of electrons and holes equals: ๐ท๐ถ๐ท๐ป ๐๐−๐ −๐ ๐ฎ๐ = ๐ฎ๐ = ∝ = ๐๐ = ๐. ๐ ๐ ๐๐๐๐ ๐๐−๐ ๐−๐ ๐ฌ๐๐ ๐ ๐. ๐ ๐ ๐. ๐ ๐ ๐๐−๐๐ Where, α is absorption coefficient, Popt illumination power , Ept is the red light , where the photon energy was converted into Joules. The excess carrier densities are then obtained from: ๐น๐ = ๐น๐ = ๐๐ ๐ฎ๐ = ๐๐ ๐ ๐๐−๐ ๐ ๐. ๐ ๐ ๐๐๐๐ = ๐. ๐ ๐ ๐๐๐๐ ๐๐−๐ The excess carrier densities are then obtained from: So that the electron and hole densities equal: ๐ = ๐๐ + ๐น๐ = ๐๐๐๐ + ๐. ๐ ๐ ๐๐๐๐ = ๐. ๐ ๐ ๐๐๐๐ ๐๐−๐ Problem 2.14 How many phosphorus atoms must be added to decrease the resistivity of n-type silicon at room temperature from 1 โฆ−cm to 0.1 โฆ−cm. Make sure you include the doping dependence of the mobility. State your assumptions. Solution Starting with a initial guess that the conductivity is due to electrons with a mobility of 1400 cm2/V-s, the corresponding doping density corresponding to the initial resistivity of 1 โฆ−cm equals: ๐ ๐ ๐ต๐ซ ≅ ๐ = = = ๐. ๐๐ ๐ ๐๐๐๐ ๐๐−๐ −๐๐ ๐ ๐๐ ๐ ๐. ๐ ๐ ๐๐ ๐ ๐๐๐๐ ๐ ๐ The mobility corresponding to this doping density equals ๐๐ = ๐๐๐๐ + ๐๐๐๐ − ๐๐๐๐ ๐+ ( ๐ต๐ซ ๐ต๐ ๐ = ๐๐๐๐ ๐๐๐ /๐๐ ) Since the calculated mobility is not the same as the initial guess, this process must be repeated until the assumed mobility is the same as the mobility corresponding to the calculated doping density, yielding: Nd,initial = 4.94 x 1015 cm-3 and µn = 1265 cm2/V-s Repeating this procedure for a resistivity of 0.1 โฆ−cm one find the final doping density to be Nd,final = 8.08 x 1016 cm-3 and µn = 772 cm2/V-s The added density of phosphorous atoms therefore equals Nd, added = 4.94 x 1015 - = 7.59 x 1016 cm-3 Problem 2.26 A piece of silicon has a resistivity which is specified by the manufacturer to be between 2 and 5 Ohm cm. Assuming that the mobility of electrons is 1400 cm2/V-sec and that of holes is 450 cm2/V-sec, what is the minimum possible carrier density and what is the corresponding carrier type? Repeat for the maximum possible carrier density. Solution The minimum carrier density is obtained for the highest resistivity and the material with the highest carrier mobility, i.e. the n-type silicon. The minimum carrier density therefore equals: ๐ ๐ ๐= = = ๐. ๐๐ ๐ ๐๐๐๐ ๐๐−๐ −๐๐ ๐ ๐๐ ๐๐๐๐ ๐. ๐ ๐ ๐๐ ๐ ๐๐๐๐๐ ๐ The maximum carrier density is obtained for the lowest resistivity and the material with the lowest carrier mobility, i.e. the p-type silicon. The maximum carrier density therefore equals: ๐ ๐ ๐= = = ๐. ๐๐ ๐ ๐๐๐๐ ๐๐−๐ −๐๐ ๐ ๐๐ ๐๐๐๐ ๐. ๐ ๐ ๐๐ ๐ ๐๐๐๐ ๐ Problem 2.27 A silicon wafer has a 2-inch diameter and contains 1014 cm-3 electrons with a mobility of 1400 cm2/V-sec. How thick should the wafer be so that the resistance between the front and back surface equals 0.1 Ohm? Solution The resistance is given by ๐ณ ๐จ Where A is the area of the wafer and L the thickness, so that the wafer thickness equals: ๐น๐จ ๐. ๐ ๐ ๐ ๐ (๐. ๐๐)๐ ๐ณ= = = ๐. ๐๐๐ ๐๐ ๐ ๐๐. ๐ The resistivity, ๐, was obtained from: ๐ ๐ ๐= = = ๐๐. ๐ ๐ ๐๐ ๐ ๐ ๐๐ ๐. ๐ ๐ ๐๐−๐๐ ๐ ๐๐๐๐๐ ๐๐๐๐ Part (3) Solved PROBLEMS ๐น= ๐ Temperature Dependence of Semiconductor Conductivity Band gap of Si depends on the temperature as Eg = 1.17 eV − 4.73 × 10−4 T2 / T + 636 . Find a concentration of electrons in the conduction band of intrinsic (undoped) Si at T = 77 K if at 300 K ni = 1.05 × 1010 cm−3. Solution: (1.2) ๐๐๐ ๐ฌ๐ ๐ฌ๐ ๐ = ๐ต๐ ๐ต๐ ๐๐๐ (− ) ≈ ๐ป ๐๐ฑ๐ฉ (− ) ๐ฒ๐ป ๐ฒ๐ป Therefore, ๐ป๐ ๐๐ (๐ป๐ ) = ๐๐ (๐ป๐ ) ( ) ๐ป๐ ๐⁄ ๐ ๐๐ฑ๐ฉ (− ๐ฌ๐ ๐ป๐ ๐ฌ๐ ๐ป๐ + ) ๐ ๐ฒ ๐ป๐ ๐ ๐ฒ ๐ป ๐ Putting the proper values in the formula we obtain that ni(77K) ≈ 10−20cm−3. 5. Hole mobility in Ge at room temperature is 1900 cm2 V−1s−1. Find the diffusion coefficient. Solution: (1.5) From eD = μkT, it follows that D = 49 cm2/s. Example 2.4b Calculate the intrinsic carrier density in germanium, silicon and gallium arsenide at 300, 400, 500 and 600 K. Solution The intrinsic carrier density in silicon at 300 K equals: − ๐ฌ๐ ๐๐ (๐๐๐๐ฒ) = √๐ต๐ ๐ต๐ ๐๐๐ ( ) ๐ ๐ฒ๐ป − ๐. ๐๐ = √๐. ๐๐ ๐ ๐๐๐๐ ๐ ๐. ๐๐ ๐ ๐๐๐๐ ๐๐๐ ( ) ๐ ๐ ๐. ๐๐๐๐ = ๐. ๐๐ ๐ ๐๐๐ ๐−๐ Similarly, one finds the intrinsic carrier density for germanium and gallium arsenide at different temperatures, yielding: 300 K 400 K 500 K 600 K Germanium 2.02 x 1013 1.38 x 1015 1.91 x 1016 1.18 x 1017 Silicon 8.72 x 109 4.52 x 1012 2.16 x 1014 3.07 x 1015 Gallium Arsenide 2.03 x 106 5.98 x 109 7.98 x 1011 2.22 x 1013 Example 2.2 Calculate the energy band gap of germanium, silicon and gallium arsenide at 300, 400, 500 and 600 K. Solution The band gap of silicon at 300 K equals: ๐ ๐ป๐ ๐. ๐๐๐ ๐ ๐๐−๐ ๐ (๐๐๐)๐ ๐ฌ๐ (๐๐๐ ๐) = ๐ฌ๐ (๐ ๐) − = ๐. ๐๐๐ − ๐ป+๐ ๐๐๐ + ๐๐๐ = ๐. ๐๐ ๐๐ฝ Similarly, one finds the energy band gap for germanium and gallium arsenide, as well as at different temperatures, yielding: Germanium Silicon 0.66 eV 0.62 eV 0.58 eV 0.54 eV 1.12 eV 1.09 eV 1.06 eV 1.03 eV T = 300 K T = 400 K T = 500 K T = 600 K Gallium Arsenide 1.42 eV 1.38 eV 1.33 eV 1.28 eV Problem 2.2 At what temperature does the energy band gap of silicon equal exactly 1 eV? Solution The energy band gap is obtained from: ๐ ๐ป๐ ๐. ๐๐๐ ๐ ๐๐−๐ ๐ ๐ป๐ ๐ฌ๐ (๐ป) = ๐ฌ๐ (๐ ๐) − = ๐. ๐๐๐ − = ๐ ๐๐ฝ ๐ป+๐ ๐ป + ๐๐๐ The type equation here is quadratic equation can be solved yielding ๐ฌ๐ (๐ ๐) − ๐ฌ๐ (๐ป ๐) ๐ป= ๐๐ ๐ ๐ (๐ฌ๐ (๐ ๐) − ๐ฌ๐ (๐ป ๐)) ( ) ( ) ๐ฌ ๐ ๐ − ๐ฌ ๐ป ๐ ๐ ๐ √ + ( ) + ๐๐ ๐ = ๐๐๐ ๐ฒ Problem (6) If no electron-hole pairs were produced in germanium (Ge) until the temperature reached the value corresponding to the energy gap, at what temperature would Ge become conductive? (Eth = 3/2 kT) Solution ๐ฌ๐๐ = ๐ป= ๐ ๐ฒ๐ป ๐ , ๐ฌ๐ = ๐. ๐๐๐ ๐. ๐ ๐ ๐๐−๐๐ ๐ฑ ๐. ๐๐ ๐ ๐. ๐ ๐ ๐๐−๐๐ ๐ ๐ = ๐๐๐๐ ๐ฒ = ๐. ๐ ๐ ๐๐๐ ๐๐ช −๐๐ ๐ ๐ ๐. ๐๐ ๐ ๐๐ The temperature would have to be 5.3 x 103oC, about 4400oC above the melting point of Ge. Example (3) Hole mobility in Ge at room temperature is 1900 cm2 V−1s−1. Find the di๏ฌusion coe๏ฌcient. Solution: From eD = µkT, it follows that D = 49 cm2/s. 8. How does the reverse current of a Si p-n junction change if the temperature raises from 20 to 50 โฆC? The same for a Ge pn junction. Band gaps of Si and Ge are 1.12 and 0.66 eV, respectively. Solution: (3.8) Since ๐ฑ๐ ~ ๐๐๐ ~ ๐ป๐ ๐๐๐ (− ๐ฌ๐ ๐ฒ๐ป ), we get ๐ฌ๐ ๐ฌ๐ ๐ฑ๐ (๐ป๐ ) ๐ป๐ ๐ = ( ) ๐๐๐ (− + ) ๐ฑ๐ (๐ป๐ ) ๐ป๐ ๐ฒ ๐ป๐ ๐ฒ ๐ป๐ From here the ratios of the reverse currents in the p-n junctions made of Ge and Si are 15 and 82, respectively. 9. Estimate temperatures at which p-n junctions made of Ge, Si, and GaN lose their rectifying characteristics. In all cases Na = Nd = 1015 cm−3. Assume that Eg are independent of the temperature and are 0.66, 1.12, and 3.44 eV for Ge, Si, and GaN, respectively. Intrinsic carrier concentrations at room temperature are nGei = 2 × 1013, nSii = 1010, and nGaNi = 10−9 cm−3. Solution: (3.9) p-n junction stops working when concentrations of electrons and holes equalize. It happens when Nd(Na) ≈ ni = √NcNv exp(−Eg/2kT) ≈ T3/2 exp(−Eg/2kT). From here and the parameters given we get that the maximum temperatures are TGe ≈ 400 K, TSi ≈ 650 K, and TGaN ≈ 1700 K. That is, only wide band gap semiconductors are suitable for extremely applications. Part (4) Solved PROBLEMS Electron and Hole Concentrations Example 2.6a A germanium wafer is doped with a shallow donor density of 3 ni/2. Calculate the electron and hole density. Solution The electron density is obtained from equation ๐ + ๐ต๐ซ − ๐ต− ๐ต+ − ๐ต− ๐ ๐ ๐จ ๐ซ ๐จ ๐ √ √ ๐๐ = + ( ) + ๐๐ = ๐๐ ( + + ๐) ๐ ๐ ๐ ๐๐ = ๐ ๐๐ and the hole density is obtained using the mass action law: ๐๐๐ ๐๐ ๐๐ = = ๐๐ ๐ Example 2.6b A silicon wafer is doped with a shallow acceptor doping of 10 16 cm-3. Calculate the electron and hole density. Solution Since the acceptor doping is much larger than the intrinsic density and much smaller than the effective density of states, the hole density equals: ๐๐ −๐ ๐๐ ≅ ๐ต+ ๐ = ๐๐ ๐๐ The electron density is then obtained using the mass action law ๐๐๐ ๐๐๐๐ ๐๐ = + = ๐๐ = ๐๐๐ ๐๐−๐ ๐ต๐ซ ๐๐ Problem 2.6 Calculate the effective density of states for electrons and holes in germanium, silicon and gallium arsenide at room temperature and at 100 °C. Use the effective masses for density of states calculations. Solution The effective density of states in the conduction band for germanium equals: ๐ ๐ ๐๐∗ ๐ฒ๐ป ๐ต๐ = ๐ ( ) ๐๐ ๐⁄ ๐ ๐⁄ ๐ ๐ ๐ ๐. ๐๐ ๐ ๐. ๐๐ ๐ ๐๐−๐๐ ๐ ๐. ๐๐ ๐ ๐๐−๐๐ ๐ ๐๐๐ ๐ =๐ ( ) (๐. ๐๐๐ ๐ ๐๐−๐๐ )๐ = ๐. ๐๐ ๐ ๐๐๐๐ ๐−๐ = ๐. ๐๐ ๐ ๐๐๐๐ ๐๐−๐ Where, the effective mass for density of states is used. Similarly, one finds the effective densities for silicon and gallium arsenide and those of the valence band, using the effective masses listed below: me/m0 Nc (cm-3) Nv (cm-3) Germanium 0.55 1.02 x 1019 5.64 x 1018 Silicon 1.08 2.81 x 1019 1.83 x 1019 Gallium Arsenide 0.067 4.35 x 1017 7.57 x 1018 The effective density of states at 100 °C (372.15 K) are obtain from: ๐ป ๐ต๐ (๐ป) = ๐ต๐ (๐๐๐๐) ( ) ๐๐๐ ๐⁄ ๐ yielding: T = 100°C Nc (cm-3) Nv (cm-3) Germanium 1.42 x 1019 7.83 x 1018 Silicon 3.91 x 1019 2.54 x 1019 Gallium Arsenide 6.04 x 1017 1.05 x 1018 Problem 2.7 Calculate the intrinsic carrier density in germanium, silicon and gallium arsenide at room temperature (300 K). Repeat at 100 °C. Assume that the energy band gap is independent of temperature and use the room temperature values. Solution The intrinsic carrier density is obtained from: ๐ฌ๐ ๐๐ (๐ป) = √๐ต๐ ๐ฝ๐ ๐๐๐ (− ) ๐๐ฒ๐ป where both effective densities of states are also temperature dependent. Using the solution of Problem 2.6 one obtains T = 300 K ni (cm-3) T = 100°C ni(cm-3) Germanium 2.16 x 1013 Germanium 3.67 x 1014 Silicon 8.81 x 109 Silicon 8.55 x 1011 Gallium Arsenide 1.97 x 106 Gallium Arsenide 6.04 x 108 Example 2.11 Calculate the electron and hole densities in an n-type silicon wafer (Nd = 1017 cm-3) illuminated uniformly with 10 mW/cm2 of red light (Eph = 1.8 eV). The absorption coefficient of red light in silicon is 10-3 cm-1. The minority carrier lifetime is 10 µs. Solution The generation rate of electrons and holes equals: ๐๐๐๐ ๐๐−๐ −๐ ๐ฎ๐ = ๐ฎ๐ = ๐ = ๐๐ ๐ฌ๐๐ ๐จ ๐. ๐ ๐ ๐. ๐ ๐ ๐๐−๐๐ = ๐. ๐ ๐ ๐๐๐๐ ๐๐−๐ ๐−๐ where the photon energy was converted into Joules. The excess carrier densities are then obtained from ๐ ๐ = ๐ ๐ = ๐๐ ๐ฎ๐ = ๐๐ ๐ ๐๐−๐ ๐ ๐. ๐ ๐ ๐๐๐๐ = ๐. ๐ ๐ ๐๐๐ ๐๐−๐ So that the electron and hole densities equal: ๐ = ๐๐ + ๐ ๐ = ๐๐๐๐ + ๐. ๐ ๐ ๐๐๐ = ๐๐๐๐ ๐๐−๐ (๐๐๐๐ )๐ ๐๐๐ ๐= + ๐ ๐ = + ๐. ๐ ๐ ๐๐๐ = ๐. ๐ ๐ ๐๐๐ ๐๐−๐ ๐๐ ๐๐ ๐๐ Problem 2.11 A silicon wafer contains 1016 cm-3 electrons. Calculate the hole density and the position of the intrinsic energy and the Fermi energy at 300 K. Draw the corresponding band diagram to scale, indicating the conduction and valence band edge, the intrinsic energy level and the Fermi energy level. Use ni = 1010 cm-3. Solution The hole density is obtained using the mass action law: ๐๐๐ ๐๐๐๐ ๐= = = ๐๐๐ ๐๐−๐ ๐๐ ๐ ๐๐ The position of the intrinsic energy relative to the midgap energy equals: ๐ฌ๐ + ๐ฌ๐ ๐ ๐๐∗ ๐ ๐. ๐๐ ๐ฌ๐ − = − ๐ฒ๐ป ๐๐ ∗ = ๐ ๐. ๐๐๐๐ ๐๐ ๐ ๐ ๐๐ ๐ ๐. ๐๐ = ๐. ๐๐ ๐๐๐ฝ The position of the Fermi energy relative to the intrinsic energy equals: ๐ต๐ ๐๐๐๐ ๐ฌ๐ญ − ๐ฌ๐ = ๐ฒ๐ป ๐๐ ( ) = ๐. ๐๐๐๐ ๐๐ = ๐๐๐ ๐๐๐ฝ ๐๐ ๐๐๐๐ Problem 2.12 A silicon wafer is doped with 1013 cm-3 shallow donors and 9 x 1012 cm-3 shallow acceptors. Calculate the electron and hole density at 300 K. Use ni = 1010 cm-3. Solution Since there are more donors than acceptors, the resulting material is n-type and the electron density equals the difference between the donor and acceptor density or: ๐ = ๐ต๐ − ๐ต๐ = ๐๐๐๐ − ๐ ๐ ๐๐๐๐ = ๐๐๐๐ ๐๐−๐ The hole density is obtained by applying the mass action law: ๐๐๐ ๐๐๐๐ ๐= = = ๐๐๐ ๐๐−๐ ๐๐ ๐ ๐๐ Example (1) A Si sample at room temperature is doped with 1011As atoms/cm3. What are the equilibrium electron and hole concentrations at 300 K? Solution Since the NAis zero we can write, ๐๐ ๐๐ = ๐๐๐ ๐๐๐ ๐๐ + ๐ต๐จ = ๐๐ + ๐ต๐ซ ๐๐๐ − ๐ต๐ซ − ๐๐๐ = ๐ Solving this quadratic equation results in n0= 1.02x1011[cm-3] and thus, p0= ni2/ n0= 2.25x1020/ 1.02x1011 p0= 2.2x109[cm-3] Notice that, since ND>ni, the results would be very similar if we assumed no=ND=1011cm-3, although there would be a slight error since NDis not much greater than ni. Question 2: What are the carrier concentrations and Conductivity in intrinsic Si?[For Si: ๏ฅg = 1.1 eV, me* = 0.25me, mh* = 0.5me, ๏ญe = 0.15 m2V-1s-1, ๏ญh = 0.05 m2V-1s-1] Solution: For intrinsic material , nc = pv = ni, Obtain ni from: 3 2 ๏ฌ ๏ฅ ๏ผ ๏ฆ kT ๏ถ exp ni = 2๏จm m ๏ฉ ๏ง ๏ท ๏ญ๏ญ ๏ฝ ๏จ ๏ฐ๏จ ๏ธ ๏ฎ 2kT ๏พ For Si: * * e h 3 4 g 2 ๏ฅg = 1.1 eV, me* = 0.25me, mh* = 0.5me So at room temperature (T = 300K): ๐⁄ ๐๐ ๐๐ = ๐ (๐. ๐๐ ๐๐ ๐ ๐. ๐ ๐๐ ) ๐๐ฑ๐ฉ {− { ๐⁄ ๐ ๐ ๐ ๐๐๐ } ๐. ๐๐ ๐๐๐ ๐ ๐. ๐ ๐๐ฝ } = ๐. ๐ ๐ ๐๐๐๐ ๐−๐ ๐ ๐ ๐๐๐ ๐ Conductivity ๏ณ = nce๏ญe + pve๏ญh ๏ ๏ ๏ ๏ณ๏ = nie๏ญe + nie๏ญh ๐ = (๐. ๐ ๐ ๐๐๐๐ ๐−๐ ๐ ๐. ๐ ๐๐๐−๐๐ ๐ ๐. ๐๐ ๐๐ /๐๐ฌ) + (๐. ๐ ๐ ๐๐๐๐ ๐−๐ ๐ ๐. ๐ ๐๐๐−๐๐ ๐ ๐. ๐๐ ๐๐ /๐๐ฌ)๏ ๏ ๏ณ = (2.3 ๏ด 10-4) + (7.8 ๏ด 10-5) ๏-1m-1 = (2.3 + 0.78) x 10-4 ๏ณ = 3.1 ๏ด 10-4๏-1m-1 Comparing answers for Q1 and Q2: doping Si with 1 part in 106 (of P) has led to an increase in ๏ณ of a factor > than 106. Example 10 (3) Pure germanium has a band gap of 0.67 eV. It is doped with 3 x 1021/ m3 of donor atoms. Find the densities of electrons and holes at 300 K. (effective masses me = 0.55 mo and mh = 0.37 mo). Solution: For Ge , the intrinsic concentration is − ๐ฌ๐ ⁄ ๐๐๐ป √๐ต๐ ๐ต๐ ๐ ๐๐ = From tables, we find for pure germanium NC = 1 x 1025 and NV = 6 x 1024 , Eg = 067 eV Substituting −๐.๐๐⁄ ๐ ๐ ๐.๐๐๐ ๐๐ = √๐๐ ๐๐๐๐ ๐ ๐๐ ๐๐๐๐ ๐ Given numerical values, ni = 2.4 x 1019 / m3 The density of donor atoms is ND = 3 x 1021/m3. Thus the electron density is given by: ๐ต๐ ๐ต๐๐ + ๐ ๐๐๐ √ ๐= + ≅ ๐ต๐ ๐๐ ๐ต๐ >> ๐๐ ๐ ๐ Substituting, ๐= ๐๐๐๐๐๐ ๐ ๐๐ )๐ +๐ (๐.๐๐๐๐๐๐ )๐ (๐๐๐๐ + √ ๐ Thus, n = 3 x , using ๐๐๐ = n p , we get for the density of holes (2.4 x 1019)2 = 3 x 1021p , then p =(2.4 x 1019)2/3 x 1021= p = 1.92 x 1017/m3. 1021/m3 Problem (4) The resistivity of a silicon wafer at room temperature is 5 โฆ cm. What is the doping density? Find all possible solutions. Solution: Starting with an initial guess that the conductivity is due to electrons with a mobility of 1400 cm2/V-s, the corresponding doping density equals: ๐ ๐ = = ๐. ๐ ๐ ๐๐๐๐ ๐๐−๐ −๐๐ ๐ ๐๐ ๐ ๐. ๐ ๐ ๐๐ ๐ ๐๐๐๐ ๐ ๐ The mobility corresponding to this doping density equals ๐๐๐๐ − ๐๐๐๐ ๐๐ = ๐๐๐๐ + ๐ต ∝ ๐ + ( ๐ ) ๐ต๐ซ ≅ ๐ = ๐ต๐ Since the calculated mobility is not the same as the initial guess, this process must be repeated until the assumed mobility is the same as the mobility corresponding to the calculated doping density, yielding: Nd = 9.12 x 1014 cm-3 and µn = 1365 cm2/V-s. For p-type material one finds: Na = 2.56 x 1015 cm-3 and µp = 453 cm2/V-s Nd = 9.12 x 1014 cm-3 and µn = 1365 cm2/V-s For p-type material one finds: Na = 2.56 x 1015 cm-3 and µp = 453 cm2/V-s Problem (5) Consider the problem of finding the doping density, which results in the maximum possible resistivity of silicon at room temperature. (ni = 1010 cm-3, µn = 1400 cm2/V-sec and µp = 450 cm2/V-sec.) Should the silicon be doped at all or do you expect the maximum resistivity when dopants are added? If the silicon should be doped, should it be doped with acceptors or donors (assume that all dopant is shallow). Calculate the maximum resistivity, the corresponding electron and hole density and the doping density. Solution Since the mobility of electrons is larger than that of holes, one expects the resistivity to initially decrease as acceptors are added to intrinsic silicon. The maximum resistivity (or minimum conductivity) is obtained from: ๐๐๐ ๐๐⁄ ๐ (๐ ๐๐ + ๐) ๐ (๐ ๐๐ + ๐๐๐ ) ๐ ๐ =๐ =๐ = ๐ ๐ ๐ ๐ ๐ ๐ ๐ Which yields, ๐๐ ๐ = ๐๐ √ = ๐. ๐๐ ๐๐ = ๐. ๐ ๐ ๐๐๐ ๐๐−๐ ๐๐ The corresponding hole density equals p = 1.76 ni = 1.76 x 109 cm-3 And the amount of acceptors one needs to add equals Na = 1.20 ni = 1.20 x 109 cm-3. The maximum resistivity equals: ๐ ๐ ๐๐๐๐ = = ๐ (๐ ๐๐ + ๐๐๐ ) ๐ ๐๐ (๐๐ + ๐๐ ) ๐ = = ๐๐๐ ๐๐. ๐๐ ๐. ๐ ๐ ๐๐−๐๐ ๐ ๐๐๐๐ (๐๐๐๐ + ๐๐๐) Problem (6) The electron density in silicon at room temperature is twice the intrinsic density. Calculate the hole density, the donor density and the Fermi energy relative to the intrinsic energy. Repeat for n = 5 ni and n = 10 ni. Also repeat for p = 2 ni, p = 5 ni and p = 10 ni, calculating the electron and acceptor density as well as the Fermi energy relative to the intrinsic energy level. Solution: The hole density is obtained using the mass action law: p = ni2/n The doping density is obtained by requiring charge neutrality Nd - Na = n - p The Fermi energy is obtained from: EF - Ei = kT ln(n/ni) yielding: p Nd - Na n = 2 ni ni/2 1.5 ni n = 5 ni ni /5 4.8 ni n = 10 ni ni/10 9.9 ni EF - Ei kT ln(2) kT ln(5)) kT ln(10) n Nd - Na EF - Ei p = 2 ni ni /2 -1.5 ni -kT ln(2) p = 5 ni ni /5 -4.8 ni -kT ln(5) p = 10 ni ni /10 -9.9 ni -kT ln(10) Exercise 7 A sample of Ge at 300 K is doped with 3 x 1021/m3 of donor atoms and 4 x 1021/m3 acceptor atoms. Find the densities of electrons and holes at 300 K. (answer, n = 5.76 x 1017/m3 , p = 1021/m3 ) Problem (8) (a) The lattice constant of GaAs is 5.65 A, Determine the number of Ga atoms and As atoms per cm3. (b) Determine the volume density of germanium atoms in a germanium semiconductor. The lattice constant of germanium is 5.65 A. Solution: (a) 4 Ga atoms per unit cell Density= ๐ ๐ (๐.๐๐ ๐ ๐๐−๐ ) Density of Ga=2.22×1022cm−3 4 As atoms per unit cell, so that Density of As=2.22×1022cm−3 ๐ (b) 8 Ge atoms per unit cell Density= −๐ ๐ (๐.๐๐ ๐ ๐๐ → Density of ) Ge=4.44×1022cm−3 Problem (9) Calculate the density of valence electrons in silicon. Solution: Density or silicon atoms= 5×1022cm−3 and 4 valence electrons per atom, So Density of Valence electrons = 4 x 5×1022cm−3= 2 x 1023cm−3 Problem 10 (a) Determine the amount (in grams) of boron (B) that, substitution ally incorporated into 1 kg of germanium (Ge), will establish a charge carrier density of 3.091 x 1017/cm3. (b) Draw a schematic energy band diagram for this material, and label all critical features. Solution (a) The periodic table gives the molar volume of Ge as 13.57 cm3 and 1 mole of Ge weighs 72.61 g, so set up the ratio ๐๐. ๐๐ ๐๐๐๐ ๐ = ๐๐. ๐๐ ๐ and solve for x to get 187.30 cm3 for the total volume. The addition of boron gives 1 charge carrier/B atom. B concentration in Si must be 3.091 x 1017 B/cm3 NA of B atoms weighs 10.81 g ∴ ๐. ๐๐๐ ๐ ๐๐๐๐ ๐ฉ ๐๐๐๐๐ ๐๐๐๐๐ = ๐.๐๐๐ ๐ ๐๐๐๐ ๐.๐๐ ๐ ๐๐๐๐ ๐ ๐๐. ๐๐ = ๐. ๐๐ ๐ ๐๐๐ ๐ ∴ for every 1 cm3 of Ge, add 5.55 x 10–6 g for 187.30 cm3 of Ge, add 187.30 x 5.55 x 10–6 = 1.04 x 10–3 g B Conduction band Eg B+ ….…….B+ ………….. B+ 3.091X1017B ions in the band Acceptor level for B Valance band3.091X1017holes in the V.B Problem (11) The number of electron-hole pairs in intrinsic germanium (Ge) is ๐ ๐⁄ − ๐ฌ๐⁄ ๐๐ ๐ ๐ฒ๐ป๐๐ (๐ฌ๐ given by: ๐๐ = ๐. ๐ ๐ ๐๐๐๐ ๐ป = ๐. ๐๐ ๐๐ฝ) (a) What is the density of pairs at T = 20°C? (b) Will undoped Ge be a good conductor at 200°C? If so, why? Solution (a) Recall: T in thermally activated processes is the absolute temperature: T oK = (273.16 + t oC); Boltzmann’s constant = k = 1.38 x 10–23 J/oK T = 293.16K: ๐๐ −๐๐ ๐⁄ − ๐.๐๐ ๐ ๐.๐ ๐ ๐๐ ⁄ ๐๐๐ ๐ ๐ ๐.๐๐ ๐ ๐๐−๐๐ ๐ ๐๐๐.๐๐ ๐ (๐๐๐. ๐๐) ๐ ๐๐ −๐ ๐๐ ๐ ๐๐ = ๐. ๐ ๐ ๐๐ ๐ = ๐. ๐ ๐ ๐๐ ๐ ๐๐๐๐ ๐ ๐. ๐ ๐ ๐๐ = ๐. ๐๐ ๐ ๐๐ / ๐๐ (b) 200 oC = 473.16 K ๐ − ๐.๐๐ ๐ ๐.๐ ๐ ๐๐−๐๐⁄ ๐๐๐ ๐ ๐ ๐.๐๐ ๐ ๐๐−๐๐ ๐ ๐๐๐.๐๐ ๐๐ = ๐. ๐ ๐ ๐๐ ๐ (๐๐๐. ๐๐) ⁄๐ ๐ = ๐. ๐ ๐ ๐๐๐๐ ๐ ๐, ๐๐ ๐ ๐๐๐ ๐ ๐. ๐๐ ๐ ๐๐−๐ = ๐. ๐๐ ๐ ๐๐๐๐ / ๐๐๐ ๐๐ The number of conducting electrons (in the conduction band) at 200oC is by about five orders of magnitude less than that of a good conductor. The material will not be a good conductor. (There are additional factors which contribute to the relatively poor conductivity of Ge at this temperature.) Problem (12) Band gap of Si depends on the temperature as ๐ป๐ ๐ฌ๐ = ๐. ๐๐ ๐๐ฝ − ๐. ๐๐ ๐ ๐๐ ๐ป + ๐๐๐ Find a concentration of electrons in the conduction band of intrinsic (un doped) Si at T = 77 K if at 300 K ni = 1.05×1010 cm−3. −๐ Solution: ๐๐๐ = ๐ต๐ ๐ต๐ ๐๐๐ (− ๐ฌ๐ ๐ฌ๐ ) ≈ ๐ป๐ ๐๐๐ (− ) , ๐๐๐๐๐๐๐๐๐ ๐ฒ๐ป ๐ฒ๐ป ๐๐ (๐ป๐ ) = ๐๐ (๐ป๐ ) ๐⁄ ๐ ๐๐๐ (− ๐ฌ๐ (๐ป๐ ) ๐ฌ๐ (๐ป๐ ) + ) ๐๐ฒ๐ป๐ ๐๐ฒ๐ป๐ Putting the proper values in the formula we obtain that ni(77K) ≈ 10−20cm−3. Problem (13) (a) Assume the mobility ratio µn / µp = b in Si is a constant independent of impurity concentration. Find the maximum resistivity p, in terms of the intrinsic resistivity pi at 300 K. If b = 3 and the hole mobility of intrinsic Si is 450 cm2/V-s, calculate ρi and pn. (b) Find the electron and hole concentration, mobility, and resistivity of a GaAs sample at 300 K with 5X1015 zinc atoms/cm3, 1017 sulfur atoms/cm3, and 1017 carbon atoms/cm3. Problem (14) Consider a compensated n-type silicon at T= 300 K, with a conductivity of σ= 16 S/cm and an acceptor doping concentration of 10I7cm-3. Determine the donor concentration and the electron mobility. (A compensated semiconductor is one that contains both donor and acceptor impurity atoms in the same region.) Exercise (2) For a two band model of silicon, the band gap is 1.11 eV. Taking the effective masses of electrons and holes as me = 1.08 mo and mh = o.81 mo , calculate the intrinsic carrier concentration in silicon at 300 K. (KT=0.026 eV) Solution: Applying the equation ๐ ๐ ๐ฒ๐ป ๐๐ = ( ) ๐ ๐ ๐๐ ๐⁄ ๐ ๐⁄ −๐ซ ๐ ๐ ⁄๐ ๐ฒ๐ป (๐๐ ๐๐ ) (๐ซ) Then, ๐ ๐ ๐ ๐ ๐. ๐๐๐ ⁄๐ ๐⁄ −๐.๐๐⁄ ๐๐ ๐.๐๐๐ ( ) ๐๐ = ( ) ๐. ๐๐ ๐ ๐ฑ ๐. ๐๐ ๐ ๐ ๐ ๐ ๐. ๐๐ ๐๐ = ๐. ๐ ๐ ๐๐๐๐ ๐−๐ Example (4) Carrier Concentrations 3 What is the hole concentration in an N-type semiconductor with 1015cm– of donors? (ni is a strong function of Eg and T according to Eq. ๐๐ = − ๐ฌ๐ ⁄ ๐๐ฒ๐ป , but is independent of the dopant concentration. ni at room √ ๐ต๐ ๐ต๐ ๐ temperature is roughly 1010cm–3 for Si and 107cm–3 for GaAs, which has a larger band gap than Si. For silicon, the np product is therefore 1020cm–6 regardless of the conductivity type (P type or N type) and the dopant concentrations). Solution: For each ionized donor, an electron is created. Therefore, n = 1015cm–3. ๐๐๐ ๐๐๐๐ ๐๐−๐ ๐= = = ๐๐๐ ๐๐−๐ ๐๐ −๐ ๐ ๐๐ ๐๐ With a modest temperature increase of 60°C, n remains the same at 1015cm–3, while p increases by about a factor of 2300 because ni2 increases according to Eq. ๐๐ = − ๐ฌ๐ ⁄ ๐๐ฒ๐ป √๐ต๐ ๐ต๐ ๐ Example (5) What is n if p = 1017cm–3 in a P-type silicon wafer? Solution: ๐๐๐ ๐๐๐๐ ๐๐−๐ ๐= = = ๐๐๐ ๐๐−๐ ๐๐ −๐ ๐ ๐๐ ๐๐ Part (5) Solved PROBLEMS The Concept of Mobility , FIELD DEPENDENCE Problem 2.28 –(1) Electrons in silicon carbide have a mobility of 1000 cm2/Vsec. At what value of the electric field do the electrons reach a velocity of 3 x 107 cm/s? Assume that the mobility is constant and independent of the electric field. What voltage is required to obtain this field in a 5 micron thick region? How much time do the electrons need to cross the 5 micron thick region? Solution: The electric field is obtained from the mobility and the velocity: ๐ ๐๐๐๐ ๐บ= = = ๐๐ ๐๐ฝ/๐๐ ๐ ๐ ๐ ๐๐๐ Combined with the length one finds the applied voltage. V = εL = 30,000 x 5 x 10-4 = 15 V The transit time equals the length divided by the velocity: tr = L/v = 5 x 10-4 /3 x 107 = 16.7 ps 1 Thermal Velocity EXAMPLE 2 What are the approximate thermal velocities of electrons and holes in silicon at room temperature? SOLUTION: Assume T = 300 K and recall mn = 0.26 m0. 1 3 2 ๐พ๐๐๐๐ก๐๐ ๐๐๐๐๐๐ฆ = ๐๐ ๐๐กโ = ๐พ๐ 2 2 1⁄ 2 3 ๐พ๐ 300 ๐พ −23 ๐ฝ⁄ ) ๐ฅ ( = ๐ฅ 1.38 ๐ฅ 10 ๐ฅ 9.1 ๐ฅ 10−31 ๐๐)] [(3 ๐๐กโ = √ ๐ ๐พ 0.26 = 2.3 ๐ฅ ๐5 ๐⁄๐ = 2.3 ๐ฅ 107 ๐๐⁄๐ Note that 1 J = 1 kg·m2/s2. Using mp = 0.39 m0 instead of mn, one would find the hole thermal velocity to be 2.2 × 107cm/s. So, the typical thermal velocity of electrons and holes is 2.5 × 107cm/s, which is about 1000 times slower than the speed of light and 100 times faster than the sonic speed. Part (6) Solved PROBLEMS complete ionization 8. Find Debye length in p-type Ge at 300 K if Na = 1014 cm−3. Assume that all acceptors are ionized, ε = 16. Solution: (1.8) LD = 0.48 μm. Example 2.5 Calculate the ionization energy for shallow donors and acceptors in germanium and silicon using the hydrogen-like model. Solution Using the effective mass for conductivity calculations (Appendix 3) one finds the ionization energy for shallow donors in germanium to be: ∗ ๐๐๐๐๐ ๐. ๐๐ ๐ฌ๐ − ๐ฌ๐ซ = ๐๐. ๐ ๐๐ฝ = ๐๐. ๐ ๐๐ฝ = ๐. ๐ ๐๐๐ฝ (๐๐)๐ ๐๐ ๐๐๐ The calculated ionization energies for donors and acceptors in germanium and silicon are provided below. donors acceptors Germanium 6.4 meV 11.2 meV Silicon 13.8 meV 20.5 meV Note that the actual ionization energies differ from this value and depend on the actual donor atom Example (1) A Si sample is doped with 10-4 atomic% of P donors. Assuming complete ionization of donors at room temperature, calculate the charge carrier concentration and conductivity at room temperature. [For Si: ρ= 2330 kg m-3, atomic weight = 28, μe= 0.15 m2V-1s-1 , μh= 0.05 m2V-1s-1, ni= 1.5x1010carriers per cm3] Solution: 1) Calculate the fraction of donor atoms (phosphorus atoms per silicon atom) where NSi–number of Si atoms per unit volume ๐ต๐ซ = ๐๐−๐ ๐ต๐บ๐ Calculate the number of silicon atoms per unit volume ๐ ๐๐๐๐ ๐๐ ๐−๐ ๐ต๐บ๐ = ๐ ๐ต๐จ๐๐๐๐๐ ๐๐ = ๐ ๐ ๐ ๐๐๐๐ ๐๐๐๐๐. ๐๐๐−๐ ๐จ๐บ๐ ๐๐ ๐ ๐๐−๐ ๐๐ ๐๐๐−๐ = ๐ ๐ ๐๐๐๐ ๐บ๐ − ๐๐๐๐ ๐๐ 3) Calculate the number of donors atoms (phosphorus) ๐ต๐ซ = ๐ ๐ ๐๐๐๐ ๐ − ๐๐๐๐ ๐๐ 4) As NA=0 and ND>>ni, then we can safely assume that no=ND and po is very small ~ zero ๐ = ๐๐ ๐ ๐ ๐ ๐๐ ๐๐ ๐ = (๐๐๐๐ ๐ − ๐๐๐๐ ๐๐ ) ๐ (๐. ๐ ๐๐๐−๐๐ ๐ช) ๐ (๐. ๐๐ ๐๐ ๐ฝ−๐ ๐−๐ ) = ๐๐๐๐ ๐−๐ ๐−๐ Example (2) A Si sample is doped with 10-4 atomic% of P donors. Assuming complete ionisation of donors at room temperature, calculate the charge carrier concentration and conductivity at room temperature. [For Si: ๏ฒ = 2330 kg m-3, atomic weight = 28, ๏ญe = 0.15 m2V-1s-1, Avogadro’s No= 6 x 1023] Answer 1 N ๏ฝ 10 N Where NSi – number of Si atoms per unit volume ๏ญ6 d Si Obtain NSi from NSi = Resistivity x Avogadro’s No. / Atomic weight ๏ฒ N ๏ฝ ๏ด 6 ๏ด 10 28 ๏ด 10 23 Si ๐ต๐บ๐ = ๏ญ3 ๐๐๐๐ ๐ ๐ ๐ ๐๐๐๐ −๐ ๐๐ ๐ ๐๐ This gives NSi = 5 × 1028 m-3 So Nd =NSi x 10-4 % = 5 × 1028 m-3 x 10-6 Nd = 5 × 1022 m-3. Complete ionisation, n-type semiconductor: So charge carrier concentration is nc = Nd = 5 × 1022 m-3 (Neglect pv) , then Conductivity ๏ณ ๏ณ = nc e ๏ญe[hole contribution negligible] So ๏ณ = 5 × 1022๏ด 1.6 ๏ด 10-19๏ด 0.15 ๏-1m-1= 1200 ๏-1m-1 Example (6) Find Debye length in p-type Ge at 300 K if Na = 1014 cm−3. Assume that all acceptors are ionized, ฯต = 16. Solution: LD = 0.48 µm. 9. Calculate the ambipolar di๏ฌusion coe๏ฌcient of intrinsic (un doped) Ge at 300 K. µn/µp = 2.1, µn = 3900 cm2 V−1s−1. Solution: D = 65 cm2/s. 10. Holes are injected into n-type Ge so that at the sample surface โp0 = 1014 cm−3. Calculate โp at the distance of 4 mm from the surface if τp = 10−3 s and Dp = 49 cm2/s. Solution: ๐ซ๐ = ๐ซ๐๐ ๐๐๐ (− ๐ณ √๐ซ๐ ๐๐ ) = ๐. ๐ ๐ ๐๐๐๐ ๐๐−๐ Problem 2.20 The expression for the Bohr radius can also be applied to the hydrogen-like atom consisting of an ionized donor and the electron provided by the donor. Modify the expression for the Bohr radius so that it applies to this hydrogen-like atom. Calculate the resulting radius of an electron orbiting around the ionized donor in silicon. (๐๐ = 11.9 and µe* = 0.26 µ0) Solution The Bohr radius is obtained from: ๐๐ ๐๐ ๐๐ ๐๐ = ๐ ๐๐ ๐๐ However, since the electron travel through silicon one has to replace the permittivity of vacuum with the dielectric constant of silicon and the free electron mass with the effective mass for conductivity calculations so that: ๐๐ ๐๐. ๐ ๐๐ , ๐ ๐๐๐๐ ๐๐ ๐๐๐๐๐๐๐ = ๐๐ ∗ = ๐๐๐ ๐ ๐๐ = ๐. ๐๐ ๐๐ ๐๐ ๐๐ ๐. ๐๐ Example (1) Complete Ionization of the Dopant Atoms In a silicon sample doped with 1017cm–3 of phosphorus atoms, what fraction of the donors are not ionized (i.e., what fraction are occupied by the “extra” electrons)? Solution: First, assume that all the donors are ionized and each donor donates an electron to the conduction band. N = ND = 1017 cm-3 From, previous example, EF is located at 146 meV below Ec. The donor level Ed is located at 45 meV below Ec for phosphorus (see Table). The probability that a donor is not ionized, i.e., the probability that it is occupied by the “extra” electron, according to Eq. ๐(๐ฌ) = ๐ , is : (๐ฌ− ๐ฌ ) ๐+ ๐ ๐ญ ⁄ ๐ฒ๐ป ๐ ๐ท๐๐๐๐๐๐๐๐๐๐ ๐๐ ๐๐๐ − ๐๐๐๐๐๐๐๐๐๐ ≈ = (๐ฌ๐ −๐ฌ๐ )⁄ ๐ฒ๐ป ๐ + ๐⁄๐ ๐ ๐ (๐๐๐−๐๐)๐๐๐ฝ⁄ ๐๐๐๐๐ฝ ๐ = ๐. ๐ % ๐ + ๐⁄๐ (The factor 1/2 in the denominators stems from the complication that a donor atom can hold an electron with upspin or downspin. This increases the probability that donor state occupied by an electron.) Therefore, it is reasonable to assume complete ionization, i.e., n = Nd. Ec ED Ef 45m eV 146 m eV Ev Location of EF and Ed. Not to scale. Part (7) Solved PROBLEMS Effective masses and Fermi distribution Function Problem (1) Consider the general exponential expression for the concentration of electrons in the CB, n= Ncexp −(Ec −EF) /kT, and the mass action law, np = ni2. What happens when the doping level is such that n approaches Nc and exceeds it? Can you still use the above expressions for n and p? Consider an n-type Si that has been heavily doped and the electron concentration in the CB is 1020 cm-3. Where is the Fermi level? Can you use np = ni2 to find the hole concentration? What is its resistivity? How does this compare with a typical metal? What use is such a semiconductor? Solution Consider n = Ncexp[−(Ec − EF)/kT] (1) 2 and np = ni ( 2 ) These expressions have been derived using the Boltzmann tail (E > EF + a few kT) to the Fermi − Dirac (FD) function f(E) as in (in the textbook). Therefore, the expressions are NOT valid when the Fermi level is within a few kT of Ec. In these cases, we need to consider the behavior of the FD function f(E) rather than its tail and the expressions for n and p are complicated. It is helpful to put the 1020 cm-3 doping level into perspective by considering the number of atoms per unit volume (atomic concentration, nSi) ,in the Si crystal: nat = (Density)NA / Mat = (2.33×103 kg m-3)(6.022×1023 mol−1) (28.09 ×10-3 kg mol ) i.e. nat = 4.995 × 1028 m-3 or 4.995 × 1022 cm-3 Given that the electron concentration n = 1020 cm-3 (not necessarily the donor concentration!), we see that n/nat = (1020 cm-3) / (4.995 × 1022 cm-3) = 0.00200 which means that if all donors could be ionized we would need 1 in 500 doping or 0.2% donor doping in the semiconductor (n is not exactly Nd for degenerate semiconductors). We cannot use Equation (1) to find the position of EF. The Fermi level will be in the conduction band. The semiconductor is degenerate (see Figure 5Q7-1). EFn CB EC EC EV VB EV EFp (a) Degenerate n-type semiconductor. Large number of donors form a band that overlaps the CB. (b) Degenerate p-type semiconductor. Drift m O B I L I T y (cm2 V-1 S-1) 2000 1000 100 50 1015 1016 1017 1018 1019 1020 Dopant concentration (cm-3) The variation of the drift mobility with dopant concentration in Si for electrons and holes at 300 K. Take T = 300 K, and µe ≈ 900 cm2 V-1 s-1 from Figure. The resistivity is ρ = 1/(en µe) = 1/[(1.602 × 10-19 C)(1020 cm-3)(900 cm2 V-1 s-1)] ∴ ρ = 6.94 × 10-5 โฆ cm or 694 × 10-7 โฆ m Compare this with a metal alloy such as nichrome which has ρ = 1000 nโฆ m = 10 × 10-7 โฆ m. The difference is only about a factor of 70. This degenerate semiconductor behaves almost like a “metal”. Heavily doped degenerate semiconductors are used in various MOS (metal- oxide- semiconductor) devices where they serve as the gate electrode (substituting for a metal) or interconnect lines. Problem (2) Gold in Si has two energy levels in the band gap: EC - EA = 0.54 eV, ED – EF = 0.29 eV. Assume the third level ED– EF = 0.35 eV is inactive. (a) What will be the state of charge of the gold levels in Si doped with high concentration of boron atoms? Why? (b) What is the effect of gold on electron and hole concentrations? Problem (3) For an n-type silicon sample doped with 2.86x 10l6cm-3 phosphorous atoms, find the ratio of the neutral to ionized donors at 300 K. (EC - ED) = 0.045 eV. Example (9) Show that ๐ฌ๐ญ − ๐ฌ๐ซ −๐ = ๐ต๐ซ [๐ + ๐ ๐๐๐ ( )] ๐ฒ๐ป [Hint: The probability of occupancy is ๐ ๐ฌ − ๐ฌ๐ญ −๐ ๐ญ (๐ฌ) = [๐ + ๐๐๐ ( )] ๐ ๐ฒ๐ป where h is the number of electrons that can physically occupy the level E, and g is the number of electrons that can be accepted by the level, also called the ground-state degeneracy of the donor impurity level (g = 2).] ๐ต+ ๐ซ Pr0blem (7) 1. (a) Derive an expression for the total number of states in a semiconductor material (per unit volume) between Ec and Ec + kT, where Ec is the conduction band edge (bottom of the conduction band), k is Boltzmann’s constant and T is the temperature. by integrating the density of states over the energy range given in this problem. Solution: The density of states represents the number of states per unit volume. For this problem, we simply need to integrate the density of states, g(E) ๐ ๐ ๐๐∗ ๐(๐ฌ) = ( ) ๐ ๐ ๐ ๐๐ ๐⁄ ๐ √๐ฌ − ๐ฌ๐ From EC to EC + KT ๐ฌ๐ +๐ฒ๐ป ∫ ๐ฌ๐ ๐ ๐ ๐∗๐ ๐๐ (๐ฌ) ๐ ๐ฌ = ( ) ๐ ๐ ๐ ๐๐ ๐ ๐ ๐∗๐ = ( ) ๐ ๐ ๐ ๐๐ ๐⁄ ๐ ๐ ๐ ๐∗๐ = ( ) ๐ ๐ ๐ ๐๐ ๐⁄ ๐ ๐ฌ๐ +๐ฒ๐ป ๐ฌ๐ ๐ฒ๐ป ∫ ๐ ๐⁄ ๐ ๐ ๐ ๐ ๐⁄ ๐๐ ๐ (๐ฒ๐ป) ๐⁄ ๐ ๐⁄ ๐ ๐ ๐ ๐๐∗ ๐ฒ๐ป = ( ) ๐ ๐ ๐ ๐๐ ๐๐∗ = ( ) ๐๐ ๐⁄ ๐ ๐⁄ ๐ (๐ฌ − ๐ฌ๐ ) ∫ ๐⁄ ๐ ๐ ๐ ๐∗๐ ๐ฒ๐ป ๐ ( ) ๐ ๐ ๐ ๐๐ ๐ ๐ฌ For values of, mo = 9.11 x 10-31 kg , KT = 0.026 x 1.6 x 1o-19 J, h = 1.05 x 10-34 J.s we find: ๐ฌ๐ +๐ฒ๐ป ∫ ๐๐ (๐ฌ) ๐ ๐ฌ = ๐. ๐๐ ๐ ๐๐๐๐ ๐−๐ = ๐. ๐๐ ๐ ๐๐๐๐ ๐๐−๐ ๐ฌ๐ (b) Evaluate the expression you derived in (a) for GaAs and Si. Solution: For GaAs, using me=0.067 m0, we ๏ฌnd 3.41×1017 cm−3. For Si, using me=1.08 m0, we ๏ฌnd 2.21×1019 cm−3. Example (3) Silicon crystal is doped with 5 x 1020/m3 atoms per m3 . The donor level is 0.05 eV from the edge of the conduction band. Taking the band gap to be 1.12 eV, calculate the position of the Fermi level at 200 K. Solution The intrinsic carrier concentration can be obtained from the known carrier concentration in Si at 300 K. As the carrier concentration at 300K is 1.5x1016/m3, the carrier concentration at 200 K is ๐ ๐๐๐ ⁄๐ ( ) ๐ ๐. ๐ ๐ ๐๐๐๐ = ๐. ๐๐ ๐ ๐๐๐๐ /๐ฆ๐ ๐๐๐ As the doping concentration is much larger than ni. we can take, ๐ ≈ ๐ต๐ซ = ๐ ๐ ๐๐๐๐ /๐๐ , ๐๐๐๐ ๐ฌ๐๐ญ − ๐ฌ๐๐ญ = ๐ฒ๐ป ๐๐ ๐⁄๐๐ = ๐. ๐๐๐ ๐๐ฝ Exercise (4) Germanium has ionized acceptor density of๐ ๐ ๐๐๐๐ /๐๐ and donor density of ๐ ๐ ๐๐๐๐ /๐๐ .Taking the band gap to be 0.67 eV, calculate the equilibrium density of majority and minority carriers at 450 K and also the Fermi energy. [Hint: Using the intrinsic concentration at 300 K, find ni at 450 K and use the expression for n] Ans, n = 2.02 x 1021/m3, p = 9.62 x 1017/m3, ๐ฌ๐๐ญ − ๐ฌ๐๐ญ = ๐. ๐๐๐ ๐๐ฝ Problem (5) 2. Consider a silicon crystal whose band gap energy is Eg =1.12 eV and whose temperature is kept at T=300โฆK. (a) If the Fermi level, Ef, is located in the middle of the band gap, what is the probability of ๏ฌnding an electron (or equivalently, the probability of a state being occupied) at E = Ec + kT. Solution: The probability is given by the Fermi-Dirac function. Since Ef = Ec−Eg/2, ๐ ๐(๐ฌ) = ๐ฌ (๐ฌ − ๐ฌ๐ + ๐⁄๐) ⁄ ]+๐ ๐๐๐ [ ๐ฒ๐ป As E = EC + KT , we find : ๐ (๐ฌ๐ + ๐ฒ๐ป) = = ๐ ๐ฌ (๐ฒ๐ป + ๐⁄๐) ⁄ ]+๐ ๐๐๐ [ ๐ฒ๐ป ๐ = ๐๐๐ (−๐๐. ๐) (๐. ๐๐๐ + ๐. ๐๐)⁄ ๐๐๐ ( ๐. ๐๐๐) + ๐ ≅ ๐. ๐๐ ๐ ๐๐−๐๐ (b) If the Fermi level, Ef is located at the conduction band edge, EF = Ec, what the probability of ๏ฌnding an electron at E = Ec + kT. Solution: The probability is given by evaluating the FermiDirac probability density, with Ef = Ec ๐ ๐ญ(๐ฌ) = (๐ฌ − ๐ฌ๐ )⁄ ๐๐๐ [ ๐ฒ๐ป] + ๐ With E = Ec + kT we ๏ฌnd, ๐ ๐ญ (๐ฌ๐ + ๐ฒ๐ป) = ≅ ๐. ๐๐ ๐๐๐ (๐) + ๐ Problem (6) The equilibrium electron concentration is given by the product of the density of states and the probability function, n(E) = gc (E) F(E). If E −EF>> kT, the Fermi-Dirac probability function can be approximated with the Maxwell-Boltzmann function ๐ (๐ฌ − ๐ฌ๐ญ )⁄ ๐(๐ฌ) = ≅ ๐๐๐ [− ๐ฒ๐ป] (๐ฌ − ๐ฌ๐ญ )⁄ ๐๐๐ [ ๐ฒ๐ป] + ๐ (a) Using this approximation, ๏ฌnd the energy relative to the conduction band edge, E−Ec, at which the electron concentration becomes maximum. Solution: The electron density, n(E) = g(E)f(E), can be written in the form ๐ (๐) = ๐๐๐๐๐๐๐๐ ๐ √๐ ๐๐๐ (−๐) Where x = (E−Ec)/kT, for purposes of ๏ฌnding the maxima. Taking the derivative and setting equal to zero ๐ ๐ (๐) ๐ = ๐๐๐๐๐๐๐๐ ๐ ( − √๐) ๐๐๐ (−๐) = ๐ ๐ ๐ ๐√๐ We ๏ฌnd that the distribution peaks at E −Ec = kT/2. (b) Using this approximation, calculate the electron concentration per unit energy interval (in units of cm−3 eV−1) in silicon at energy E = Ec −kT. Assume the Fermi level is located at the center of the band gap, EF = Ec −Eg/2. Solution: We want to evaluate ๐ (๐ฌ) = ๐(๐ฌ)๐(๐ฌ) ๐ ๐ ๐๐∗ = ( ) ๐ ๐ ๐ ๐๐ ๐⁄ ๐ ( ) √(๐ฌ − ๐ฌ๐ )๐๐๐ [− ๐ฌ − ๐ฌ๐ญ ⁄๐ฒ๐ป] at E = Ec + kT for Ef = εg/2. The result is n(Ec + kT) = g(E)f(E) ๐ (๐ฌ) = ๐(๐ฌ)๐(๐ฌ) = ๐ ๐ ๐ ๐∗๐ ⁄๐ ( ) √๐ฒ๐ป ๐ ๐ ๐ ๐๐ ( ๐ฒ๐ป + ๐๐๐ [− ๐ฌ๐ ⁄ ) ๐⁄ ๐ฒ๐ป] ๐ (๐ฌ) = ๐(๐ฌ)๐(๐ฌ) ๐ ๐ ๐ ๐๐∗ ⁄๐ ( ) = ( ๐ ) √๐. ๐๐๐ ๐๐๐ [− ๐. ๐๐๐ + ๐. ๐๐ ⁄๐. ๐๐๐] ๐ ๐๐ ๐ = ๐. ๐๐ ๐ ๐๐๐๐ ๐๐−๐ ๐๐ฝ−๐ Repeat the calculation in (b) without using the approximation. Solution: The answer is really close, to within a part in roughly 10−10. Problem (7) If a silicon sample is doped with 1016 phosphorous impurities/cm3, find the ionized donor density at 77 K. Assume that the ionization energy for phosphorous donor impurities and the electron effective mass are independent of temperature. (Hint: First select a N+D value to calculate the Fermi level, then find the corresponding N+D . If they don’t agree, select another N+D value and repeat the process until a consistent N+D is obtained.) Problem (8) Using graphic method to determine the Fermi level for a boron-doped silicon sample with an impurity concentration of 1015 cm-3 at 300 K (note ni = 9.65x104 crn-3). Problem (9) The Fermi-Dirac distribution function is given by ๐ ๐ (๐ฌ) = (๐ฌ − ๐ฌ๐ญ )⁄ ๐ + ๐๐๐ ๐ฒ๐ป The differentiation of F(E) with respect to energy is F’(E). ๐ Find the width of F’(E), i.e., ๐ [๐ฌ (๐๐ ๐ญ๐๐๐ ) − ๐ฌ (๐๐ ๐ญ๐๐๐ )], ๐ where ๐ญ๐๐๐ is the maximum value of F‘(E). Problem (10) Find the position of the Fermi level with respect to the bottom of the conduction band (Ec– EF) for a silicon sample at 300 K, which is doped with 2x 1010cm-3 fully ionized donors. Problem (11) The Gamma Function is defined as ๐ ๐ช(๐) = ∫ ๐๐−๐ ๐๐๐ (−๐) ๐ ๐ ๐ (a) Find ๐ช(1/2), and (b) show that ๐ช(n) = (n - I)๐ช(n - I). Example 1.5 Calculate the energy relative to the Fermi energy for which the Fermi function equals 5%. Write the answer in units of kT. Solution: The problems states that ๐ (๐ฌ) = ๐ ๐ฌ− ๐ฌ๐ญ = ๐. ๐๐ ๐ + ๐๐๐ ( ) ๐ฒ๐ป Which can be solved yielding? ๐ฌ − ๐ฌ๐ญ = ๐๐ (๐๐) ๐ฒ๐ป = ๐ ๐ฒ๐ป Problem 1.9 Prove that the probability of occupying an energy level below the Fermi energy equals the probability that an energy level above the Fermi energy and equally far away from the Fermi energy is not occupied. Solution The probability that an energy level with energy โE below the Fermi energy EF is occupied can be rewritten as: ๐ซ๐ฌ ๐๐๐ ๐ ๐ฒ๐ป ๐(๐ฌ๐ญ − ๐ซ ๐ฌ) = ๐ฌ๐ญ − ๐ซ๐ฌ− ๐ฌ๐ญ = ๐ซ๐ฌ ๐ + ๐๐๐ ๐๐๐ +๐ ๐ฒ๐ป ๐ฒ๐ป ๐ ๐ =๐− = ๐ − ๐ซ๐ฌ ๐ฌ +๐ซ๐ฌ− ๐ฌ๐ญ ๐๐๐ +๐ ๐ + ๐๐๐ ๐ญ ๐ฒ๐ป ๐ฒ๐ป ( ) = ๐ − ๐ ๐ฌ๐ญ + ๐ซ ๐ฌ so that it also equals the probability that an energy level with energy โE above the Fermi energy, EF, is not occupied. Problem 2.3 Prove that the probability of occupying an energy level below the Fermi energy equals the probability that an energy level above the Fermi energy and equally far away from the Fermi energy is not occupied. Solution The probability that an energy level with energy โE below the Fermi energy EF is occupied can be rewritten as โ๐ฌ ๐๐๐ ๐ ๐ฒ๐ป ๐ (๐ฌ๐ญ โ๐ฌ) = = ๐ฌ๐ญ − โ๐ฌ− ๐ฌ๐ญ โ๐ฌ ๐ + ๐๐๐ ๐๐๐ +๐ ๐ฒ๐ป ๐ฒ๐ป ๐ ๐ ( ) =๐− = ๐ − โ๐ฌ ๐ฌ๐ญ − โ๐ฌ− ๐ฌ๐ญ = ๐ − ๐ ๐ฌ๐ญ + โ ๐ฌ ๐๐๐ +๐ ๐ + ๐๐๐ ๐ฒ๐ป ๐ฒ๐ป so that it also equals the probability that an energy level with energy โE above the Fermi energy, EF, is not occupied. Problem 2.4 At what energy (in units of kT) is the Fermi function within 1 % of the Maxwell-Boltzmann distribution function? What is the corresponding probability of occupancy? Solution The Fermi function can be approximated by the MaxwellBoltzmann distribution function with an approximate error of 1 % if ๐๐๐ฉ − ๐๐ญ๐ฉ ๐ ๐. ๐๐ = ๐. ๐๐ ๐๐ = ๐๐ญ๐ซ ๐๐ญ๐ซ ๐๐๐ฉ using x = (E - EF)/kT, this condition can be rewritten as: 1 + exp (x) = 1.01 exp(x) from which one finds x = ln(100) = 4.605 so that E = EF + 4.605 kT and fFD(EF + 4.605 kT) = 0.0099 Problem 2.5 Calculate the Fermi function at 6.5 eV if EF = 6.25 eV and T = 300 K. Repeat at T = 950 K assuming that the Fermi energy does not change. At what temperature does the probability that an energy level at E = 5.95 eV is empty equal 1 %. Solution The Fermi function at 300 K equals: ๐ ๐(๐. ๐๐ ๐๐ฝ) = = ๐. ๐๐ ๐ ๐๐−๐ ๐.๐−๐.๐๐ ๐ + ๐๐๐ ( ) ๐.๐๐๐๐ The Fermi function at 950 K equals: ๐ ๐(๐. ๐๐ ๐๐ฝ) = = ๐. ๐๐๐ ๐.๐−๐.๐๐ ๐ + ๐๐๐ ( ) ๐.๐๐๐๐ The probability that the Fermi function equals 1 % implies: ๐ ๐(๐. ๐๐ ๐๐ฝ) = ๐. ๐๐ = ๐.๐๐−๐.๐๐ ๐ + ๐๐๐ ( ๐ฒ๐ป ) ⁄๐ resulting in ๐ป= ๐. ๐ ๐๐ ( ๐ ๐.๐๐ ๐ ๐ฒ − ๐) = ๐๐๐. ๐ ๐๐ช Example 2.7 A piece of germanium doped with 1016 cm-3 shallow donors is illuminated with light generating 1015 cm-3 excess electrons and holes. Calculate the quasi-Fermi energies relative to the intrinsic energy and compare it to the Fermi energy in the absence of illumination. Solution The carrier densities when illuminating the semiconductor are: ๐ = ๐๐ + ๐ ๐ = ๐๐๐๐ + ๐๐๐๐ = ๐. ๐ ๐ ๐๐๐๐ ๐๐−๐ ๐ = ๐๐ + ๐ ๐ = ๐๐๐๐ ๐๐−๐ and the quasi-Fermi energies are: ๐ ๐๐. ๐ ๐ ๐๐๐๐ ๐ญ๐ − ๐ฌ๐ = ๐ฒ๐ป ๐๐ = ๐. ๐๐๐๐ ๐ ๐๐ = ๐๐๐ ๐๐๐ฝ ๐๐ ๐ ๐ ๐๐๐๐ ๐ ๐ ๐ ๐๐๐๐ ๐ญ๐ − ๐ฌ๐ = ๐ฒ๐ป ๐๐ = ๐. ๐๐๐๐ ๐ ๐๐ = ๐๐๐ ๐๐๐ฝ ๐๐ ๐ ๐ ๐๐๐๐ In comparison, the Fermi energy in the absence of light equals ๐๐ ๐๐๐๐ ๐ญ๐ญ − ๐ฌ๐ = ๐ฒ๐ป ๐๐ = ๐. ๐๐๐๐ ๐ ๐๐ = ๐๐๐ ๐๐๐ฝ ๐๐ ๐ ๐ ๐๐๐๐ which is very close to the quasi-Fermi energy of the majority carriers. Problem 2.8 Calculate the position of the intrinsic energy level relative to the midgap energy Emid gap = (Ec + Ev)/2 in germanium, silicon and gallium arsenide at 300 K. Repeat at T = 100 °C. Solution: The intrinsic energy level relative to the midgap energy is obtained from: ๐ ๐๐∗ ๐ฌ๐ = ๐ฌ๐๐๐ ๐๐๐ = ๐ฒ๐ป ๐๐ ∗ ๐ ๐๐ where the effective masses are the effective masses for density of states calculations as listed in the table below. The corresponding values of the intrinsic level relative to the midgap energy are listed as well. 45.92 meV me*/m0 mh*/m0 T = 300 K T = 100 C Germanium 0.55 0.37 7.68 meV 9.56 meV Silicon 1.08 0.81 5.58 meV 6.94 meV Gallium arsenide 0.067 0.45 36.91 meV 45.92 meV Problem 2.9 Calculate the electron and hole density in germanium, silicon and gallium arsenide if the Fermi energy is 0.3 eV above the intrinsic energy level. Repeat if the Fermi energy is 0.3 eV below the conduction band edge. Assume that T = 300 K. Solution The electron density, n, can be calculated from the Fermi energy using: ๐ฌ๐ญ − ๐ฌ๐ ๐. ๐ ๐ = ๐๐ ๐๐๐ = ๐๐ ๐๐๐ ( ) ๐ฒ๐ป ๐. ๐๐๐๐ and the corresponding hole density equals ๐๐๐ ๐= ๐ the resulting values are listed in the table below. If the Fermi energy is 0.3 eV below the conduction band edge, one obtains the carrier densities using: ๐ฌ๐ญ − ๐ฌ๐ ๐. ๐ ๐ = ๐ต๐ ๐๐๐ = ๐ต๐ ๐๐๐ ( ) ๐ฒ๐ป ๐. ๐๐๐๐ and the corresponding hole density equals: ๐๐๐ ๐= ๐ the resulting values are listed in the table below. Germanium Silicon Gallium Arsenide EF - Ei = 0.3 eV EF - Ei = - 0.3 eV ni (cm-3) Nc (cm-3) n (cmp (cm-3) n (cm-3) p (cm-3) 2.03 x 1013 1.02 x 1019 2.24 x 1018 1.48 x 108 9.27 x 1013 4.45 x 1012 1.45 x 1010 6.62 x 1019 1.60 x 1015 1.32 x 105 6.02 x 1014 3.50 x 105 2.03 x 106 4.37 x 1017 2.23 x 1011 18.4 3.97 x 1012 1.04 Problem 2.10 The equations ๐ − ๐ต+ ๐ต+ − ๐ต− ๐ ๐ − ๐ต๐ ๐ ๐๐ = + √( ) + ๐๐๐ ๐ ๐ ๐ ๐ต๐− − ๐ต+ ๐ต๐− − ๐ต+ ๐ ๐ ๐๐ = + √( ) + ๐๐๐ ๐ ๐ are only valid for non-degenerate semiconductors (i.e. Ev + 3kT < EF<Ec - 3kT). Where exactly in the derivation was the assumption made that the semiconductor is nondegenerate? Solution The above two Equations were derived using charge neutrality and the mass action law. Of those two assumptions, the use of the mass action law implies that the semiconductor is nondegenerate. The mass action law was ∞ (๐ฌ๐ญ −๐ฌ) (๐ฌ๐ญ −๐ฌ๐ ) ๐ ๐ √๐ ∗๐⁄๐ ๐ฒ๐ป ๐๐ ≅ ∫ ๐๐ √๐ฌ − ๐ฌ๐ ๐ ๐ ๐ฌ = ๐ต๐ ๐ ๐ฒ๐ป ๐ ๐ ๐ฌ๐ ๐ ๐ ๐ ๐∗๐ ๐ฒ๐ป ⁄๐ ๐ต๐ = ๐ ( ) ๐๐ These equations, representing a closed form solution for the thermal equilibrium carrier densities as a function of the Fermi energy, were in turn obtained by solving the Fermi integral and assuming that: Ev + 3kT < EF<Ec - 3kT i.e. that the Fermi energy must be at least 3kT away from either bandedge and within the bandgap. Problem 2.31 Find the equilibrium electron and hole concentrations and the location of the Fermi energy relative to the intrinsic energy in silicon at 27 oC, if the silicon contains the following concentrations of shallow dopants. a) 1 x 1016 cm-3 boron atoms b) 3 x 1016 cm-3 arsenic atoms and 2.9 x 1016 cm-3 boron atoms. Solution a) Boron atoms are acceptors, therefore Na = 1016 cm-3 Since these are shallow acceptors and the material is not compensated, degenerate or close to intrinsic, the hole density equals the acceptor density: p ≈ 1016 cm-3 Using the mass action law we then find the electron density n = n2i/p = 1 x 104 cm-3 The Fermi energy is then obtained from: ๐ ๐๐๐ ๐ฌ๐ญ − ๐ฌ๐ = ๐ฒ๐ป ๐๐ = ๐. ๐๐๐๐ ๐๐ = −๐๐๐ ๐๐๐ฝ ๐๐ ๐๐๐๐ b) Arsenic atoms are donors, therefore Na = 2.9 x 1016 cm-3 and Nd = 3 x 1016 cm-3 Since these are shallow acceptors and the material is not degenerate or close to intrinsic, the electron density approximately equals the difference between the donor and acceptor density n ≈ Nd – Na = 1015 cm-3 Using the mass action law we then find the hole density p = n2i/n = 1 x 105 cm-3 The Fermi energy is then obtained from: ๐ ๐๐๐๐ ๐ฌ๐ญ − ๐ฌ๐ = ๐ฒ๐ป ๐๐ = ๐. ๐๐๐๐ ๐๐ = ๐๐๐ ๐๐๐ฝ ๐๐ ๐๐๐๐ Example (2) 1–2 Oxygen Concentration versus Altitude , We all know that there is less oxygen in the air at higher altitudes. What is the ratio of the oxygen concentration at 10 km above sea level, Nh, to the concentration at sea level, N0, assuming a constant temperature of 0°C? SOLUTION: There are fewer oxygen molecules at higher altitudes because the gravitational potential energy of an oxygen molecule at the higher altitude, Eh, is larger than at sea level, E0. According to Equation −(๐ฌ− ๐ฌ๐ญ )⁄ ๐ฒ๐ป ๐(๐ฌ) ≈ ๐ ๐ฌ − ๐⁄๐ฒ๐ป ๐ ๐ฌ − ๐ฌ๐⁄ ๐ต๐ −( ๐ ๐ฒ๐ป) = = ๐ ๐ฌ ๐ ๐ต๐ ๐− ⁄๐ฒ๐ป E0 –Eh is the potential energy difference, i.e., the energy needed to lift an oxygen molecule from sea level to 10 km. Eh E0= altitude x weight of O2 molecule x acceleration of gravity = 104 m x O2 molecular weight atomic mass unit x 9.8 m s-2 = 104 m x 32 x1.66 x1027 kgx 9.8 m s-2= 5.2 x 10-21 J − ๐.๐ ๐ ๐๐๐๐⁄ ๐ต๐ ๐.๐๐ ๐ ๐๐−๐๐ ๐ฑ. ๐ฒ−๐ ๐ ๐๐๐ ๐ฒ = ๐−๐.๐๐ = ๐. ๐๐ ∴ = ๐ ๐ต๐ Therefore, the oxygen concentration at 10 km is 25% of the sea level concentration. This example and the sand-in-a-dish analogy presented to demystify the concept of equilibrium, and to emphasize that each electron energy state has a probability occupied that governed by the Fermi function. Example (3) Finding the Fermi Level in Si Where is EF located in the energy band of silicon, at 300K with n = 1017cm–3? In addition, for p = 1014cm–3? Solution: From Eq. −(๐ฌ๐ −๐ฌ๐ญ )⁄ ๐ฒ๐ป ๐ = ๐ต๐ ๐ ๐ฌ๐ − ๐ฌ๐ = ๐ฒ๐ป ๐๐ ( ๐ต๐⁄ ๐) ๐๐ = ๐. ๐๐๐ ๐๐ (๐. ๐ ๐ ๐๐ ⁄ ๐๐ ) = ๐. ๐๐๐ ๐๐ฝ ๐๐ Therefore, EF is located at 146 meV below Ec, as shown in Figure. For p = 1014cm–3, from Equation, ๐ต ๐ฌ๐ญ − ๐ฌ๐ = ๐ฒ๐ป ๐๐ ( ๐⁄๐) ๐๐ = ๐. ๐๐๐ ๐๐ (๐. ๐ ๐ ๐๐ ⁄ ๐๐ ) = ๐. ๐๐ ๐๐ฝ ๐๐ Therefore, EF is located at 0.31 eV above Ev. 0.146 EF Ec EF 0.31 Ev Example (1) Complete Ionization of the Dopant Atoms In a silicon sample doped with 1017cm–3 of phosphorus atoms, what fraction of the donors are not ionized (i.e., what fraction are occupied by the “extra” electrons)? Solution: First, assume that all the donors are ionized and each donor donates an electron to the conduction band. N = ND = 1017 cm-3 From, previous example, EF is located at 146 meV below Ec. The donor level Ed is located at 45 meV below Ec for phosphorus (see Table). The probability that a donor is not ionized, i.e., the probability that it is occupied by the “extra” electron, according to Eq. ๐(๐ฌ) = ๐ , is : (๐ฌ− ๐ฌ ) ๐+ ๐ ๐ญ ⁄ ๐ฒ๐ป ๐ท๐๐๐๐๐๐๐๐๐๐ ๐๐ ๐๐๐ − ๐๐๐๐๐๐๐๐๐๐ ≈ (๐ฌ๐ −๐ฌ๐ )⁄ ๐ฒ๐ป ๐ + ๐⁄๐ ๐ ๐ = ๐ = ๐. ๐ % (๐๐๐−๐๐)๐๐๐ฝ⁄ ๐ ๐๐๐๐๐ฝ ๐ + ⁄๐ ๐ (The factor 1/2 in the denominators stems from the complication that a donor atom can hold an electron with upspin or downspin. This increases the probability that donor state occupied by an electron.) Therefore, it is reasonable to assume complete ionization, i.e., n = Nd. Ec ED Ef 45m eV 146 m eV Ev Location of EF and Ed. Not to scale. Part (8) Solved PROBLEMS Energy: Density of States Example 2.3 Calculate the number of states per unit energy in a 100 by 100 by 10 nm piece of silicon (m* = 1.08 m0) 100 meV above the conduction band edge. Write the result in units of eV-1. Solution The density of states equals: ๐ ๐ √๐ ∗๐⁄ ๐(๐ฌ) = ๐ ๐ √๐ฌ − ๐ฌ๐ ๐๐ ๐ ๐ ๐ √๐(๐. ๐๐ ๐ ๐. ๐๐ ๐๐−๐๐ ) ⁄๐ √๐. ๐ ๐ ๐. ๐ ๐ ๐๐−๐๐ = − ๐๐ ๐ (๐. ๐๐๐ ๐ ๐๐ ) = ๐. ๐๐ ๐ ๐๐๐๐ ๐−๐ ๐ฑ−๐ So that the total number of states per unit energy equals ๐ (๐ฌ) ๐ฝ = ๐. ๐๐ ๐ ๐๐๐๐ ๐ ๐๐−๐๐ ๐ฑ−๐ = ๐. ๐๐ ๐ ๐๐๐ ๐๐ฝ−๐ Example (7) Derive the density of states in the conduction band as given by Eq. ๐ต ๐⁄ √๐ ๐๐ ๐๐ (๐ฌ − (๐ฌ)๐ด๐ ๐ ๐ ๐๐ ๐ฌ๐ ) ๐⁄ ๐ (Hint: The wavelength ส of a standing wave is related to the length of the semiconductor L by vส = nx where nx is an integer. The wavelength can be expressed by de Broglie hypothesis ส = h/px. Consider a three-dimensional cube of side L) Example (8) 10. Calculate the average kinetic energy of electrons in the conduction band of an n-type non- degenerate semiconductor. The density of states is given by Eq. ๐ต ๐⁄ √๐ ๐๐ ๐๐ (๐ฌ − (๐ฌ)๐ด๐ ๐ ๐ ๐๐ Exercise (1 ) Derive the expression. ๐ฌ๐ ) ๐⁄ ๐ ๐ (๐ฌ๐ − ๐ฌ๐๐ญ )⁄ ๐ ๐ ๐๐ ๐ฒ๐ป ⁄๐ (๐ฌ๐− ๐ฌ๐ญ)⁄ ๐ฒ๐ป ๐ฒ๐ป ๐= ( ) ๐ = ๐ต๐ ๐ ๐ ๐ ๐๐ For an intrinsic semiconductor the number of electrons in the conduction band is equal to the number of holes in the valence band since a hole is left in the valence band only when an electron makes a transition to the conduction band, n=p Using this and assuming that the effective masses of the electrons and holes are the same one gets, (๐ฌ๐ญ − ๐ฌ๐ )⁄ ๐๐ป ๐ = (๐ฌ๐ − ๐ฌ๐ญ )⁄ ๐๐ป ๐ Conduction Band Energy EC Fermi Level EV Valance Band Giving : ๐ฌ๐ช + ๐ฌ๐ฝ (๐ช) ๐ i.e. the Fermi level lies in the middle of the forbidden gap. Note that there is no contradiction with the fact that no state exists in the gap as is only an energy level and not a state. By substituting the above expression for Fermi energy in(A) or (B), ๐ฌ๐ญ = ๐ ๐ ๐๐ ๐ฒ๐ป ๐= ( ) ๐ ๐ ๐๐ ๐⁄ ๐ (๐ฌ๐ญ − ๐ฌ๐ช )⁄ ๐ฒ๐ป ๐ (๐ฌ๐ญ − ๐ฌ๐ )⁄ ๐ฒ๐ป = ๐ต๐ช ๐ (๐จ) ๐ ๐ ๐๐ ๐ฒ๐ป ๐= ( ) ๐ ๐ ๐๐ ๐⁄ ๐ (๐ฌ๐ − ๐ฌ๐ญ )⁄ ๐ฒ๐ป ๐ = (๐ฌ๐ − ๐ฌ๐๐ญ )⁄ ๐ฒ๐ป ๐ต๐ ๐ (๐ฉ) We obtain an expression for the number density of electrons or holes (n = p = ni) ๐ ๐ ๐ ๐ฒ๐ป ⁄๐ ๐⁄ −๐ซ ๐ ๐ ⁄๐ ๐ฒ๐ป ( ) ๐๐ = ( ) ๐ ๐ ๐ ๐ ๐ ๐ ๐๐ Where Δ is the width of the gap (๐ซ) Example 2.4 Calculate the effective densities of states in the conduction and valence bands of germanium, silicon and gallium arsenide at 300 K. Solution The effective density of states in the conduction band of germanium equals: ๐ ๐ ๐๐∗ ๐ฒ๐ป ๐ต๐ = ๐ ( ) ๐๐ ๐⁄ ๐ −๐๐ −๐๐ ๐⁄ ๐ ๐ ๐ ๐ ๐. ๐๐ ๐ ๐. ๐๐ ๐ ๐๐ ๐ ๐. ๐๐ ๐ ๐๐ ๐ ๐๐๐ =๐ ( ) (๐. ๐๐๐ ๐ ๐๐−๐๐ )๐ = ๐. ๐๐ ๐ ๐๐๐๐ ๐−๐ = ๐. ๐๐ ๐ ๐๐๐๐ ๐๐−๐ where the effective mass for density of states was. Similarly, one finds the effective density of states in the conduction band for other semiconductors and the effective density of states in the valence band: -3 Nc (cm ) Nv (cm-3) Germanium 1.02 x 1019 5.64 x 1018 Silicon 2.81 x 1019 1.83 x 1019 Gallium Arsenide 4.35 x 1017 7.57 x 1018 Note that the effective density of states is temperature dependent and can be obtain from: ๐ ๐ป ⁄๐ ๐ต๐ (๐ป) = ๐ต๐ (๐๐๐๐ฒ) ( ) ๐๐๐ where Nc(300 K) is the effective density of states at 300 K. Part (9) Solved PROBLEMS Compounds Problem (1) Consider the GaAs crystal at 300 K. a. Calculate the intrinsic conductivity and resistivity. b. In a sample containing only 1015 cm-3 ionized donors, where is the Fermi level? What is the conductivity of the sample? c. In a sample containing 1015 cm-3 ionized donors and 9 × 1014 cm-3 ionized acceptors, what is the free hole concentration? Solution: a - Given temperature, T = 300 K, and intrinsic GaAs. From Tables, ni = 1.8 × 106 cm-3, µe ≈ 8500 cm2 V-1 s-1 and µh ≈ 400 cm2 V-1 s-1. Thus, σ = eni( µe + µh) ∴σ = (1.602 × 10-19 C)(1.8 × 106 cm-3)(8500 cm2 V-1 s-1 + 400 cm2 V-1 s-1) ∴σ = 2.57 × 10-9โฆ-1 cm-1 ∴ρ = 1/ σ = 3.89 × 108โฆ cm B - Donors are now introduced. At room temperature, n = Nd = 1015 cm-3>>ni>> p. σ n = eNdµe≈(1.602 ×10-19 C)(1015 cm-3)(8500 cm2 V-1 s-1) = 1.36 โฆ-1 cm1 ∴ρn = 1/ σn = 0.735 โฆ cm In the intrinsic sample, EF = EFi, ni = Ncexp[−(Ec − EFi)/kT] (1) In the doped sample, n = Nd, EF = E=, n = Nd = Ncexp[−(Ec − EFn)/kT] (2) Eqn. (2) divided by Eqn. (1) gives, Nd/ni = exp (EFn − EFi)/ kT ( 3 ) ∴โEF = EFn − EFi = kT ln(Nd/ni) (4) Substituting we find, โEF = (8.617 × 10-5 eV/K)(300 K)ln[(1015 cm-3)/(1.8 × 106 cm-3)] ∴โEF = 0.521 eV above EFi (intrinsic Fermi level) c The sample is further doped with Na = 9 × 1014 cm-3 = 0.9 × 1015 cm-3 acceptors. Due to compensation, the net effect is still an n-type semiconductor but with an electron concentration given by, n = Nd − Na = 1015 cm-3 − 0.9 × 1015 cm-3 = 1 × 1014 cm-3 (>>ni) The sample is still n-type though there are less electrons than before due to the compensation effect. From the mass action law, the hole concentration is: p = ni2 / n = (1.8 × 106 cm-3)2 / (1 × 1014 cm-3) = 0.0324 cm-3 On average there are virtually no holes in 1 cm3 of sample. We can also calculate the new conductivity. We note that electron scattering now occurs from Na + Nd number of ionized centers though we will assume that µe ≈ 8500 cm2 V-1 s-1. σ = en µe≈ (1.602 × 10-19 C)(1014 cm-3)(8500 cm2 V-1 s-1) = 0.136 โฆ-1 cm-1 Problem (2) AlN and GaSb are compounds, solid at room temperature. On the basis of bonding considerations and data provided in the periodic table, attempt to predict differences in the properties of these solids. Solution Both compounds are of the III–V family, which hybridize and form “adamantine” (diamond–like) structures which places them into the category of semiconductor. AlN ΔEN = 1.43. The covalent radii of the constituents are small and, combined with the large EN, the bonds (polar covalence’s) are very strong – the semiconductor is expected to exhibit a large band gap (likely transparent). GaSb ΔEN = 0.24. The covalent radii of both constituents are significantly larger (than those of AlN), the ionic contribution to bonding is small – the semiconductor is expected to exhibit a much smaller band gap than AlN. AlN: Eg = 3.8 eV ,GaSb: Eg = 0.8 eV Problem (4) Calculate thermal velocity of electrons and holes in GaAs at room temperature. E๏ฌective masses are m∗e/m0 = 0.063 and m∗h/m0 = 0.53. Solution: ๐๐ = ∗ ๐ ∞ ∫๐ ๐ ๐๐๐ (− ๐ ๐ ⁄๐๐ฒ๐ป) ๐ ๐ ๐ ∞ ∫๐ ๐๐ฒ๐ป √ = ∗ ๐ ๐ ๐∗ ๐๐๐ (− ๐ ๐ ⁄๐๐ฒ๐ป) ๐ ๐ ๐ Thermal velocities of electrons and holes are 4.3×107 and 1.5×107 cm/s, respectively. Part (10) Solved PROBLEMS Transparent Semiconductors 1. Which of the following semiconductors are transparent, partially transparent, nontransparent for visible light (λ = 0.4 – 0.7 μm): Si, GaAs, GaP, and GaN? Solution: (1.1) 1. It follows from Table 2 that Si and GaAs are not transparent, GaP is partially transparent, and GaN is transparent for the visible light. Problem (3) 1. Which of the following semiconductors are transparent, partially transparent, non transparent for visible light (λ = 0.4–0.7 µm): Si, GaAs, GaP, and GaN? Solution: 1. It follows from Table 2 that Si and GaAs are not transparent, GaP is partially transparent, and GaN is transparent for the visible light. Example (1) Measuring the Band-Gap Energy if a semiconductor is transparent to light with a wavelength longer than 0.87 µm, what is its band-gap energy? SOLUTION: Photon energy of light with 0.87 µm wavelength is, with c being the speed of light ๐ ๐. ๐๐ ๐ ๐๐−๐๐ (๐. ๐) ๐ ๐ ๐ ๐๐๐ ๐/๐ ๐๐= ๐ = ๐ ๐. ๐๐ ๐๐ −๐๐ ๐. ๐๐ ๐ ๐๐ ๐ ๐๐ = ๐. ๐๐ ๐๐ ๐. ๐๐ ๐ ๐๐−๐๐ ๐๐ฝ ๐๐ = ๐. ๐ ๐ ๐๐−๐๐ ๐ ๐. ๐๐ ๐๐ = ๐. ๐๐ ๐๐ฝ ๐๐ = ๐. ๐๐ ๐๐ฝ ๐. ๐๐ ๐๐ Therefore, the band gap of the semiconductor is 1.42 eV. The semiconductor is perhaps GaAs (Table). Band-gap energies of selected semiconductors. Semiconductor InSb Ge Si GaAs GaP ZnSe Diamond Eg (eV) 0.18 0.67 1.12 1.42 2.25 2.7 6.0 Part (11) Solved PROBLEMS THE DRIFT CURRENT , THE DIFFUSION CURRENT Example 1.5 Calculate the built-in potential barrier of a pn junction. Consider a silicon pn junction at T = 300 K, doped at Na = 1016 cm−3 in the p-region and Nd = 1017cm−3 in the n-region. Solution: We have ni = 1.5 × 1010cm−3 for silicon at room temperature. We then find ๐๐ ๐ง๐ ๐๐๐๐ ๐ฑ ๐๐๐๐ ๐๐๐ข = ๐๐ ๐ฅ๐ง ( ๐ ) = ๐. ๐๐๐ ๐ฅ๐ง [ ] = ๐. ๐๐๐ ๐ (๐. ๐ ๐ฑ ๐๐๐๐ )๐ ๐ง๐ข Comment: Because of the log function, the magnitude of Vbi is not a strong function of the doping concentrations. Therefore, the value of Vbi for silicon pn junctions is usually within 0.1 to 0.2 V of this calculated value. Exercise 1.5 Calculate Vbi for a GaAs pn junction at T = 300 K for Na = 1016 cm−3 and Nd = 1017 cm−3 (b) Repeat part (a) for a Germanium pn junction with the same doping concentrations. Solution: (a) Vbi = 1.23 V, (b) Vbi = 0.374 V). Example 2.10 The hole density in an n-type silicon wafer (Nd = 1017 cm-3) decreases linearly from 1014 cm-3 to 1013 cm-3 between x = 0 and x = 1 µm. Calculate the hole diffusion current density. Solution The hole diffusion current density equals: ๐๐ ๐ ๐ ๐ ๐ ๐๐ ๐ฑ๐ = ๐ ๐ซ๐ = ๐. ๐ ๐ ๐๐−๐๐ ๐ ๐. ๐ ๐ = ๐. ๐๐ ๐จ/๐๐ −๐ ๐ ๐ ๐๐ ๐ ๐ซ๐ = ๐ฝ๐ ๐๐ = ๐. ๐๐๐๐ ๐ ๐๐๐ = ๐. ๐ ๐ ⁄๐ and the hole mobility in the n-type wafer was obtained from Table as the hole mobility in a p-type material with the same doping density. Problem 2.18 Consider the problem of finding the doping density, which results in the maximum possible resistivity of silicon at room temperature. (ni = 1010 cm-3, µn = 1400 cm2/V-sec and µp = 450 cm2/V-sec.) Should the silicon be doped at all or do you expect the maximum resistivity when dopants are added? If the silicon should be doped, should it be doped with acceptors or donors (assume that all dopant is shallow). Calculate the maximum resistivity, the corresponding electron and hole density and the doping density. Solution Since the mobility of electrons is larger than that of holes, one expects the resistivity to initially decrease as acceptors are added to intrinsic silicon. The maximum resistivity (or minimum conductivity) is obtained from: ๐ (๐ ๐๐ + ๐ (๐ ๐๐ + ๐ ๐๐ ) ๐ ๐ =๐ = ๐ ๐ ๐ ๐ ๐ ๐ ๐ which yields: ๐= √ ๐๐๐ ๐ ๐๐ ) =๐ ๐๐ ๐๐ = ๐. ๐๐ ๐๐ = ๐. ๐ ๐ ๐๐๐ ๐๐−๐ ๐๐ The corresponding hole density equals p = 1.76 ni = 1.76 x 109 cm-3 and the amount of acceptors one needs to add equals Na = 1.20 ni = 1.20 x 109 cm-3. The maximum resistivity equals: ๐ ๐ ๐๐๐๐ = = = ๐๐๐ ๐ฒ๐ ๐๐ ๐ ๐๐ ๐ ๐๐๐๐ ๐ (๐ ๐๐ + ๐ ๐๐ ) Problem 2.30 Phosphorous donor atoms with a concentration of 1016 cm-3 are added to a piece of silicon. Assume that the phosphorous atoms are distributed homogeneously throughout the silicon. The atomic weight of phosphorous is 31. a) What is the sample resistivity at 300 K? b) What proportion by weight does the donor impurity comprise? The density of silicon is 2.33 gram/cm3. c) If 1017 atoms cm-3 of boron are included in addition to phosphorous, and distributed uniformly, what is the resulting resistivity and type (i.e., p- or n-type material)? d) Sketch the energy-band diagram under the condition of part c) and show the position of the Fermi energy relative to the valence band edge. Solution a) The electron mobility in the silicon equals ๐๐๐๐ − ๐๐๐๐ ๐๐๐๐ − ๐๐. ๐ ๐๐ = ๐๐๐๐ + ๐ = ๐๐. ๐ + ๐.๐๐๐ ๐ต๐ซ ๐๐๐๐ ๐+ ( ) ๐+ ( ๐๐ ) ๐ต ๐ ๐.๐ ๐ ๐๐ ๐ ๐= b) = ๐๐๐๐ ๐๐ /๐๐ ๐ ๐ ๐ = = ๐ ๐ (๐ ๐๐ + ๐ ๐๐ ) ๐. ๐ ๐ ๐๐−๐๐ ๐ ๐๐๐๐๐ ๐๐๐๐ = ๐. ๐๐ ๐ ๐๐ ๐๐๐๐๐๐ | ๐๐๐๐๐๐ ๐ ๐๐๐๐๐๐ | ๐๐๐๐๐๐ ๐+๐๐ ๐ด๐ ๐จ ๐ต๐ ๐๐ ๐ ๐. ๐ ๐ ๐๐๐๐ ๐ ๐๐๐ ๐ ๐๐๐๐ = = ๐ ๐๐๐๐๐๐ ๐๐ ๐๐ ๐๐๐๐ | = ๐. ๐ ๐ ๐๐−๐ c) The semiconductor is p-type since Na>Nd The hole density is obtained from: ๐ − − ๐ต+ ๐ต+ ๐ − ๐ต๐ ๐ − ๐ต๐ ๐= + √( ) + ๐๐๐ ๐ ๐ ๐ ๐ ๐ ๐๐๐๐ ๐ ๐ ๐๐๐๐ √ = + ( ) + (๐๐๐๐ )๐ = ๐ ๐ ๐๐๐๐ ๐๐−๐ ๐ ๐ and the mobility is calculated from the sum of the donor and acceptor densities ๐๐๐๐ − ๐๐๐๐ ๐๐๐. ๐ − ๐๐. ๐ ๐๐ = ๐๐๐๐ + = ๐๐. ๐ + ๐ ๐.๐๐๐ ๐ต ๐๐๐ ๐๐๐๐ ๐+ ( ) ๐+ ( ๐๐ ) ๐ต ๐ ๐.๐๐ ๐ ๐๐ ๐ = ๐๐๐. ๐ ๐๐ /๐๐ leading to the conductivity of the material: ๐ ๐ ๐ ๐= = = ๐ ๐ (๐ ๐๐ + ๐ ๐๐ ) ๐. ๐ ๐ ๐๐−๐๐ ๐ ๐๐๐. ๐๐ ๐๐ ๐๐๐๐ = ๐. ๐๐ ๐ ๐๐ d) ๐ต๐ ๐๐๐๐ ๐ฌ๐ญ − ๐ฌ๐ = ๐ฒ๐ป ๐๐ = ๐. ๐๐๐๐ ๐๐ = ๐๐๐ ๐๐๐ฝ ๐ ๐ ๐ ๐๐๐๐ Problem 2.32 The electron concentration in a piece of lightly doped, n-type silicon at room temperature varies linearly from 1017 cm-3 at x = 0 to 6 x 1016 cm-3 at x = 2 µm. Electrons are supplied to keep this concentration constant with time. Calculate the electron current density in the silicon if no electric field is present. Assume µn = 1000 cm2/V-s and T = 300 K. Solution The diffusion current is obtained from: ๐ ๐ ๐๐−๐๐ − ๐ ๐ ๐๐๐๐ −๐๐ ๐ฑ๐ = ๐ ๐ซ ๐ = ๐. ๐ ๐ ๐๐ ๐ ๐๐. ๐ ๐ ๐ ๐ ๐ ๐ ๐๐−๐ = ๐๐๐ ๐จ/๐๐ where the diffusion constant Dn is obtained from: Dn = µn x Vt = 1000 x 0.0258 = 25.8 cm2 Example 4.1 An abrupt silicon p-n junction consists of a p-type region containing 2 x 1016 cm-3 acceptors and an n-type region containing also 1016 cm-3 acceptors in addition to 1017 cm-3 donors. a. Calculate the thermal equilibrium density of electrons and holes in the p-type region as well as both densities in the ntype region. b. Calculate the built-in potential of the p-n junction. c. Calculate the built-in potential of the p-n junction at 400 K. Solution a. The thermal equilibrium densities are: In the p-type region: ๐๐๐ ๐๐๐๐ ๐๐ −๐ ๐ = ๐ต๐ = ๐ ๐ ๐๐ ๐๐ , ๐ = = = ๐ ๐ ๐๐๐ ๐๐−๐ ๐๐ ๐ ๐ ๐ ๐๐ In the n-type region ๐๐๐ ๐๐๐๐ ๐๐ −๐ ๐ = ๐ต๐ − ๐ต๐ = ๐ ๐ ๐๐ ๐๐ , ๐ = = ๐ ๐ ๐ ๐๐๐๐ = ๐. ๐๐ ๐ ๐๐๐ ๐๐−๐ b. The built-in potential is obtained from ๐ ๐ ๐๐ ๐ ๐ ๐๐๐๐ ๐ ๐ ๐ ๐๐๐๐ ๐๐ = ๐ฝ๐ ๐๐ = ๐. ๐๐๐๐ ๐๐ = ๐. ๐๐๐ฝ ๐๐๐๐ ๐๐๐ c. Similarly, the built-in potential at 400 K equals ๐ ๐ ๐๐๐๐ ๐ ๐ ๐ ๐๐๐๐ ๐๐ = ๐ฝ๐ ๐๐ = ๐. ๐๐๐๐ ๐๐ = ๐. ๐๐๐ฝ (๐. ๐๐ ๐๐๐๐๐ )๐ ๐๐๐ where the intrinsic carrier density at 400 K was obtained from Example 2.4 b. ๐ ๐ ๐๐ Example 1.4 Calculate the diffusion current density for a given semiconductor. Consider silicon at T = 300 K. Assume the electron concentration varies linearly from n = 1012 cm−3 to n = 1016 cm−3 over the distance from x = 0 to x = 3 μm. Assume Dn = 35 cm2/s. We have ๐๐ง ๐ซ๐ง ๐๐๐๐ − ๐๐๐๐ −๐๐ ๐ = ๐ ๐๐ง = ๐ ๐๐ง = ๐ . ๐ ๐ฑ ๐๐ ๐ฑ ๐๐ ๐ฑ ( ) = ๐๐๐ ๐⁄ ๐ −๐ ๐ฆ ๐๐ฑ ๐ซ๐ฑ ๐ − ๐ ๐ฑ ๐๐ Comment: Diffusion current densities on the order of a few hundred amperes per square centimeter can also be generated in a semiconductor. Exercise 1.4 Consider silicon at T = 300 K. Assume the hole concentration is given by p = 1016e−x/Lp (cm−3), where Lp = 10−3 cm. Calculate the hole diffusion current density at (a) x = 0 and (b) x = 10−3cm. Assume Dp = 10 cm2/s. Solution: (a) 16 A/cm2, (b) 5.89 A/cm2) Example 1.7 Determine the current in a pn junction diode. Consider a pn junction at T = 300 K in which IS = 10−14 A and n = 1. Find the diode current for VD = +0.70 V and VD = −0.70 V. Solution: For VD = +0.70 V, the pn junction is forward-biased and we find ๐ข๐ = ๐๐ฌ ๐๐ ⁄ [๐ ๐๐ − ๐] = ๐๐−๐๐ [๐ ๐.๐⁄ ๐,๐๐๐ − ๐] โถ ๐. ๐๐ ๐ฆ๐ For ๐๐ = −๐. ๐ ๐ , the pn junction is reverse bias ๐ข๐ = ๐๐ฌ [๐ ๐๐ ⁄๐ ๐ − ๐] = ๐๐−๐๐ [๐ −๐.๐⁄ ๐,๐๐๐ − ๐] ≅ − ๐๐−๐๐ ๐ Comment: Although IS is quite small, even a relatively small value of forward-bias voltage can induce a moderate junction current. With a reverse-bias voltage applied, the junction current is virtually zero. Exercise 1.7 (a) A silicon pn junction at T = 300 K has a reverse-saturation current of IS = 2 × 10−14 A. Determine the required forward-bias voltage to produce a current of (i) ID = 50 μA and (ii) ID = 1 mA. (b) Repeat part (a) for IS = 2 × 10−12 Solution a. (i) 0.563 V, (ii) 0.641 V; (b) (i) 0.443 V, (ii) 0.521 V). Part (12) Solved PROBLEMS continuity equation Problem (1) Consider n-type silicon with Nd = 1015cm−3 at T = 300โฆK. A light source is turned on at t = 0. The source illuminates the semiconductor uniformly, generating carriers at the rate of Gn = Gp = 1019cm−3s−1. There is no applied ๏ฌeld. (a) Write down the continuity equation and solve it to ๏ฌnd the expression for the excess minority carrier concentration, ๐น๐(๐), as a function of time for t ≥ 0. Solution: When there is no applied electric ๏ฌeld the carrier distribution is diffusion driven. The continuity equation for the minority carrier ๐๐(๐ , ๐) ๐ ๐ ๐ฑ๐ (๐ , ๐) = + ๐ฎ๐ (๐ , ๐) − ๐น๐ (๐ , ๐) ๐๐ ๐ ๐๐ Then reduces to , ๐๐น๐ ๐๐น๐ = ๐ฎ๐ − ๐๐ ๐๐ With the general solution ๐ ๐น๐ (๐) = ๐จ ๐๐๐ (− ) + ๐ฎ๐ ๐๐ ๐ ๐ Using the initial condition (before the light was turned on) that ๐น๐(๐) = 0, then we ๏ฌnd that๐จ = − ๐ฎ๐ ๐. The full solution then is, ๐ ๐น๐ (๐) = ๐ฎ๐ ๐๐ {๐ − ๐๐๐ (− )} ๐๐ (b) As t →∞, the system will approach steady state. When the steady state excess carrier concentration is 5×1013cm−3, ๏ฌnd the minority carrier lifetime, ๐๐ . Solution: The system will approach steady state as t → ∞. Evidently, the steady state carrier density is given ๐น๐(๐)|๐ญ → ∞ = ๐ฎ๐ ๐๐ . The ๐๐ must then take on the value ๐๐ ๐๐ = ๐ ๐ ๐๐ ⁄๐ฎ . With Gp = 1019 cm−3s−1, then the minority ๐ (hole) carried lifetime must be ๐๐ = 5×10−6s. (c) Determine the time at which the excess carrier concentration becomes half of the steady state value,๐น๐(๐)|๐ญ → ∞ that you calculated in (b). Solution: The value at which ๐ ๐ ๐๐๐ (− ) = ๐๐, ๐ = ๐๐ (๐)๐๐ = ๐. ๐๐ ๐ ๐ ๐ ๐๐−๐ ๐ ๐ ๐ Problem (2) 2. Consider an n-type semiconductor as shown. Illumination produces a constant excess carrier generation rate of Gp is the region −L ≤ x ≤ L. Assume the minority current density is zero at x = −3L and x = 3L. Find the steady state minority carrier concentration as a function of x, ๐น๐(๐). There is no applied electric ๏ฌeld. -3L -L 0 L 3L X An illuminated semiconductor Solution: When there is no applied electric ๏ฌeld the carrier distribution is di๏ฌusion driven. The continuity equation for the minority carrier ๐๐(๐ , ๐) ๐ ๐ ๐ฑ๐ (๐ , ๐) = + ๐ฎ๐ (๐ , ๐) − ๐น๐ (๐ , ๐) ๐๐ ๐ ๐๐ Then reduces to, ๐๐ ๐น๐ (๐, ๐) ๐น๐ ๐ = ๐ซ๐ + ๐ฎ๐ − ๐๐ ๐๐ In − ๐ณ ≤ ๐ ≤≤ ๐ณ And ๐๐ ๐น๐ (๐, ๐) ๐น๐ ๐ = ๐ซ๐ − ๐๐ ๐๐ In − ๐๐ณ ≤ ๐ ≤≤ −๐ณ ๐๐๐ ๐ณ ≤ ๐ ≤≤ ๐๐ณ , with boundary conditions that ๐ ๐น๐ ๐ ๐น๐ (− ๐๐ณ) = (๐ ๐ณ) = ๐ ๐๐ ๐๐ and ๐น๐(−๐ณ) and ๐น๐(๐ณ) are continuous. From symmetry, we need only solve for x > 0 with new boundary condition that ๐ ๐น๐ (๐) = ๐ ๐๐ The solution is ๐ ๐ ๐ฎ๐ ๐๐ + ๐จ ๐๐๐ (− ) + ๐ฉ ๐๐๐ ( ) ๐ ≤ ๐ ≤ ๐ณ ๐ณ๐ ๐ณ๐ ๐น๐ (๐) = ๐ ๐ ๐ช ๐๐๐ (− ) + ๐ซ ๐๐๐ ( ) ๐ณ ≤ ๐ ≤ ๐๐ณ ๐ณ ๐ณ ๐ ๐ { } Where, ๐ณ๐๐ = ๐ซ๐ ๐๐ The end conditions at 0 and L then lead to A = B And ๐ช = ๐ซ ๐๐๐ ( ๐๐ณ ) ๐ณ๐ These results in ๐ฎ๐ ๐๐ + ๐ฌ ๐๐๐๐ ( ๐น๐ (๐) = { ๐ญ๐๐๐๐ ( ๐ ) ๐ณ๐ ๐ − ๐๐ณ ) ๐ณ๐ ๐ ≤๐ ≤๐ณ ๐ณ ≤ ๐ ≤ ๐๐ณ } Where ๐ = ๐๐ ๐๐ง๐ ๐ = ๐ ๐ ๐๐ฑ๐ฉ ( ๐๐ณ ) ๐ณ๐ Are the new constants to ๏ฌnd and where ๐ ๐๐๐๐ (๐) = ๐๐๐(๐) + ๐๐๐ (−๐) is the hyperbolic cosine function? We will later also use the derivative of this function. ๐ ๐๐๐๐ (๐) = ๐๐๐(๐) + ๐๐๐ (−๐) The hyperbolic sine function. At x = L, we ๏ฌnd ๐ณ ๐๐ณ ๐ฎ๐ ๐๐ + ๐ฌ ๐๐๐๐ ( ) = ๐ญ ๐๐๐๐ ( ) ๐ณ๐ ๐ณ๐ ๐ ๐๐ณ ๐ฌ ๐๐๐๐ ( ) = − ๐ญ ๐๐๐๐ ( ) ๐ณ๐ ๐ณ๐ where we have used the evenness of cosh and oddness of sinh. Solving, we ๏ฌnd ๐ณ ๐๐๐๐ ( ) ๐ณ๐ ๐ญ= − ๐ฌ ๐๐ณ ๐๐๐๐ ( ) ๐ณ๐ ๐๐ณ ๐ฎ๐ ๐๐ ( ) ๐ณ๐ ๐ฌ= − ๐ณ ๐๐ณ ๐๐ณ ๐ณ ๐ณ๐ ๐ณ๐ ๐ณ๐ ๐ณ๐ ๐๐๐๐ ( ) ๐๐๐๐ ( ) + ๐๐๐๐ ( ) ๐๐๐๐ ( ) ๐๐ณ ๐ฎ๐ ๐๐ ๐๐๐๐ ( ) ๐ณ๐ = ๐๐ณ ๐๐๐๐ ( ) ๐ณ๐ Where the identity, ๐๐ณ ๐ณ ๐๐ณ ๐๐ณ ๐ณ ) = ๐๐๐๐ ( ) ๐๐๐๐ ( ) + ๐๐๐๐ ( ) ๐๐๐๐ ( ) ๐ณ๐ ๐ณ๐ ๐ณ๐ ๐ณ๐ ๐ณ๐ has been used. Substituting back, we ๏ฌnd ๐๐๐๐ ( ๐ณ ๐ฎ๐ ๐๐ ๐๐๐๐ ( ) ๐ณ๐ ๐ญ= ๐๐ณ ๐๐๐๐ ( ) ๐ณ๐ ๐๐ณ ๐ ๐ณ๐ ๐ณ๐ ๐๐๐๐ ( ) ๐๐๐๐ ( ) ๐น๐ (๐) = (๐ − ๐๐ณ ) ๐ ≤๐ ≤๐ณ ๐๐๐๐ ( ) ๐ณ๐ ๐ณ ๐−๐๐ณ ๐ณ๐ ๐ณ๐ ๐ฎ๐ ๐๐ ๐๐๐๐ ( ) ๐๐๐๐ ( ๐๐ณ ) ๐ณ ≤ ๐ ≤ ๐๐ณ ๐๐๐๐ ( ) ๐ณ๐ (b) Suppose the excess carriers are generated such that the excess carrier concentrations are 10% of the equilibrium majority carrier concentrations. Calculate the quasi-Fermi levels relative the intrinsic Fermi levels, that is, Fn −Ei and Ei−Fp. Solution: Here we can use that ๐ฌ −๐ฌ ๐๐ + ๐น๐ = ๐๐ ๐๐๐ ( ๐ ๐) , to find, ๐ฒ๐ป ๐. ๐ ๐ ๐ต๐ ๐ญ๐ − ๐ฌ๐ = ๐ฒ๐ป ๐๐ ( ) = ๐. ๐๐๐ ๐๐ฝ ๐๐ The minority carriers than are given by ๐๐ = ๐๐๐ ๐๐ = ๐ ๐ ๐๐−๐ ๐๐−๐ , And , ๐ = ๐ + ๐น๐ ≈ ๐น๐ = ๐๐ ๐๐๐ ( ๐ฌ๐ − ๐ฌ๐ญ ) ๐ฒ๐ป That yields, ๐ฌ๐ − ๐ฌ๐ = ๐ฒ๐ป ๐๐ ( ๐. ๐ ๐ ๐ต๐ ) = ๐. ๐๐๐ ๐๐ฝ ๐๐ Part (13) Solved PROBLEMS PN junction theory Example A silicon diode at temperature T = 300K has doping concentration NA = ND = 1.2x1016 cm -3 , ni = 1.5 x1010 cm -3, Dn = 25 cm2 s -1, Dp = 10 cm2 s -1, KS = 11.7, Lp = 2.2x10-3cm and Ln = 3.5x10-3cm, and cross section area = 1x10-2 cm2 . Solution: The minority hole in n - region ๐ง๐๐ข ๐. ๐๐๐ฑ๐๐๐๐ ๐ฉ๐ง๐จ = = = ๐. ๐๐๐๐ฑ๐๐๐ ๐๐ฆ−๐ ๐๐ ๐๐ ๐. ๐๐ฑ๐๐ The minority electron in npo p-region ๐ง๐๐ข ๐. ๐๐๐ฑ๐๐๐๐ ๐ง๐ฉ๐จ = = = ๐. ๐๐๐๐ฑ๐๐๐ ๐๐ฆ−๐ ๐๐ ๐๐ ๐. ๐๐ฑ๐๐ The reverse saturation current Is =๐จ [ ๐ ๐ซ๐ ๐๐๐ ๐ณ๐ ๐๐ ๐ ๐.๐๐๐ ๐ ๐๐๐ ๐.๐ ๐ ๐๐−๐ + ๐ ๐ซ๐ ๐๐๐ ๐ณ๐ ] = ๐. ๐๐๐ ๐ ๐๐ −๐๐ [ ๐๐ ๐ ๐.๐๐๐๐ ๐ ๐๐๐ ๐.๐ ๐ ๐๐−๐ + ] = ๐. ๐๐ ๐ ๐๐−๐๐ ๐จ Example An abrupt silicon (nI = 1010 cm-3) p-n junction consists of a p-type region containing 1016 cm-3acceptors and an n-type region containing 5 x 1016 cm-3 donors. a. Calculate the built-in potential of this p-n junction. b. Calculate the total width of the depletion region if the applied voltage Va equals 0, 0.5 and -2.5 V. c. Calculate maximum electric field in the depletion region at 0, 0.5 and -2.5 V. d. Calculate the potential across the depletion region in the n-type semiconductor at 0, 0.5 and -2.5 V. Solution: The built-in potential is calculated from: The depletion layer width is obtained from: the electric field from and the potential across the n-type region equals Where One can also show that: This yields the following numeric values: Example: Consider an abrupt p-n diode with Na = 1018 cm-3 and Nd = 1016 cm-3. Calculate the junction capacitance at zero bias. The diode area equals 10-4 cm2. Repeat the problem while treating the diode as a one-sided diode and calculate the relative error. Solution: The built in potential of the diode equals: The depletion layer width at zero bias equals: And the junction capacitance at zero bias equals: Repeating the analysis while treating the diode as a one-sided diode, one only has to consider the region with the lower doping density so that And the junction capacitance at zero bias equals The relative error equals 0.5 %, which justifies the use of the onesided approximation. Example An abrupt silicon p-n junction (Na = 1016 cm-3 and Nd = 4 x 1016 cm-3) is biased with Va = 0.6 V. Calculate the ideal diode current assuming that the n-type region is much smaller than the diffusion length with wn' = 1 mm and assuming a "long" p-type region. Use mn = 1000 cm2/V-s and mp = 300 cm2/V-s. The minority carrier lifetime is 10 ms and the diode area is 100 mm by 100 mm. Solution: The current is calculated from: With Dn = mn Vt = 1000 x 0.0258 = 25.8 cm2/V-s Dp = mp Vt = 300 x 0.0258 = 7.75 cm2/V-s np0 = ni2/Na = 1020/1016 = 104 cm-3 pn0 = ni2/Nd = 1020/4 x 1016 = 2.5 x 103 cm-3 Yielding I = 40.7 mA Note that the hole diffusion current occurs in the "short" n-type region and therefore depends on the quasi-neutral width in that region. The electron diffusion current occurs in the "long" p-type region and therefore depends on the electron diffusion length in that region. Example b. Calculate the diffusion capacitance of the diode described in Example 4.4 at zero bias. Use µn= 1000 cm2/V-s, µp = 300 cm2/V-s, wp' = 1 µm and wn' = 1 mm. The minority carrier lifetime equals 0.1 ms. c. For the same diode, find the voltage for which the junction capacitance equals the diffusion capacitance. Solution a. The diffusion capacitance at zero volts equals Using And Where the "short" diode expression was used for the capacitance associated with the excess charge due to electrons in the p-type region. The "long" diode expression was used for the capacitance associated with the excess charge due to holes in the n-type region.The diffusion constants and diffusion lengths equal Dn = µn x Vt = 25.8 cm2/s Dp = µp x Vt = 7.75 cm2/s And the electron transit time in the p-type region equals b. The voltage at which the junction capacitance equals the diffusion capacitance is obtained by solving Yielding Va = 0.442 V Part (14) Solved PROBLEMS ideal and Nonideal p-n Junction 1. Find the built-in potential for a p-n Si junction at room temperature if the bulk resistivity of Si is 1 โฆcm. Electron mobility in Si at RT is 1400 cm2 V−1 s−1; µn/µp = 3.1; ni = 1.05×1010 cm−3. Solution: By de๏ฌnition, e๐๐ = Fn −Fp. Concentrations of the free carriers are given by ๐ฌ๐ − ๐ญ๐ ๐ญ๐ ๐ = ๐ต๐ (− ๐ = ๐ต๐ ๐๐๐ (− ) , ) ๐ฒ๐ป ๐ฒ๐ป From here we get that ๐ ๐ ๐๐ ๐ ๐๐ = ๐ฌ๐ + ๐ฒ๐ป ๐๐ ( ) + ๐ฒ๐ป ๐๐ ( ) = ๐ฌ๐ + ๐ฒ๐ป ๐๐ ( ) ๐ต๐ ๐ต๐ ๐ต๐ ๐ต๐ ๐ฌ๐ ๐๐๐ = ๐ต๐ ๐ต๐ ๐๐๐ (− ) ๐ฒ๐ป We obtain , ๐ฒ๐ป ๐๐ ๐๐ = ๐๐ ( ๐ ) ๐ ๐๐ From n = 1/eρµn and p = 1/eρµp, we ๏ฌnally get ๐๐ = 0.68 V. 2. For the p-n Si junction from the previous problem calculate the width of the space charge region for the applied voltages V = −10, 0, and +0.3 V. ฯตSi = 11.9 Solution: Taking into account that at room temperature all donors and acceptors are ionized, i.e. n = Nd and p = Na, from the values found in the previous problem and ๐⁄ ๐ (๐๐ − ๐ฝ) ๐ต๐ + ๐ต๐จ ๐ ๐= { } ๐๐ ๐ ๐ต ๐ ๐ต๐จ we get ω(−10V) = 2 µm, ω(0V) = 0.5 µm, and ω(+0.3V) = 0.4 µm. 1. For the parameters given in the previous problem ๏ฌnd the maximum electric ๏ฌeld within the space charge region. Compare these values with the electric ๏ฌeld within a shallow donor: E ≈ e/ ฯตSi a2B, where aB is the Bohr radius of a shallow donor, ๐๐๐ ๐๐ ๐๐∗ ๐๐ = ∗ ๐ ๐๐๐ = ๐. ๐๐ ๐๐ ๐ ๐๐ Solution: From the previous problem and ๐⁄ ๐ ๐ ๐ (๐๐ − ๐ฝ) ๐ต๐ + ๐ต๐จ ๐ ๐ฌ = ๐{ } ๐ ๐ต๐ ๐ต๐จ we obtain that E(−10V) = 105 V/cm, E(0V) = 2.6×104 V/cm, and E(+0.3V) = 2×104 V/cm. The electric ๏ฌeld within a shallow donor is, in turn, E ≈ 3.4×105 V/cm, that is, comparable to that of the p-n junction. 4. Calculate the capacity of the p-n junction from the problem 2 if the area of the junction is 0.1 cm2. Solution: Since ๐๐บ ๐๐ ๐ we get C(−10V) = 0.5 nF, C(0V) = 2 nF, and C(+0.3V) = 2.6 nF. ๐ช= 5. n-Si of a p-n Si junction has a resistivity of 1 โฆcm. What should be the resistivity of p-Si so that 99 % of the total width of the space charge region would be located in n-Si (p+-n junction)? For the parameters needed see problem 1. Solution: From the conditions of the problem ωa = 0.01ω and ωd = 0.99ω. Since ωa/ωd = Nd/Na , we get that Na = 99Nd. Because Nd = 1/eρµn = 4.5×1015 cm−3, we get Na = 4.4×1017 cm−3. 6. At room temperature under the forward bias of 0.15 V the current through a p-n junction is 1.66 mA. What will be the current through the junction under reverse bias? Solution: js = 1.66mAexp(−eV/kT) = 4 µA. 7. For a p+-n Si junction the reverse current at room temperature is 0.9 nA/cm2. Calculate the minority-carrier lifetime if Nd = 1015 cm−3, ni = 1.05×1010 cm−3, and µp = 450 cm2 V−1 s−1. Solution: For a p+-n junction ๐⁄ ๐ ๐ ๐ซ๐ ๐ ๐ซ๐ ๐๐๐ ๐ ๐๐๐ ๐ซ๐ ๐ ๐ฑ๐ = = = ( ) ๐ณ๐ ๐ต๐ ๐ณ๐ ๐ต๐ ๐ ๐ Taking into account that µ = eD/kT, we ๏ฌnally get τp = 4.5×10−9 s. 8. How does the reverse current of a Si p-n junction change if the temperature raises from 20 to 50 โฆC? The same for a Ge p-n junction. Band gaps of Si and Ge are 1.12 and 0.66 eV, respectively. Solution: ๐ฌ๐ Since๐๐ ~ ๐๐๐ ~ ๐ป๐ ๐๐๐ (− ) ๐ฒ๐ป we get ๐ฌ๐ ๐ฌ๐ ๐๐ (๐ป๐ ) ๐ป๐ ๐ = ( ) ๐๐๐ (− + ) ๐๐ (๐ป๐ ) ๐ป๐ ๐ฒ๐ป๐ ๐ฒ๐ป๐ From here the ratios of the reverse currents in the p-n junctions made of Ge and Si are 15 and 82, respectively. 9. Estimate temperatures at which p-n junctions made of Ge, Si, and GaN lose their rectifying characteristics. In all cases Na = Nd = 1015 cm−3. Assume that Eg are independent of the temperature and are 0.66, 1.12, and 3.44 eV for Ge, Si, and GaN, respectively. Intrinsic carrier concentrations at room temperature are niGe= 2×1013,niSi = 1010, and niGaN = 10−9 cm−3. Solution: p-n junction stops working when concentrations of electrons and holes equalize. It happens when − ๐ฌ๐ − ๐ฌ๐ ๐ ๐ต๐ (๐ต๐จ ) ≅ ๐๐ ≈ √๐ต๐ ๐ต๐ ๐๐๐ ( ) ~ ๐ป ⁄๐ ๐๐๐ ( ) ๐ ๐ฒ๐ป ๐ ๐ฒ๐ป From here and the parameters given we get that the maximum temperatures are TGe ≈ 400 K, TSi ≈ 650 K, and TGaN ≈ 1700 K. That is, only wide band gap semiconductors are suitable for extremal applications. Problem 2.25 Electrons in silicon carbide have a mobility of 1000 cm2/Vsec. At what value of the electric field do the electrons reach a velocity of 3 x 107 cm/s? Assume that the mobility is constant and independent of the electric field. What voltage is required to obtain this field in a 5 micron thick region? How much time do the electrons need to cross the 5 micron thick region? Solution The electric field is obtained from the mobility and the velocity: ๐ ๐๐๐๐ ๐บ= = = ๐๐ ๐ฒ๐ฝ/๐๐ ๐ ๐ ๐ ๐๐๐ Combined with the length one finds the applied voltage. V = ๐บ L = 30,000 x 5 x 10-4 = 15 V The transit time equals the length divided by the velocity: tr = L/ ๐ = 5 x 10-4/3 x 107 = 16.7 ps Example 4.2 An abrupt silicon (ni = 1010 cm-3) p-n junction consists of a ptype region containing 1016 cm-3 acceptors and an n-type region containing 5 x 1016 cm-3 donors. a. Calculate the built-in potential of this p-n junction. b. Calculate the total width of the depletion region if the applied voltage Va equals 0, 0.5 and -2.5 V. c. Calculate maximum electric field in the depletion region at 0, 0.5 and -2.5 V. d. Calculate the potential across the depletion region in the n-type semiconductor at 0, 0.5 and -2.5 V. Solution The built-in potential is calculated from: ๐๐ ๐๐ ๐๐๐๐ ๐ ๐ ๐ ๐๐๐๐ ๐๐ = ๐ฝ๐ ๐๐ = ๐. ๐๐๐๐ ๐๐ = ๐. ๐๐๐ฝ ๐๐๐๐ ๐๐๐ The depletion layer width is obtained from: ๐= √ ๐ ๐๐ ๐ ๐ ( + ) (๐๐ − ๐ฝ๐ ) ๐ ๐ต๐ ๐ต๐ the electric field from ๐ (๐๐ − ๐ฝ๐ ) ๐ and the potential across the n-type region equals ๐ ๐ต๐ ๐๐๐ ๐๐ = ๐ ๐๐ Where, ๐ต๐ ๐๐ = ๐ ๐ต๐ + ๐ต๐ one can also show that (๐๐ − ๐ฝ๐ )๐ต๐ ๐๐ = ๐ต๐ + ๐ต๐ This yields the following numeric values: ๐บ (๐ = ๐) = w ๐บ ๐๐ Va = 0 V 0.315 µm 40 kV/cm 0.105 V Va = 0.5 V 0.143 µm 18 kV/cm 0.0216 Va = -2.5 V 0.703 µm 89 kV/cm V 0.522 V Example 4.3 An abrupt silicon p-n junction (Na = 1016 cm-3 and Nd = 4 x 1016 cm-3) is biased with Va = 0.6 V. Calculate the ideal diode current assuming that the n-type region is much smaller than the diffusion length with wn = 1 µm and assuming a "long" ptype region. Use µn = 1000 cm2/V-s and µp = 300 cm2/V-s. The minority carrier lifetime is 10 µs and the diode area is 100 µm by 100 µm. Solution: The current is calculated from: ๐ฝ๐ ๐ซ๐ ๐๐๐ ๐ซ๐ ๐๐๐ ⁄ ๐ฐ=๐๐จ [ + ] (๐ ๐ฝ๐ − ๐) ๐ณ๐ ๐พ๐ with Dn = µnVt = 1000 x 0.0258 = 25.8 cm2/V-s DP = µPVt = 300 x 0.0258 = 7.75 cm2/V-s np0 = n2i/Na = 1020/1016 = 104 cm-3 pn0 = n2i/Nd = 1020/4 x 1016 = 2.5 x 103 cm-3 ๐ณ๐ = √๐ซ๐ ๐๐ = √๐๐. ๐ ๐ ๐๐−๐ = ๐๐๐ ๐๐ yielding I = 40.7 µΑ Note that the hole diffusion current occurs in the "short" ntype region and therefore depends on the quasi-neutral width in that region. The electron diffusion current occurs in the "long" p-type region and therefore depends on the electron diffusion length in that region. Example 4.4 Consider an abrupt p-n diode with Na = 1018 cm-3 and Nd = 1016 cm-3. Calculate the junction capacitance at zero bias. The diode area equals 10-4 cm2. Repeat the problem while treating the diode as a one-sided diode and calculate the relative error. Solution The built in potential of the diode equals: ๐ต๐ ๐ต๐ ๐๐ = ๐ฝ๐ ๐๐ = ๐. ๐๐๐ฝ ๐๐๐ The depletion layer width at zero bias equals: ๐พ= √ ๐ ๐๐ (๐๐ − ๐) = ๐. ๐๐ ๐๐ ๐ ๐ต๐ And the junction capacitance at zero bias equals: ๐๐ ๐ช๐๐ = | = ๐. ๐๐ ๐๐ญ ๐พ ๐๐=๐ Repeating the analysis while treating the diode as a onesided diode, one only has to consider the region with the lower doping density so that ๐พ = ๐๐ = √ ๐ ๐๐ (๐ − ๐ฝ๐ ) = ๐. ๐๐ ๐๐ ๐ ๐ต๐ ๐ And the junction capacitance at zero bias equals ๐๐ ๐ช๐๐ = | = ๐. ๐๐ ๐๐ญ ๐พ ๐๐=๐ The relative error equals 0.5 %, which justifies the use of the one-sided approximation. 1.3 Ideal p-n Junction 1. Find the built-in potential for a p-n Si junction at room temperature if the bulk resistivity of Si is 1 ฮcm. Electron mobility in Si at RT is 1400 cm2 V−1 s−1; μn/μp = 3.1; ni = 1.05 × 1010 cm−3. Solution: (3.1) By definition, e๐๐ = Fn − Fp. Concentrations of the free carriers are given by ๐ฌ๐ − ๐ญ๐ ๐ฌ๐ − ๐ญ๐ ๐ = ๐ต๐ ๐๐๐ (− ) , ๐ต๐ ๐๐๐ (− ) ๐ฒ๐ป ๐ฒ๐ป From here we get that ๐ ๐ ๐๐ ๐๐๐ = ๐ฌ๐ + ๐ฒ๐ป ๐๐ ( ) + ๐ฒ๐ป ๐๐ ( ) = ๐ฌ๐ + ๐ฒ๐ป ๐๐ ( ) ๐ต๐ ๐ต๐ ๐ต ๐ ๐ต๐ Since, ๐๐๐ = ๐ต๐ ๐ต๐ ๐๐๐ (− ๐ฌ๐ ) ๐ฒ๐ป we obtain that ๐ฒ๐ป ๐๐ ๐๐ ( ๐ ) ๐ ๐๐ From n = 1/e ρ μn and p = 1/e ρ μp, we finally get ๐๐ = 0.68 V. ๐๐ = 6. At room temperature under the forward bias of 0.15 V the current through a p-n junction is 1.66 mA. What will be the current through the junction under reverse bias? Solution: (3.6) js = 1.66 mA exp(−eV/kT) = 4 μA. 7. For a p+-n Si junction the reverse current at room temperature is 0.9 nA/cm2. Calculate the minority-carrier lifetime if Nd = 1015 cm−3, ni = 1.05 × 1010 cm−3, and μp = 450 cm2 V−1 s−1. Solution: (3.7) For a p+-n junction ๐⁄ ๐ ๐ ๐ซ๐ ๐ ๐๐๐ ๐ซ๐ ๐ ๐๐๐ ๐ซ๐ ๐ ๐ฑ๐บ = = = ( ) ๐ณ๐ ๐ต๐ ๐ณ๐ ๐ต๐ ๐๐ Taking into account that μ = eD/kT, we finally get τp = 4.5 × 10−9 s. 1. Problem: A silicon p-n junction is formed between n-type Si doped with ND = 1017 cm-3and p-type Si doped with NA = 1016 cm-3. (a) Sketch the energy band diagram. Label all axes and all important energy levels. (b) Find nn0, np0, pp0, and pn0. Sketch the carrier concentration (of both electrons and holes) as a function of position. (c) Calculate the built-in potential Vbi in eV. Solution: (a) The energy band diagram with labeled important energy levels and axes is ECp Ei ECn EF EVp Eg EVn (b) Given n+= 1.5 x 1010 cm-3, in the quasi-neutral p-region, Ppo = NA = 1016 cm−3 In the quasi-neutral n-region, ๐ง๐ง๐จ = ๐๐ = ๐๐๐๐ ๐๐ฆ−๐ In the depletion region, ๐ง๐๐ข ๐ง๐ฉ๐จ = = ๐. ๐๐ ๐ฑ๐๐๐ ๐๐ฆ−๐ ๐๐ for p-side and ๐๐๐ ๐๐๐ = = ๐. ๐๐ ๐๐๐๐ ๐๐−๐ ๐ต๐ซ for n-side.. The diagram for carrier concentration is: n(Xp) p(Xn) pn Np 0 0 (b) The build-in potential is ๐๐ ๐๐ ๐๐ ๐๐ ๐ฉ๐ฉ ๐๐๐ข = ๐ฅ๐ง ๐ = ๐ฅ๐ง = ๐. ๐๐๐ ๐๐ ๐ช ๐ช ๐ฉ๐ง ๐ง๐ข Problem: 4 Consider a p+-n Si junction at T = 300 K with NA = 1018 cm-3 and ND = 1016 cm-3. The minority carrier hole diffusion constant is Dp = 12 cm2/s and the minority carrier hole lifetime is τp = 100 ns. The crosssectional area of the junction is A = 10-4 cm2. Calculate the reverse saturation current Is = AJs. Calculate also the current at a forward bias Va = 0.5 V. Solution: Since NA >> ND, it is an asymmetric junction and the total current is dominated by the most heavily-doped side of the junction. the saturation current density is given by: ๐๐ฌ = ๐ช ๐๐ฉ ๐ฉ๐ง๐จ ๐๐ฉ Where, ๐⁄ ๐ ๐๐ฉ = (๐๐ฉ ๐๐ฉ ) −๐ = ๐. ๐๐๐ ๐ฑ ๐๐ ๐๐ฆ −๐ ๐๐ง๐ ๐ฉ๐ง๐จ ๐ง๐๐ข = = ๐. ๐๐ ๐ฑ ๐๐−๐ ๐๐ฆ−๐ ๐๐ Js = 3:9492 x 10-11 A/cm2 Is = - A Js = - 3:9492 x 10-15 A For a forward bias Va = 0.5 V, the current is: So, ๐ = ๐๐ฌ (๐ ๐ช๐๐จ⁄ ๐๐ − ๐ ) = ๐. ๐๐ ๐๐ Problem (1) 1. n-Si with Nd = 7 × 1015 cm−3 additionally contains Nt = 1015 cm−3 generation- recombination centers located at the intrinsic Fermi level with σn = σp = 10−15 cm2 and vt = 107 cm/s. Calculate generation rate, if 1. n and p are low as compared to the equilibrium value 2. only p is below the equilibrium value. For Si, ni = 1.05×1010 cm−3. Solution : By de๏ฌnition ๐๐๐ − ๐ ๐ ๐ฎ๐ = − ๐น๐ = ๐๐ (๐ + ๐๐ ) + ๐๐ (๐ + ๐๐ ) −๐ ๐ −๐ Where ๐−๐ ๐ = ๐๐ = ๐ต๐ ๐๐ ๐๐ = ๐๐ ๐ . In the ๏ฌrst case n and p are less than ni. Thus, np <๐๐๐ and hence ๐๐๐ ๐๐ ๐ฎ๐ = = = ๐. ๐ ๐ ๐๐๐๐ ๐๐−๐ /๐ ๐๐ (๐๐ + ๐๐ ) ๐ ๐๐ In the second case n = Ndโซni, whereas p <ni, hence ๐๐๐ ๐๐๐ ๐๐๐ ๐ฎ๐ = = = = ๐. ๐ ๐ ๐๐๐๐ ๐๐−๐ /๐ (๐ ) ๐๐ + ๐๐ + ๐๐ ๐ ๐ ๐ ๐ ๐ ๐ต๐ Problem (2) Illumination of n-type Si (Nd = 1016 cm−3) generates 1021 cm−3/s electron-hole pairs. Si has Nt = 1015 cm−3 generation-recombination centers with σn = σp = 10−16 cm2. Calculate equilibrium concentration of electrons and holes if Et = Ei, where Ei is the Fermi level of intrinsic Si, and vt = 107 cm/s. Solution: In equilibrium, the generation G = 1021 cm−3/s and recombination R rates are equal ๐ ๐ − ๐๐๐ ๐๐ ๐๐ ๐ฎ๐ = ๐น = ≈ = ๐๐ (๐ + ๐๐ ) + ๐๐ (๐ + ๐๐ ) ๐๐ ๐ + ๐๐ ๐ ๐ (๐ + ๐) Here we used ๐๐ = ๐๐ = ๐ = (Ntvtσn)−1 = 10−6 sec. In n-type Si under illumination, n = Nd + โn, p ≈ โp = โn. Thus, (๐ต๐ + โ๐) โ๐ ๐ฎ๐ป = ๐ต๐ + ๐ โ๐ Solving this equation with respect to โn we obtain p = โn = 1.1×1015 cm−3 and n = 1.1×1016 cm−3. SOLVED PROBLEMS The reverse saturation current at 3ooK of a p-n Ge diode is 5 uA . Find the voltage to be applied across the junction to obtain a forward current of 50 mA. Solution ๐ฐ = ๐ฐ๐ [๐๐๐ ( ๐๐ฝ ) − ๐] ๐ฒ๐ป So, ๐๐ฝ ๐ฐ ๐๐ ๐ ๐๐−๐ ๐๐๐ ( ) = + ๐= + ๐ = ๐๐๐ −๐ ๐ฒ๐ป ๐ฐ๐ ๐ ๐ ๐๐ Or , ๐ฒ๐ป ๐. ๐๐ ๐ ๐๐−๐๐ ๐ ๐๐๐ ๐ ๐ฝ= ๐๐ ๐๐ = ๐ ๐. ๐๐๐ ๐ ๐ = ๐. ๐๐๐ ๐ฝ๐๐๐ ๐ ๐. ๐ ๐ ๐๐−๐๐ Problem (3) 3. A p+-n Si junction (ni = 1.05×1010 cm−3, ฯตSi = 11.9) is formed in an ntype substrate with Nd = 1015 cm−3. If the junction contains 1015 cm−3 generation-recombination centers located at the intrinsic Fermi level with σn = σp = 10−15 cm2 (vt = 107 cm/s), calculate generation current density at a reverse bias of 10 V. Solution: Generation current in the space charge region w is given by ๐ ๐๐ ๐ ๐๐ = ๐๐ Here, ๐−1 = Ntσnvt = 107 s−1. The width w of the space charge region for a p+-n junction under reverse bias is ๐⁄ ๐⁄ ๐ ๐ (๐๐ − ๐ฝ) ๐ ๐ (๐ฝ) ๐= { } ≈ { } = ๐. ๐ ๐๐ ๐ ๐ ๐๐ต๐ ๐ ๐ ๐ ๐ต๐ Here we used relation |V|โซ๐๐ . From here we obtain that jg = 3 µA/cm2. Problem (4) For a p-n Si junction with the p-side doped to 1017 cm−3, the n-side doped to 1019 cm−3 (n+-p junction), and a reverse bias of −2 V, calculate the generation current density at room temperature, assuming that the e๏ฌective lifetime is 10−5 s. Solution: Using the formulae of the previous problem and relation ๐ฒ๐ป ๐ต๐ ๐๐ = ๐๐ ( ๐ ) ๐ ๐๐ 2 we get js = 1.6 nA/cm . Problem (5) For a p-n GaAs junction at room temperature ๏ฌnd the donor/acceptor concentration at which de Broglie wavelength ๐๐ ๐ (๐ = ) √๐ ๐∗ ๐ฌ ๐๐ฒ๐ป ๐∗๐ ๐∗๐ = ๐. ๐๐ , = ๐. ๐๐ ๐๐๐ ๐๐ฎ๐๐จ๐ = ๐๐. ๐ , ๐๐ฎ๐๐จ๐ (๐ฌ = ), ๐ ๐ ๐๐ ๐๐ = ๐. ๐ ๐ ๐๐๐ ๐๐−๐ ๐๐๐ ๐ต๐จ = ๐ต๐ซ Solution: From the parameters given, we ๏ฌnd λn = 2.5×10−6 cm and λp = 8.5×10−7 cm. If Nd = Na = N the width of the space charge region is ๐๐๐ ๐⁄๐ ๐= { } ๐ ๐๐ต By de๏ฌnition, w = λ. Substituting ๐ฒ๐ป ๐ต๐ ๐๐ = ๐๐ ( ๐ ) ๐ ๐๐ into the expression above and after some simpli๏ฌcations, we get ๐ ๐ ๐ฒ๐ป ๐ต ๐ต= ๐๐ ( ) ๐ ๐ ๐๐ ๐ ๐๐ Solving the above equation numerically, we obtain N = 6.8 × 1018 cm−3 and 6.2×1019 cm−3 for electron and holes, respectively. Problem (6) When a silicon p+-n junction is reverse-biased to 30 V, the depletionlayer capacitance is 1.75 nF/cm2. If the maximum electric ๏ฌeld at avalanche breakdown is 3×105 V/cm, ๏ฌnd the breakdown voltage. ฯตSi = 11.9. Solution: Since C = ๐ /4πw0, and under strong reverse bias w0 ≈ (๐ V/2πeNd)1/2, we obtain Nd = 1.1×1015 cm−3. Maximum electric ๏ฌeld is at the interface and for a p+-n junction equals E ≈ 4πeNdw1/๐. From conditions of the problem we ๏ฌnd that at the breakdown w 1 = 18 µm and, hence, the breakdown voltage is 273 V . Problem (7) For a p+-n Si junction with Nd = 1016 cm−3, the breakdown voltage is 32 V. Calculate the maximum electric ๏ฌeld at the breakdown. ฯตSi = 11.9 Solution: The width of the space charge region is w ≈ (๐ V/2πeNd)1/2 = 2 µm. From here we get that the maximum electric ๏ฌeld at the breakdown is ๐ ๐ ๐ ๐ต๐ ๐ฌ= ๐ = ๐ ๐ ๐๐๐ ๐ฝ⁄๐๐ ๐ 1.4 Non ideal p-n Junction 1. n-Si with Nd = 7 × 1015 cm−3 additionally contains Nt = 1015 cm−3 generation recombination centers located at the intrinsic Fermi level with σn = σp = 10−15 cm2 and vt = 107 cm/s. Calculate generation rate, if 1. n and p are low as compared to the equilibrium value 2. only p is below the equilibrium value. For Si, ni = 1.05 × 1010 cm−3. Solution: (4.1) By definition ๐๐๐ − ๐๐ ๐ฎ๐ = − ๐น๐ = ๐๐ (๐ + ๐๐ ) + ๐๐ (๐ + ๐๐ ) where −๐ ๐ ๐−๐ ๐ = ๐๐ = ๐๐ ๐๐ ๐๐ = ๐๐ /๐๐๐ In the first case n and p are less than ni. Thus, np < ๐๐๐ and hence , ๐๐๐ ๐๐ ๐๐ ๐๐−๐⁄ ๐ฎ๐ = (๐ = = ๐, ๐ ๐ ๐๐ ๐๐๐ ๐๐ ๐ + ๐ ๐ ) ๐ ๐๐ In the second case n = Nd โซ ni, whereas p < ni, hence ๐๐๐ ๐๐๐ ๐๐๐ −๐ ๐ฎ๐ = = = = ๐, ๐ ๐ ๐๐๐๐ ๐๐ ⁄๐๐๐ ๐๐ (๐ + ๐๐ + ๐๐ ) ๐ ๐๐ ๐๐ ๐ต๐ 2. Illumination of n-type Si (Nd = 1016 cm−3) generates 1021 cm−3/s electron-hole pairs. Si has Nt = 1015 cm−3 generationrecombination centers with σn = σp = 10−16 cm2. Calculate equilibrium concentration of electrons and holes if Et = Ei, where Ei is the Fermi level of intrinsic Si, and vt = 107 cm/s. Solution: (4.2) In equilibrium, the generation G = 1021 cm−3/s and recombination R rates are equal, ๐ ๐ − ๐๐๐ ๐๐ ๐ฎ = ๐น = ≈ ๐๐ (๐ + ๐๐ ) + ๐๐ (๐ + ๐๐ ) ๐๐ ๐ + ๐๐ ๐ = (๐ ๐)/๐( ๐ + ๐) Here we used ๐๐ = ๐๐ = ๐ = (Nt vt σn)−1 = 10−6 sec. In n-type Si under illumination, n = Nd + Δn , p ≈ Δp = Δn. Thus, (๐ต๐ + โ ๐)โ๐ ๐ฎ๐ป = ๐ต๐ + ๐ โ ๐ Solving this equation with respect to Δn we obtain p = Δn = 1.1×1015 cm−3 and n = 1.1 × 1016 cm−3. 3. A p+-n Si junction (ni = 1.05×1010 cm−3, ε = 11.9) is formed in an n-type substrate with Nd = 1015 cm−3. If the junction contains 1015 cm−3 generation-recombination centers located at the intrinsic Fermi level with σn = σp = 10−15 cm2 (vt = 107 cm/s), calculate generation current density at a reverse bias of 10 V. Solution: (4.3) Generation current in the space charge region w is given by ๐ ๐๐ ๐ ๐๐ = ๐๐ Here, τ−1 = Nt σn vt = 107 s−1. The width w of the space charge region for a p+-n junction under reverse bias is ๐⁄ ๐ ⁄๐ ๐ (๐๐ − ๐ฝ) ๐ ๐ |๐ | ๐= ( ) ≈ ( ) = ๐. ๐ ๐๐ ๐ ๐ ๐ต๐ ๐ ๐ ๐ ๐ต๐ Here we used relation |V | โซ ๐๐ . From here we obtain that jg = 3 μA/cm2. 4. For a p-n Si junction with the p-side doped to 1017 cm−3, the n-side doped to 1019 cm−3 (n+-p junction), and a reverse bias of −2 V, calculate the generation current density at room temperature, assuming that the effective lifetime is 10−5 s. Solution: (4.4) Using the formulae of the previous problem and relation ๐ฒ๐ป ๐๐ ๐๐ = ๐๐ ( ๐ ) ๐ ๐๐ we get js = 1.6 nA/cm2. 5. For a p-n GaAs junction at room temperature find the donor/acceptor concentration at which de Broglie wavelength (λ = 2πh /√2m* E) of electrons/holes is equal to the width of the space charge region. Assume <Ei > 3 kT/2, m*e/m0 = 0.063, m*h/m0 = 0.53, and εGaAs = 12.9, nGaAsi = 2.1 × 106 cm−3, and Na = Nd. Part (14) Solved PROBLEMS The transition capacitance , The diffusion capacitance Example 4.5 a. Calculate the diffusion capacitance of the diode described in Example 4.4 at zero bias. Use µn = 1000 cm2/V-s, µp = 300 cm2/V-s, wp' = 1 µm and wn' = 1 mm. The minority carrier lifetime equals 0.1 ms. b. For the same diode, find the voltage for which the junction capacitance equals the diffusion capacitance. Solution a. The diffusion capacitance at zero volts’ equals ๐ฐ๐,๐ ๐๐ ๐ฐ๐,๐ ๐๐ ๐ช๐ ,๐ = + = ๐. ๐๐ ๐ ๐๐−๐๐ ๐ญ ๐ฝ๐ ๐ฝ๐ Using ๐จ๐๐๐ ๐ซ๐ ๐ฐ๐,๐ = ๐ ๐ณ๐ And , ๐จ๐๐๐ ๐ซ๐ ๐ฐ๐๐ = ๐ ๐พ๐ Where the "short" diode expression was used for the capacitance associated with the excess charge due to electrons in the p-type region. The "long" diode expression was used for the capacitance associated with the excess charge due to holes in the n-type region. The diffusion constants and diffusion lengths equal Dn = µn x Vt = 25.8 cm2/s Dp = µp x Vt = 7.75 cm2/s ๐ณ๐ = √๐ซ๐ ๐๐ And the electron transit time in the p-type region equals ๐๐๐ ๐๐,๐ = = ๐๐๐ ๐๐ ๐ ๐ซ๐ b. The voltage at which the junction capacitance equals the diffusion capacitance is obtained by solving ๐ช๐๐ √๐ − ๐ฝ๐ = ๐ช๐ ,๐ ๐ฝ๐ ⁄ ๐ ๐ฝ๐ ๐๐ yielding Va = 0.442 V 2. For the p-n Si junction from the previous problem calculate the width of the space charge region for the applied voltages V = −10, 0, and +0.3 V. εSi = 11.9 Solution: (3.2) Taking into account that at room temperature all donors and acceptors are ionized, i.e. n = Nd and p = Na, from the values found in the previous problem and ๐⁄ ๐(๐๐ − ๐ฝ) ๐ต๐ + ๐ต๐ ๐ ๐= ( ) ๐๐ ๐ ๐ต๐ ๐ต๐ we get ω(−10V) = 2 μm , ω(0V) = 0.5 μm , and ω(+0.3V) = 0.4 μm. 3. For the parameters given in the previous problem find the maximum electric field within the space charge region. Compare these values with the electric field within a shallow donor: E ≈ e/εSia2B, where aB is the Bohr radius of a shallow donor, aB =εSih2 /m* e e2 and me /mo = 0.33. Solution: (3.3) ๐⁄ ๐ ๐ ๐ ๐ (๐๐ − ๐ฝ) ๐ต๐ ๐ต๐ ๐ฌ=๐ ( ) ๐ ๐ต๐ + ๐ต๐ we obtain that E(−10V) = 105 V/cm, E(0V) = 2.6×104 V/cm, and E(+0.3V) = 2 × 104 V/cm. The electric field within a shallow donor is, in turn, E ≈ 3.4 × 105 V/cm, that is, comparable to that of the p-n junction. 4. Calculate the capacity of the p-n junction from the problem 2 if the area of the junction is 0.1 cm2. Solution: (3.4) ๐๐ ๐= . ๐๐๐ we get C(−10V) = 0.5 nF, C(0V) = 2 nF, and C(+0.3V) = 2.6 nF. 5. n-Si of a p-n Si junction has a resistivity of 1 ฮcm. What should be the resistivity? of p-Si so that 99 % of the total width of the space charge region would be located in n-Si (p+-n junction)? For the parameters needed see problem 1. Solution: (3.5) From the conditions of the problem ωa = 0.01ω and ωd = 0.99ω. Since ωa/ωd = Nd/Na , we get that Na = 99 Nd. Because Nd = 1/eρμn = 4.5 × 1015 cm−3, we get Na = 4.4 × 1017 cm−3. Solution: (4.5) From the parameters given, we find λn = 2.5 × 10−6 cm and λp = 8.5 × 10−7 cm. If Nd = Na = N the width of the space charge region is ๐⁄ ๐ ๐๐ ๐ ๐= ( ) ๐ ๐๐ต By definition, w = λ. Substituting ๐ฒ๐ป ๐ต๐ ๐๐ = ๐๐ ( ๐ ) ๐ ๐๐ into the expression above and after some simplifications, we get ๐ ๐ ๐ฒ๐ป ๐ต ๐ต= ๐๐ ( ) ๐ ๐๐๐ ๐ ๐๐ Solving the above equation numerically, we obtain N = 6.8 × 1018 cm−3 and 6.2 × 1019 cm−3 for electron and holes, respectively. 6. When a silicon p+-n junction is reverse-biased to 30 V, the depletion-layer capacitance is 1.75 nF/cm2. If the maximum electric field at avalanche breakdown is 3 × 105 V/cm, find the breakdown voltage. εSi = 11.9. Solution: (4.6) Since C = ฯต / 4 π w0, and under strong reverse bias w0 ≈ (ฯต V / 2 π e Nd)1/2, we obtain Nd = 1.1 × 1015 cm−3. Maximum electric field is at the interface and for a p+-n junction equals E ≈ 4 π e Nd w1 / ฯต. From conditions of the problem we find that at the breakdown w1 = 18 μm and, hence, the breakdown voltage is 273 V . 7. For a p+-n Si junction with Nd = 1016 cm−3, the breakdown voltage is 32 V. Calculate the maximum electric field at the breakdown. εSi = 11.9. Solution: (4.7) The width of the space charge region is w ≈ (ฯตV / 2πeNd)1/2= 2 μm. From here we get that the maximum electric field at the breakdown is ๐๐๐๐๐ ๐ฌ= ๐ ≈ ๐ ๐ฑ ๐๐๐ ๐ฝ⁄๐๐ ๐ Problem:2 A Si p-n junction has dopant concentrations ND = 2 x 1015 cm-3 and NA = 2 x 1016 cm-3. Calculate the built-in potential Vbi in eV and the total width of the depletion region W = xn0 + xp0 at zero bias (that is, Va = 0) and under a reverse bias Va = - 8V. Solution: (a) Given ni = 1:5 x 1010 cm-3, the build-in potential is: ๐ฒ๐ป ๐ต๐จ ๐ต๐ซ ๐ฒ๐ป ๐๐ ๐ฅ๐ง = ๐ฅ๐ง = ๐. ๐๐๐ ๐๐ฝ ๐ ๐ ๐๐ ๐๐๐ The depletion width with a bias Va is give by: ๐ฝ๐๐ = (b) ๐ ๐๐ (๐ฝ๐๐ − ๐ฝ๐ ) ๐ ๐ ๐พ= √ ( + ) ๐ ๐ต๐จ ๐ต๐ซ For Va = 0V , we have W = 0:691µm and for Va = - 8V , we have W = 2:475 µm. Problem: 3 A Si p-n junction is reverse-biased with Va = -10V . Determine the percent change in junction (depletion) capacitance and built-in potential if the doping in the p region is increased by a factor of 2. Solution: Let us assume the NA and ND values are ND = 2 x 1015 cm-3 and NA = 2 x 1016 cm-3 , then the build-in potential is calculated by the equation, we have: ๐ฝ๐๐ = ๐ฒ๐ป ๐ต๐จ ๐ต๐ซ ๐ฒ๐ป ๐๐ ๐ฅ๐ง = ๐ฅ๐ง = ๐. ๐๐๐ ๐๐ฝ ๐ ๐ ๐๐ ๐๐๐ and ๐ฒ๐ป ๐ ๐ต๐จ ๐ต๐ซ ๐ฅ๐ง ( ) = ๐: ๐๐๐๐ ๐๐ฝ ๐ ๐๐๐ Therefore, Vbi is increased by 2:67%. The depletion capacitance can be calculated by ๐๐จ ๐ช๐ = ๐พ Where A is the cross-sectional area of the junction and W is the depletion width calculated by: ๐ฝ๐๐ = ๐พ= √ ๐พ= √ ๐ ๐๐ (๐ฝ๐๐ − ๐ฝ๐ ) ๐ ๐ ๐๐ (๐ฝ๐๐ − ๐ฝ๐ ) ๐ ๐ (๐ต + ๐จ ๐ ๐ ๐ต๐ซ (๐ ๐ต + ๐จ ) = 2:7549 µm ๐ ๐ต๐ซ ) = 2:6938 µm Therefore, the percent change in junction depletion capacitance is given by: ๐ช,๐ − ๐ช๐ ๐ − ๐. = = ๐. ๐๐ % ๐ช๐ ๐. Switching time Example 1.8 Determine the current ID and the diode voltage VD for the circuit shown with VDD=5V and R=1 K . Assume that the diode has a current of 1 mA at a voltage of 0.7V and that its voltage drop changes by 0.1V for every decade change in current. To begin the iteration, we assume that VD = 0.7 V and use the next equation to determine the current. ID R + vd - VDD Assuming that VDD is greater than 0.5 V or so, the diode current will be much greater than Is, and we can represent the diode i-v characteristic by the exponential relationship, resulting in ๐ฝ๐ซ ⁄ ๐ ๐ผ ๐ฝ๐ป ๐ฐ๐ซ = ๐ฐ๐ The other equation that governs circuit operation is obtained by writing a Kirchhoff loop equation, resulting in ๐ฝ๐ซ๐ซ − ๐๐ซ ๐ฐ๐ซ ๐น Assuming that the diode parameters Is and n are known , the two equations above has two unknown quantities ID and VD. Two alternative ways for obtaining the solution are graphical analysis and iterative analysis. Graphical Analysis Using the Exponential Model i VDD/R ID Load line Diode characteristics Q operating point Graphical analysis is performed by plotting the relationships of the used equations above on the i-v plane. The solution can then be obtained as the coordinates of the point of intersection of the two graphs. A sketch of the graphical construction is shown. The curve represents the exponential diode equation, and the straight line is known as the l o a d line. The load line intersects the diode curve at point Q, which represents the operating point of the circuit. Its coordinates give the values of ID and VD. Example 1.8 Determine the current ID and the diode voltage VD for the circuit shown ID R VDD + vd - With VDD=5V and R = 1 K . Assume that the diode has a current of 1 mA at a voltage of 0.7V and that its voltage drop changes by 0.1V for every decade change in current. To begin the iteration, we assume that VD = 0.7 V and determine the current ๐ฝ๐ซ๐ซ − ๐๐ซ ๐ − ๐. ๐ ๐ฐ๐ซ = = ๐. ๐ ๐๐จ ๐น ๐ We then use the diode equation to obtain a better estimate for VD. This can be done by employing Eq. as ๐ ๐ฝ๐ − ๐ฝ๐ = ๐๐ ๐ผ ๐ฝ๐ป ๐๐๐ ๐⁄๐ ๐ ๐ ๐๐ ๐ผ ๐ฝ๐ป = ๐. ๐ ๐ฝ , ๐๐๐๐ ๐ฝ๐ = ๐ฝ๐ + ๐. ๐ ๐๐๐ ๐⁄๐ ๐ Substituting V1 = 0.7 V, I1 = 1 mA, and I2 = 4.3 mA results in V2 = 0.763 V. Thus the results of the first iteration are ID = 4.3 mA and VD = 0.763 V. The second iteration proceeds in a similar manner: ๐ฝ๐ซ๐ซ − ๐๐ซ ๐ − ๐. ๐๐๐ ๐ฐ๐ซ = = ๐. ๐๐๐ ๐๐จ ๐น ๐ ๐. ๐๐๐ ๐ฝ๐ = ๐. ๐๐๐ + ๐. ๐ ๐๐๐ = ๐. ๐๐๐ ๐ฝ ๐. ๐ Thus the second iteration yields ID = 4.237 mA and VD = 0.762 V. Since these values are not much different from the values obtained after the first iteration, no further iterations are necessary, and the solution is ID = 4.237 mA and VD = 0.762 V. Example 11 The dc power supply circuit of figure shown is to be designed for the following specifications: dc output voltage = +15 V, dc load current = 100 mA, and percent ripple = 5%. The rectifier diode can be modeled with the parameters VD0 = 0.7 V and RD = 0. Calculate the required transformer secondary ac rms voltage and the value of the filter capacitor. Assume a frequency f = 60 Hz. iL (t) + To AC Power Line + vS (t) C - RL vL(t) - Solution. The peak secondary transformer voltage is given by V1 = 15+0.7 = 15.7 V. The ac rms voltage is 15.7/ √ 2 = 11.1 V rms. The effective value of the load resistor is RL = 15 / 0.1 = 150 โฆ. The value of C can be −๐ป calculated form equation ๐ท๐๐๐๐๐๐ ๐น๐๐๐๐๐ ≤ [๐ − ๐๐๐ ( )] ๐ ๐๐๐ % ๐น๐ณ ๐ช Where equality used. We obtain ๐⁄ ๐ป −๐ −๐ ๐๐ ๐ช= = = ๐๐๐๐ ๐๐ญ ๐น๐ณ ๐๐ (๐ − % ๐๐๐๐๐๐) ๐๐๐ ๐๐ (๐ − ๐⁄ ) ๐๐๐ ๐๐๐ If follows from the inequality equation ๐ท๐๐๐๐๐๐ ๐น๐๐๐๐๐ ≤ [๐ − −๐ป ๐๐๐ ( )] ๐ ๐๐๐ % that this value for C gives a percent ripple that is ๐น ๐ช ๐ณ less than 5%. Part (15) Solved PROBLEMS photoelectric effect Problem (1) (a) An electron beam strikes a crystal of cadmium sulfide (CdS). Electrons scattered by the crystal move at a velocity of 4.4 x 105 m/s. Calculate the energy of the incident beam. Express your result in eV. CdS is a semiconductor with a band gap, Eg, of 2.45 eV. (b) Cadmium telluride (CdTe) is also a semiconductor. Do you expect the band gap of this material to be greater or less than the band gap of CdS? Explain. Solution (a) Escattered eEincident e - scattered Eg Eemitted photons e-incident CdS crystal ๐ฌ๐๐๐๐๐ ๐๐๐ ๐− = ๐ฌ๐๐๐๐๐๐๐ ๐ + ๐ฌ๐๐๐๐๐๐๐๐๐ ๐− ๐ ๐๐ = ๐ฌ๐ + ๐ −๐๐ ๐ฌ๐๐๐๐๐ ๐๐๐ ๐− = ๐. ๐๐ ๐๐ฝ + ๐๐ ๐ (๐. ๐ ๐ ๐ ๐. ๐๐ ๐ ๐๐ ๐ ๐๐ฝ ๐ ๐. ๐ ๐ ๐๐−๐๐ ๐ ๐๐ ๐๐ ) ๐ ๐ฑ = ๐. ๐๐ ๐๐ฝ + ๐. ๐๐ ๐๐ฝ = ๐ ๐๐ฝ (b) Eg(CdTe) <Eg(CdS) The Cd–S bond is stronger than Cd–Te bond because although both S and Te are group 16, Te is much larger than S. Problem #8 The energy gap (Eg) of ZnSe is 2.3 eV. (a) Is this material transparent to visible radiation? Substantiate your answer. (b) How could you increase the electrical conductivity of this material? Give the reasons for the effectiveness of your suggested approach. Solution ส (Ao) CB E(hv) 4000 5397 7000 Eg= 2.3 eV E 3.1 Blue green Absorb yellow red Absorbed 1 0 2.3 2.26 1.77 E (eV) transmitted 5397 ส (Ao) wave length (a) The optical properties of ZnSe can be explained when comparing the energy band of the visible spectrum with the energy band diagram of ZnSe. Absorption takes place via photo excitation for all radiation with E ≥ 2.3 eV. From the energy distribution of the visible spectrum we recognize that the blue– green portion has photon energies in excess of the band gap (Eg = 2.3eV) and thus will be absorbed. The yellow–red potion, on the other hand, has photon energies less than the band gap – it will be transmitted. ZnSe, therefore, is expected to exhibit a yellowish–red color. (b) In principle there are two ways to increase the electrical conductivity of ZnSe: a. A temperature rise. Any rise in temperature will increase the number of “thermally activated” charge carriers in the conduction band (electrons) and in the valence band (holes) and, thus, the electronic conductivity. Aside: The electrical conductivity of solids, demonstrated by the flow of electronic charge carriers under an applied electric field (E), can be formulated through Ohm’s law, J = σE, which states that the current density (J = number of charges transported through a unit area in a unit time) is proportional (σ = conductivity) to the applied electric field. Accordingly: ๐ฑ = ๐ต ๐ ๐๐ where N = number of charge carriers/unit volume, e = electronic charge and vd = average drift velocity of charge carriers in an applied electric field. We thus obtain: ๐ต ๐ ๐๐ ๐= ๐ฌ and if we define d(v /E) = μ, the charge carrier mobility, we have: σ=Neμ In intrinsic semiconductors we have both electrons and holes contributing to conduction: eenheh σ = Ne e μe + Nneμh = Ne(μe + μh ) since Ne = Nh. Taking the number of thermally generated charge carriers, given by the relationship ๐ −๐ฌ๐ ๐ต = ๐จ๐ป ⁄๐ ๐ ⁄๐ ๐ฒ๐ป we obtain the temperature dependence of the conductivity as: ๐ −๐ฌ๐ ๐ = ๐จ๐ป ⁄๐ ๐ ⁄๐ ๐ฒ๐ป ๐ ๐ (๐๐ + ๐๐ ) To assess the temperature dependence of electrical conductivity we must take into consideration that, because of increased vibration of the atoms about their lattice positions, the charge carrier mobility will decrease (increased scattering of charge carriers) with increasing temperature. This effect explains why the electronic conductivity in metals, where N is constant, will decrease with increasing temperature. In semiconductors, where N increases with temperature, the accompanying mobility effect is not apparent at low temperatures (conductivity increases), but becomes pronounced at high temperatures (conductivity decreases). b. Introduction of shallow impurity (or defect) states close to the conduction or valence band. This is accomplished by the incorporation of appropriate dopant elements into the crystal matrix. If these impurities are shallow (~0.01 eV from the conduction or valence band), they will be totally ionized at room temperature and each will contribute an electron (donor dopant: K, Na) or holes (acceptor dopant: G, Br), thus increasing the electrical conductivity without the necessity of a temperature rise. (Be aware that certain defects in the crystal lattice may also increase the electronic conductivity.) 9. Electron mobility in Si is 1400 cm2 V−1s−1. Calculate the mean free time in scattering (Relaxations time) of electrons. E๏ฌective mass is m∗e/m0 = 0.33. Solution: From µ = eτ/m∗ we get that τ = 2.6×10−13 s. Example 1.1 A metal has a work function of 4.3 V. What is the minimum photon energy in Joule to emit an electron from this metal through the photo-electric effect? What are the photon frequency in Terahertz and the photon wavelength in micrometer? What is the corresponding photon momentum? What is the velocity of a free electron with the same momentum? Solution The minimum photon energy, Eph, equals the work function, ΦM, in units of electron volt or 4.3 eV. This also equals: ๐ฌ๐๐ = ๐ ๐๐ = ๐. ๐ ๐ ๐๐−๐๐ ๐ ๐. ๐ = ๐. ๐๐ ๐ ๐๐−๐๐ The corresponding photon frequency is: ๐. ๐๐ ๐ ๐๐−๐๐ ๐๐๐ = = ๐๐๐๐ ๐ป๐ฏ๐ ๐. ๐๐๐ ๐ ๐๐−๐๐ The corresponding wavelength equals: ๐๐ ๐. ๐๐๐ ๐ ๐๐−๐๐ ๐ ๐ ๐ ๐๐๐ ๐. ๐๐ ๐ ๐= = = = ๐. ๐๐๐ ๐๐ ๐ฌ๐๐ ๐. ๐๐ ๐ ๐๐−๐๐ ๐ฌ๐๐ (๐๐ฝ) The photon momentum, p, is: ๐ ๐. ๐๐๐ ๐ ๐๐−๐๐ ๐= = = ๐. ๐๐๐ ๐ ๐๐−๐๐ ๐๐ ๐/๐ −๐ ๐ ๐. ๐๐๐ ๐ ๐๐ And the velocity, v, of a free electron with the same momentum equals: ๐ ๐. ๐๐๐ ๐ ๐๐−๐๐ ๐= = = ๐๐๐๐ ๐/๐ ๐๐ ๐. ๐๐ ๐ ๐๐−๐๐ Where mo is the free electron mass ๐ฌ๐๐ = ๐ ๐๐ = ๐. ๐ ๐ ๐๐−๐๐ ๐ ๐. ๐ = ๐. ๐๐ ๐ ๐๐−๐๐ Example 1.2 (the blackbody radiation) The spectral density of the sun peaks at a wavelength of 900 nm. If the sun behaves as a black body, what is the temperature of the sun? Solution: A wavelength of 900 nm corresponds to a photon energy of: ๐ฌ๐๐ ๐ ๐ ๐. ๐๐๐ ๐ ๐๐−๐๐ ๐ ๐ ๐ ๐๐๐ = = = ๐. ๐๐ ๐ ๐๐−๐๐ ๐ฑ๐๐๐๐ −๐ ๐ ๐๐๐ ๐ ๐๐ Since the peak of the spectral density occurs at 2.82 kT, the corresponding temperature equals: ๐ฌ๐๐ ๐. ๐๐ ๐ ๐๐−๐๐ ๐ป= = = ๐๐๐๐ ๐ฒ๐๐๐๐๐ ๐. ๐๐ ๐ ๐. ๐๐ ๐ ๐. ๐๐ ๐๐๐−๐๐ Example 1.3 An electron is confined to a 1 micron thin layer of silicon. Assuming that the semiconductor can be adequately described by a one-dimensional quantum well with infinite walls, calculate the lowest possible energy within the material in units of electron volt. If the energy is interpreted as the kinetic energy of the electron, what is the corresponding electron velocity? (The effective mass of electrons in silicon is 0.26 m0, where m0 = 9.11 x 10-31 kg is the free electron rest mass). Solution: The lowest energy in the quantum equals: ๐ ๐ (๐. ๐๐๐ ๐ ๐๐−๐๐ )๐ ๐๐ ๐ ๐ ๐ฌ๐ = ( ) = ( ) ๐ ๐∗ ๐ ๐ณ๐ ๐ ๐ ๐. ๐๐ ๐ ๐. ๐๐ ๐ ๐๐−๐๐ ๐ ๐ ๐๐−๐ = ๐. ๐๐๐ ๐๐−๐๐ ๐๐๐๐๐ = ๐. ๐๐ ๐๐๐ฝ Then velocity of an electron with this energy equal: ๐๐ฌ๐ ๐ ๐ ๐. ๐๐ ๐ ๐๐−๐๐ ๐= √ ∗ = √ = ๐. ๐๐๐ ๐๐/๐ ๐ ๐. ๐๐ ๐ ๐. ๐๐ ๐ ๐๐−๐๐ Example 1.4 Consider an infinitely long cylinder with charge density r, dielectric constant ε0 and radius r0. What is the electric field in and around the cylinder? Solution: Because of the cylinder symmetry one expects the electric field to be only dependent on the radius, r. Applying Gauss's law one finds: ๐ธ ๐ ๐ ๐๐ ๐ณ โ โ โ๐จ= ๐บ๐๐ ๐๐ณ= ๐บ = ๐บ๐ ๐บ๐ And ๐ธ ๐ ๐ ๐๐๐ ๐ณ โโ = ๐บ ๐ ๐ ๐ ๐ณ = โ๐จ ๐บ = ๐บ๐ ๐บ๐ Where a cylinder with length L was chosen to define the surface A and edges effects were ignored. the electric field then equal: ๐๐ ๐บ(๐) = ๐ ๐บ๐ The electric field increases with the cylinder with increasing radius. The electric field decreases outside with the cylinder with increasing radius. Problem 1.1 Calculate the wavelength of a photon with a photon energy of 2 eV. Also, calculate the wavelength of an electron with a kinetic energy of 2 eV. Solution The wavelength of a 2 eV photon equals: ๐๐ช ๐. ๐๐๐ ๐ ๐๐−๐๐ ๐ฑ ๐ ๐ ๐ ๐๐๐ ๐/๐๐๐ ๐๐๐๐ซ๐จ๐ ๐ฅ๐ข๐๐๐ = = ๐ฌ๐๐ ๐. ๐๐๐ ๐ ๐๐−๐๐ ๐⁄๐ ๐๐ฝ = ๐. ๐๐ ๐๐ where the photon energy (2 eV) was first converted to Joules by multiplying with the electronic charge. The wavelength of an electron with a kinetic energy of 2 eV is obtained by calculating the deBroglie wavelength: ๐ ๐. ๐๐๐ ๐ ๐๐−๐๐ ๐ฑ ๐๐๐๐ซ๐จ๐ ๐ฅ๐ข๐๐๐ = = = ๐. ๐๐๐๐ ๐๐ ๐⁄ ๐ −๐๐ ๐. ๐๐ ๐ ๐๐ ๐ Where the momentum of the particle was calculated from the kinetic energy: ๐ = √๐ ๐ ๐ฌ = √๐ ๐ ๐. ๐๐ ๐ ๐๐−๐๐ ๐๐ ๐ ๐. ๐ ๐ ๐๐−๐๐ ๐ ๐ ๐ ๐๐ฝ = ๐. ๐๐ ๐ ๐๐−๐๐ ๐๐ ๐/๐ Problem 1.2 Consider a beam of light with a power of 1 Watt and a wavelength of 800 nm. Calculate a) the photon energy of the photons in the beam, b) the frequency of the light wave and c) the number of photons provided by the beam in one second. Solution The photon energy is calculated from the wavelength as: ๐๐ช ๐. ๐๐๐ ๐ ๐๐−๐๐ ๐ฑ๐ ๐ ๐ ๐ ๐๐๐ ๐/๐ ๐ฌ๐๐ = = ๐๐๐๐ซ๐จ๐ ๐ฅ๐ข๐๐๐ ๐๐๐ ๐ ๐๐−๐ ๐ = ๐. ๐๐ ๐ ๐๐−๐๐ ๐ฑ or in electron Volt: ๐. ๐๐๐ ๐๐−๐๐ ๐ฑ ๐ฌ๐๐ = = ๐. ๐๐๐๐ฝ ๐. ๐ ๐ ๐๐−๐๐ ๐ The frequency then equals: ๐ฌ๐๐ ๐. ๐๐ ๐ ๐๐−๐๐ ๐ฑ ๐= = = ๐๐๐ ๐ป๐ฏ๐ ๐ ๐. ๐๐๐ ๐ ๐๐−๐๐ ๐ฑ๐ And the number of photons equals the ratio of the optical power and the energy per photon: ๐ ๐๐๐๐ ๐ ๐๐๐๐ โ ๐๐๐๐๐๐๐ = = = ๐ ๐ ๐๐๐๐ −๐๐ ๐ฌ๐๐ ๐. ๐๐ ๐ ๐๐ ๐ฑ Problem 1.3 Show that the spectral density, uw(equation 1.2.4) peaks at Eph = 2.82 kT. Note that a numeric iteration is required. Solution The spectral density, uw, can be rewritten as a function of โ๐ ๐= ๐ฒ๐ป ๐ ๐ ๐ฒ ๐ป ๐๐ ๐๐ = ๐ ๐ ๐ โ ๐ ๐ ๐๐๐ (๐) − ๐ The maximum of this function is obtained if its derivative is zero or: ๐ ๐๐ ๐ ๐๐ ๐๐ ๐๐๐ (๐) = − =๐ ๐ ๐ ๐๐๐ (๐) − ๐ (๐๐๐ (๐) − ๐)๐ Therefore ๐ must satisfy: ๐ − ๐ ๐๐๐ (− ๐) = ๐ This transcendental equation can be solved starting with an arbitrary positive value of ๐. A repeated calculation of the left hand side using this value and the resulting new value for ๐ quickly converges to ๐max = 2.82144. The maximum spectral density therefore occurs at: ๐ฌ๐๐ ๐๐๐ = ๐๐๐๐ ๐ฒ๐ป = ๐. ๐๐๐๐๐ KT Problem 1.4 Calculate the peak wavelength of blackbody radiation emitted from a human body at a temperature of 37°C. Solution The peak wavelength is obtained through the peak energy ๐๐ช ๐๐ช ๐๐๐๐ซ๐จ๐ ๐ฅ๐ข๐๐๐ = = ๐ฌ๐๐ ๐๐๐ ๐. ๐๐ ๐ฒ๐ป ๐. ๐๐๐ ๐ ๐๐−๐๐ ๐ ๐ ๐ ๐๐๐ = = ๐. ๐๐ ๐ ๐๐−๐ ๐๐ −๐๐ ๐. ๐๐ ๐ ๐. ๐๐ ๐ ๐๐ ๐ ๐๐๐. ๐๐ Where the temperature was first converted to units Kelvin. Small signal Example In the circuit shown, a sinusoidal signal voltage is used to charge a 12-V car battery. The source voltage has amplitude of 20 V that is shown in Fig. 2.1.5(a). Find the values of iD and vD and sketch their waveforms. Also, find the average value of the current charging the battery. R = 100 Ω VS(t) iD + vD - 12 V In volts VS(t) 20 10 0 -10 -20 θ θ1 θ2 π 2 π θ3 θ4 3 π 4π Solution If the diode is forward-biased, vD = 0, and the diode current is (๐ฏ๐ฌ − ๐๐) ๐ข๐ = ๐ ๐๐๐ It is convenient to describe the time-varying source voltage as vS (θ) = 20 sin (θ), Where θ = (2 π f t) and f is the frequency. To have iD > 0 (forwardbiased), vS must be greater than 12 V; i.e. only if vS > 12 V, there is a current in the loop. Otherwise the diode will be reverse-biased and will not conduct. Thus, the sketch of the diode current is shown in Fig. (b). Clearly, the diode conducts between θ1 and θ2 during the first cycle of input sinusoid, and again between θ3 and θ4 during the second cycle. If iD > 0, vD = 0. If vS < 12 V, the diode is reverse-biased, and iD must be equal to zero. Therefore, if vS < 12 V, KVL gives ๐ฏ๐ = (๐ฏ๐ฌ − ๐๐)๐ The sketch of the waveform for vD is shown in (c). The average current can be found by finding the average value of the current during one period. First, during the first period, we observe that (๐ฏ๐ฌ − ๐๐) ๐ข๐ = ๐ , ๐๐ ≤ ๐ ≤ ๐๐ = ๐ ๐๐๐ Otherwise, Since vS (θ) = 20sin(θ), the values of the angles can be found using ๐ ๐ ๐๐ = ๐ฌ๐ข๐ง−๐ ( ) ๐๐ง๐ ๐๐ = ๐ − ๐ฌ๐จ๐ง−๐ ( ) = ๐ − ๐๐ ๐ ๐ The average value of the current is ๐−๐๐ ๐ ๐๐ ๐ฌ๐ข๐ง ๐ − ๐๐ ๐. ๐ ๐๐จ๐ฌ ๐๐ − ๐. ๐๐ ๐๐ = ∫ ๐๐ = ๐ ๐ ๐ ๐๐ ๐๐๐ ๐๐ Substituting the value of θ1 in the above equation, we find that ID = 15.51 mA. Breakdown Example An abrupt pn junction has doping densities of NA = 5x1015 atoms/cm3 and ND = 1016 atoms/cm3. Calculate the breakdown voltage if Εcrit = 3x105 V/cm. Solution ๐บ๐๐ (๐ต๐จ + ๐ต๐ซ ) ๐ ๐. ๐๐ ๐ ๐๐−๐๐ (๐ ๐ ๐๐๐๐ + ๐๐๐๐ ) ๐ฝ๐น = ๐ฌ๐๐๐ = = ๐๐ ๐ฝ ๐ ๐ ๐ต๐จ ๐ต๐ซ ๐ ๐ ๐. ๐ ๐ ๐๐−๐๐ ๐ ๐ ๐ ๐๐๐๐ ๐ ๐๐๐๐ Example Determine breakdown voltage for a pn junction shown , assume Vbi = 0.9 V P+ ND ND 16 cm-3 16 -3 10 5x 10 X=0 x= 1.3 µm cm Solution: First perform a check whether the depletion width still lies in the highly doped region or nit. If it does, then ๐บ๐ ๐พ = ๐ ๐ ๐๐๐ ๐ = ๐. ๐ ๐๐ ๐ ๐ต๐ซ This shows that the depletion width extend into the highest doped Nregion as well resulting in the following diagram. E X0 xN 2x105 N x 105 The electric field at x0 is obtained using the expression ๐บ๐ ๐พ = ๐ ๐ ๐๐๐ ๐ ๐ ๐. ๐ ๐๐ ๐ ๐ต๐ซ๐ Using the Poisson’s equation ๐๐ต − ๐๐ซ = ๐ ๐ ๐๐๐ (๐บ ๐ ๐ ๐ต๐ซ๐ ) = ๐. ๐๐ ๐๐ The area under the electric field curve will be equal to Vbi + BV , so that , BV = 40.7 V Example 6 A Zener diode at room temperature (VT = 0.0259 V) has the specifications VZ = 10 V, IZ = 10 mA , and rz = 20 โฆ. Calculate (a) the Zener breakdown ideality factor η, (b) the voltage VZ0 in the linear circuit shown, and (c) the voltage at which the breakdown current is IZ / 10. I i Vz Iz Tangent line Slope = 1/R + V - Vz0 Solution. ๐ผ๐ ๐ฝ๐ป ⁄๐ฐ be used to solve for ηz to obtain ๐ ๐ฐ๐ ๐๐ ๐๐ ๐ ๐ ๐๐ ๐ผ๐ = = = ๐. ๐๐ ๐ฝ๐ป ๐๐. ๐ ๐ (b) The voltage VZ0 is calculated from Eq. ๐ฝ๐๐ = ๐ฝ๐ − ๐ฐ๐ ๐๐ to obtain (a) Equation ๐๐ = ๐ฝ๐๐ = ๐ฝ๐ − ๐ฐ๐ ๐๐ = ๐๐ − ๐๐ ๐ ๐ ๐๐ = ๐. ๐ ๐ฝ (c) If IS << IZ, Eq. ๐ฝ ๐ + ๐ฝ๐ ๐ = ๐ฐ๐ [๐๐๐ ( ) − ๐] − ๐ฐ๐ ๐๐๐ (– ) ๐ผ ๐ฝ๐ป ๐ผ๐ ๐ฝ๐ป Can be solved for the voltage at which i = −1 mA as follows: ๐ ๐ = − ๐ฝ๐ − ๐ผ๐ ๐ฝ๐ป ๐๐ ( ) = −๐๐ − ๐. ๐๐ ๐ ๐๐. ๐ ๐ ๐ ๐๐ (๐. ๐) − ๐ฐ๐ = −๐. ๐๐ ๐ฝ The reverse-bias voltage is the negative of this, i.e. +9.54 V. Part (16) Solved PROBLEMS Schottky Diode Problem (1) Find a height of the potential barrier for a Au-n-Ge Schottky contact at room temperature (T = 293 K) if ρ = 1 โฆcm, ψAu = 5.1 eV, and χGe = 4.0 eV. Electron mobility in Ge is 3900 cm2 V−1 s−1, density of the states in the conduction band is Nc = 1.98×1015 ×T3/2 cm−3. Solution: eVd = 0.88 eV Problem (2) Calculate the depletion width for a Pt-n-Si Schottky diode (T = 300 K) at V = 0, +0.4, and −2 V. Concentration of doping impurity in Si equals 4×1016 cm−3. Work function of Pt is 5.65 eV, electron a๏ฌnity of Si is 4.05 eV, ฯตSi = 11.9, density of the states in the conduction band is Nc = 6.2×1015 ×T3/2 cm−3. Solution: w = 0.22, 0.19, and 0.34 µm for V = 0, +0.4, and −2 V, respectively Problem (3) For a Schottky contact Au-GaAs calculate the maximum electric ๏ฌeld within the space charge region at V = 0, +0.3, and −100 V. Nd = 1016 cm−3, χGaAs = 4.07 eV, ฯตGaAs = 12.9. Work function of Au is 5.1 eV, T = 300 K, density of the states in the conduction band is Nc = 8.63×1013 ×T3/2 cm−3. Solution: E = 5.1 × 104, 4.2 × 104, and 5.1 × 105 V/cm for V = 0, +0.3, and −100 V, respectively. Problem (4) What is the electric ๏ฌeld E for a Schottky diode Au-n-Si at V = −5 V at the distance of 1.2 µm from the interface at room temperature if ρ = 10โฆcm, µn = 1400 cm2 V−1 s−1, Nc = 6.2×1015 ×T3/2 cm−3. Solution: E = 2×104 V/cm. Problem (5) Find current densities j at room temperature for a Schottky diode Ptn-GaAs at V = +0.5 and −5 V if ρ = 50โฆcm. µn = 8800 cm2 V−1 s−1, mn/m0 = 0.063, work function of Pt is 5.65 eV, χGaAs = 4.07 eV, Nc = 8.63 × 1013 × T3/2 cm−3. Apply thermionic-emission theory. Solution: From n = 1/eρµn we obtain that n = 1.4×1013 cm−3. Thus, ๐ต๐ ๐ ๐๐ = ๐ ๐๐ − ๐๐ฎ๐๐จ๐ − ๐ฒ๐ป ๐๐ = ๐. ๐๐ ๐๐ฝ ๐ The average thermal velocity is ๐ ๐ฒ๐ป ๐๐ = ( ) ๐ ๐๐ ๐⁄ ๐ = ๐. ๐ ๐ ๐๐๐ ๐๐/๐ From here we get ๐ฑ๐ = From here we get ๐ − ๐ ๐๐ ๐ ๐ ๐๐ป ๐๐๐ ( ) = ๐ ๐ ๐๐−๐๐ ๐จ/๐๐๐ ๐ ๐ฒ๐ป ๐๐ฝ ) − ๐} ๐ฒ๐ป we obtain j(0.5V) = 1.5×10−13 A/cm2 and j(−5V) = js. ๐ = ๐๐ {๐๐๐ ( Problem (6) The capacitance of a Au-n-GaAs Schottky diode is given by the relation 1/C2 = 1.57×1015 −2.12×1015 V, where C is expressed in F and V is in Volts. Taking the diode area to be 0.1 cm2, calculate the barrier height and the dopant concentration. Solution: ๐๐ = 0.74 V, n = 2.8×1017 cm−3. 7. From comparison of the de Broglie wavelength of electron with the depletion width of a contact metal-n-Si, estimate the electron concentration at which Schottky diode loses its rectifying characteristics. For the estimate, assume that the height of the potential barrier a the contact is half the value of the band gap at room temperature (Eg = 1.12 eV), m∗e = m0, T = 300 K, and ฯตSi = 11.9. Solution: A Schottky diode loses its rectifying characteristics when de Broglie wavelength, λ, of electron becomes comparable with the depletion width, ω, of the diode. Since ๐๐ ๐ √๐๐๐ ๐ฌ๐ ๐= ๐๐๐ ๐ = ๐ ๐ ๐๐ ๐ √๐ ๐๐ ๐ฌ From the condition ๐<<๐ We obtain that , ๐ ๐๐๐ ๐๐ ๐ฒ๐ป ๐ฌ๐ ๐ โช ๐๐ ๐ ๐ ๐๐ ๐๐ Here, we assumed that the mean energy of electron is E = 3kT/2 and the potential barrier at the contact is ๐๐ = Eg/2e. Substituting numerical values in the above expression we get that for proper functioning of the Schottky diode, electron concentration must be signi๏ฌcantly less than 2×1019 cm−3. Problem 3.1 Consider a gold-GaAs Schottky diode with a capacitance of 1 pF at -1 V. What is the doping density of the GaAs? Also calculate the depletion layer width at zero bias and the field at the surface of the semiconductor at -10 V. The area of the diode is 10-5 cm2. Solution The depletion layer width can be calculated from the capacitance yielding: ๐๐ ๐จ ๐๐. ๐ ๐ ๐. ๐๐๐ ๐ ๐๐๐๐ ๐ ๐๐−๐ ๐๐ = = = ๐. ๐๐๐ ๐๐ ๐ช ๐๐−๐๐ From this one can find the doping density: ๐ ๐๐ (๐๐ − ๐ฝ๐ ) ๐ ๐๐๐. ๐ ๐ ๐. ๐๐๐ ๐ ๐๐๐๐ ๐ (๐๐ + ๐) ๐ต๐ = = ๐. ๐ ๐ ๐๐−๐๐ ๐ (๐. ๐๐ ๐ ๐๐−๐ )๐ ๐ ๐๐๐ Provided one knows the built-in potential ๐ต๐ ๐. ๐๐ ๐ ๐๐๐๐ ๐๐ = ๐๐ฉ − ๐ฝ๐ ๐๐ = ๐. ๐ − ๐. ๐๐ − ๐. ๐๐๐๐ ๐๐ ๐ต๐ ๐ต๐ Which in turn depends on the doping density. Starting with fi = 0.7 one finds Nd = 1.83 x 1017 cm-3 and the corresponding built-in potential fi = 0.708. Further iteration yields the result: Nd = 1.84 x 1017 cm-3. The depletion layer width at zero bias equals: ๐ ๐๐ (๐๐ − ๐ฝ๐ ) ๐ ๐๐๐. ๐ ๐ ๐. ๐๐๐ ๐ ๐๐๐๐ ๐ (๐. ๐๐๐ − ๐) ๐๐ = √ = ๐ ๐ต๐ ๐. ๐ ๐ ๐๐−๐๐ ๐ ๐. ๐๐ ๐ ๐๐๐๐ = ๐. ๐๐๐ ๐๐ And the electric field at the surface for Va = -10 V equals: ๐บ (๐ = ๐) = ๐ ๐ต๐ ๐๐ ๐๐ ๐ (๐๐ − ๐ฝ๐ ) ๐ ๐ต๐ ๐ ๐ ๐๐. ๐ ๐ ๐. ๐ ๐ ๐๐−๐๐ ๐ ๐. ๐๐ ๐ ๐๐๐๐ √ = √ = ๐๐๐ ๐ฒ๐ฝ/๐๐ ๐๐ ๐๐. ๐ ๐ ๐. ๐๐๐ ๐ ๐๐−๐๐ Example 3.1 Consider a chrome-silicon metal-semiconductor junction with Nd = 1017 cm-3. Calculate the barrier height and the builtin potential. Repeat for a p-type semiconductor with the same doping density. Solution The barrier height equals: ๐๐ฉ = ๐ฝ๐ − ๐ = ๐. ๐ − ๐. ๐๐ = ๐. ๐๐ ๐ฝ Note that this value differs from the one listed in Table , since the work function in vacuum was used. The built-in potential equals: ๐ต๐ ๐. ๐๐ ๐ ๐๐๐๐ ๐๐ = ๐๐ฉ − ๐ฝ๐ ๐๐ = ๐. ๐๐ − ๐. ๐๐๐๐ ๐๐ = ๐. ๐ ๐ฝ ๐ต๐ ๐๐๐๐ The barrier height for the chrome/p-silicon junction equals: ๐ฌ๐ ๐๐ฉ = ๐ + − ๐ฝ๐ = ๐. ๐๐ + ๐. ๐๐ − ๐. ๐ = ๐. ๐๐ ๐ฝ ๐ And the built-in potential equals: ๐ต๐ ๐. ๐๐ ๐ ๐๐๐๐ ๐๐ = ๐๐ฉ − ๐ฝ๐ ๐๐ = ๐. ๐๐ − ๐. ๐๐๐๐ ๐๐ = ๐. ๐๐ ๐ฝ ๐ต๐ ๐๐๐๐ 1.2 Schottky Diode 1. Find a hight of the potential barrier for a Au-n-Ge Schottky contact at room temperature (T = 293 K) if ρ = 1ฮ cm, ψAu = 5.1 eV, and าณGe = 4.0 eV. Electron mobility in Ge is 3900 cm2 V−1 s−1, density of the states in the conduction band is Nc = 1.98 × 1015 × T3/2 cm−3. Solution: (2.1) eVd = 0.88 eV. 2. Calculate the depletion width for a Pt-n-Si Schottky diode (T = 300 K) at V = 0, +0.4, and −2 V. Concentration of doping impurity in Si equals 4 × 1016 cm−3. Work function of Pt is 5.65 eV, electron affinity of Si is 4.05 eV, εSi = 11.9, density of the states in the conduction band is Nc = 6.2 × 1015 × T3/2 cm−3. Solution: (2.2) w = 0.22, 0.19, and 0.34 μm for V = 0, +0.4, and −2 V, respectively. 3. For a Schottky contact Au-GaAs calculate the maximum electric field within the space charge region at V = 0, +0.3, and −100 V. Nd = 1016 cm−3, χGaAs = 4.07 eV, εGaAs = 12.9. Work function of Au is 5.1 eV, T = 300 K, density of the states in the Conduction band is Nc = 8.63 × 1013 × T3/2 cm−3. Solution: (2.3) E = 5.1 × 104, 4.2 × 104, and 5.1 × 105 V/cm for V = 0, +0.3, and − 100 V, respectively. 4. What is the electric field E for a Schottky diode Au-n-Si at V = −5 V at the distance of 1.2 μm from the interface at room temperature if ρ = 10 ฮcm, μn = 1400 cm2 V−1 s−1, Nc = 6.2 × 1015 × T3/2 cm−3. Solution: (2.4) E = 2 × 104 V/cm. 5. Find current densities j at room temperature for a Schottky diode Pt-n-GaAs at V = +0.5 and −5 V if ρ = 50 ฮcm. μn = 8800 cm2 V−1 s−1, mn/m0 = 0.063, work function of Pt is 5.65 eV, χGaAs = 4.07 eV, Nc = 8.63 × 1013 × T3/2 cm−3. Apply thermionicemission theory. Solution: (2.5) From n = 1/eρμn we obtain that n = 1.4 × 1013 cm−3. Thus, ๐ต ๐๐๐ = ๐๐๐ − ๐๐ฎ๐จ ๐จ๐ − ๐ฒ๐ป ๐๐ ๐⁄๐ = ๐. ๐๐ ๐๐ฝ The average thermal velocity is ๐ ⁄ ๐๐ป = (๐๐ฒ๐ป⁄๐ ๐๐ ) ๐ = ๐. ๐ ๐ ๐๐๐ ๐๐⁄๐ From here we get ๐ ๐ ๐๐ ⁄๐ฒ๐ป) = ๐ ๐ ๐๐๐๐ ๐จ⁄ ๐ ๐ฑ๐ = ๐ ๐ ๐๐ป ๐๐๐ (– ๐๐ ๐ Finally, from ๐ฑ = ๐ฑ๐ (๐๐๐ (๐ ๐ฝ⁄๐ฒ๐ป) − ๐) we obtain j(0.5V) = 1.5 × 10−13 A/cm2 and j(−5V) = js. 6. The capacitance of a Au-n-GaAs Schottky diode is given by the relation 1/C2 = 1.57 × 1015 − 2.12 × 1015 V, where C is expressed in F and V is in Volts. Taking the diode area to be 0.1 cm2, calculate the barrier height and the dopant concentration. Solution: (2.6) 7. From comparison of the de Broglie wavelength of electron with the depletion width of a contact metal-n-Si, estimate the electron concentration at which Schottky diode loses its rectifying characteristics. For the estimate, assume that the height of the potential barrier a the contact is half the value of the band gap at room temperature (Eg = 1.12 eV), m*e = m0, T = 300 K, and εSi = 11.9. Solution: (2.7) ๐๐ = 0.74 V, n = 2.8 × 1017 cm−3. Part (17) Solved PROBLEMS solar cell Example 4.6 A 1 cm2 silicon solar cell has a saturation current of 10-12 A and is illuminated with sunlight yielding a short-circuit photocurrent of 25 mA. Calculate the solar cell efficiency and fill factor. Solution The maximum power is generated for: ๐ฝ๐ ๐ฝ๐ ๐ ๐ ๐ฝ๐ ⁄๐ฝ ⁄ ๐ = ๐ = ๐ฐ๐ (๐ − ๐) − ๐ฐ๐๐ + ๐ฐ๐ ๐ ๐ฝ๐ ๐ ๐ฝ๐ ๐ฝ๐ป where the voltage, Vm, is the voltage corresponding to the maximum power point. This voltage is obtained by solving the following transcendental equation: ๐ฐ ๐ + ๐๐⁄๐ฐ ๐ ๐ฝ๐ = ๐ฝ๐ ๐๐ ๐ฝ ๐ + ๐⁄๐ฝ ๐ Using iteration and a starting value of 0.5 V one obtains the following successive values for Vm: Vm = 0.5, 0.542, 0.540 V and the efficiency equals: ๐ฝ๐ ๐ฐ๐ ๐. ๐๐ ๐ ๐. ๐๐๐ ๐= [ ]= = ๐๐% ๐ท๐๐ ๐. ๐ The current, Im, corresponding to the voltage, Vm, was calculated using equation (4.6.1) and the power of the sun was assumed 100 mW/cm2. The fill factor equals: ๐ฝ๐ ๐ฐ๐ ๐. ๐๐ ๐ ๐. ๐๐๐ ๐๐๐๐ ๐๐๐๐๐๐ = = = ๐๐% ๐ฝ๐๐ ๐ฐ๐๐ ๐. ๐๐ ๐ ๐. ๐๐๐ where the open circuit voltage is calculated using equation (4.6.1) and I = 0. The short circuit current equals the photocurrent